Upload
others
View
13
Download
0
Embed Size (px)
Citation preview
Faculté de génie
Département de génie civil
PUNCHING SHEAR BEHAVIOR OF GFRP-RC EDGE
SLAB COLUMN CONNECTIONS WITH AND WITHOUT
SHEAR STIRRUPS REINFORCEMENT
COMPORTEMENT AU POINCONNEMENT DE JONCTIONS DALLE-POTEAU
DE RIVE EN BETON ARME DE PRFV AVEC OU SANS ÉTRIERS ARMATURES
DE CISAILLEMENT
Thèse de doctorat
Spécialité: génie civil
Ahmed El-Sayed Salem Ahmed SALAMA
(Ahmed Salama)
A dissertation submitted in partial fulfillment
of the requirements for the degree of
Doctor of Philosophy
(Civil Engineering)
MEMBRES DU JURY : Prof. Mathieu ROBERT (Président du jury)
Prof. Brahim BENMOKRANE (Directeur de recherche)
Prof. Adel EL-SAFTY (Examinateur)
Prof. PV VIJAY (Examinateur)
Prof. Nathalie ROY (Examinateur)
Sherbrooke (Québec) Canada
October 2019
© Copyright 2019 by Ahmed Salama
DEDICATION
I dedicate this dissertation to my mom, she was my greatest teacher, a
teacher of compassion, love and fearlessness. If love is sweet as a flower,
then my mother is that sweet flower of love. I got to grow up with a mother
who taught me to believe in myself, even when nobody else does.
i
ABSTRACT
Flat plates are commonly used in parking garages due to their functional and economic
advantages. Slabs in parking garages are susceptible to accelerated deterioration due to harsh
environment exposure as diffusion of de-icing salts, which, in turn, causing steel-corrosion
problems. The use of Glass Fiber-Reinforced Polymers (GFRP) bars has yielded a great interest
as an innovative solution to overcome such problems. However, flat plate structural system is
vulnerable to a type of brittle failure known as a punching-shear failure. This failure exaggerated
more in the case of edge slab connections due to the lack of symmetry of the portion of the slab
resisting the punching action and relatively large unbalanced moments to be transferred between
the slab and column may produce significant shear stresses that increase the likelihood of brittle
failure. Experimental and analytical investigations are carried out to examine the punching-
shear strength and behavior of reinforced concrete (RC) edge slab-column connections totally
reinforced in flexure with GFRP bars. The experimental work included edge slab-column
connections without and with GFRP stirrups as shear reinforcement. Nine full-scale
connections—one reinforced with steel bars for comparison, five reinforced solely with GFRP
bars in flexural, and three reinforced with GFRP bars and stirrups—were constructed and tested
to failure under combined vertical shear force and unbalanced moment. All slabs had identical
geometries of 2500×1350×200 mm with a 300-mm square column stub protruding 700 mm
above and below the slab surfaces. The investigated parameters are: (1) GFRP stirrups type
(closed and spiral); (2) stirrups extension (1.75d and 4.25d); (3) flexural reinforcement ratio
(1.04% and 1.55%) and type (steel and GFRP); (4) concrete strength (normal and high-strength
concretes); and (5) moment-to-shear (M/V) ratios (0.3 m and 0.6 m). The analytical investigation
is conducted through two phases. Phase I, focused on design codes assessment and proposing
simplified design approaches for connections without and with shear reinforcement,
respectively. Assessment of the available punching-shear equations provided by FRP design
provisions , ACI 440.1R-15; CSA S806-12; and JSCE-97, is conducted by comparing their
predictions against the experimental results for the tested connections and other specimens in
the literature. Phase II focused on a 3D non-linear finite element analysis (FEA) using ANSYS
software to simulate the behavior of the tested connections with shear reinforcement. Then, a
comprehensive parametric study was performed to investigate the key parameters influencing
ii Abstract
the shear capacity of such connections. The test results revealed that the final mode of
connections without shear reinforcement was punching shear failure with no signs of concrete
crushing. However, existence of GFRP stirrups shear reinforcement was shown to be essential
for significant warning before failure. GFRP stirrups shear reinforcement extended to 4.25d
yielded a significant effect in enhancing the shear strength, deformation capacity and leading to
mixed flexure/punching shear failure with considerable deformability. High-strength concrete
directly enhanced punching-shear capacity, load-deflection response, initial stiffness as well as
evidenced fewer and narrower cracks compared to their counterparts constructed with normal-
strength concrete. Meanwhile, increasing the M/V ratio for normal and high strength concrete
connections evidenced significant punching shear stresses causing reduction in the strength and
limits the deformation capacity with subsequent brittle punching shear failure. On the other
hand, the numerical results from the FEAs simulation adequately predicted the experimental
responses for the tested GFRP edge connections with and without shear reinforcement and
confirm the accuracy of the finite element model. Based on the results, a simplified design
approache is proposed to estimate the punching capacity for GFRP-reinforced edge connections
with shear stirrups. The model yielded good yet conservative predictions with respect to the
experimental results as well as the available results in the literature. The recommendations
presented herein may support the work of the North American technical committees engaged in
the development of standards and design provisions for GFRP-RC slab-column connections
columns subjected to combined vertical load and unbalanced moment.
keywords: Edge slab-column connections, Punching shear, unbalanced moment, GFRP bars,
stirrups, shear reinforcement, high strength concrete, FEM, design codes, shear strength.
iii
RÉSUMÉ
Les planchers-dalles ou dalles pleines sur poteaux sont couramment utilisés dans les
stationnements en raison de leurs avantages fonctionnels et économiques. Les dalles de
stationnements sont exposées à la dégradation accélérée due à l'exposition aux environnements
rigoureux, comme la diffusion de sels de déverglaçage qui provoque des problèmes de corrosion
de l'acier. L'utilisation de barres en polymère renforcé de fibres de verre (PRFV) a suscité un
grand intérêt en tant que solution innovante pour résoudre de tels problèmes. Cependant, le
système planchers-dalles est vulnérable à un type de rupture fragile appelée rupture par
poinçonnement. Cette défaillance est encore plus amplifiée dans le cas des jonctions dalle-
poteau de rive en raison de l’absence de symétrie de la partie de la dalle résistant au
poinçonnement et des moments de transfert ou moments non équilibrés relativement importants
à transférer entre la dalle et le poteau, pouvant produire des contraintes de cisaillement
importantes, augmentant ainsi la probabilité de rupture fragile. Des études expérimentales et
analytiques sont effectuées pour examiner la résistance au poinçonnement et le comportement
des jonctions dalle-poteau de rive en béton armé, totalement renforcés en flexion avec des barres
d’armature en PRFV. Le travail expérimental comprend des jonctions dalle-poteau de rive sans
et avec des étriers en PRFV comme armature de cisaillement. Neuf (9) jonctions pleine grandeur
(une jonction avec des barres d’armature en acier à des fins de comparaison, cinq jonctions avec
uniquement des barres d’armature en flexion en PRFV et trois jonctions avec des barres et des
étriers en PRFV) ont été fabriquées et testées jusqu'à la rupture sous une combinaison d’effort
de cisaillement vertical et d’un moment non équilibré. Toutes les dalles avaient une géométrie
identique de 2500 × 1350 × 200 mm avec un poteau de section carré de 300 mm de côté et ayant
une saillie de 700 mm au-dessus et au-dessous des surfaces de la dalle. Les paramètres étudiés
sont les suivants : (1) le type d'étrier en PRFV (fermé et en spirale) (2) – la longueur de
prolongement des étriers (1,75d et 4,25d) (3) le taux d’armature en flexion (1,04 % et 1,55 %)
et leur type (acier et PRFV) (4) la résistance en compression du béton (béton de résistance
normale et béton à haute résistance) ; et (5) les rapports moment/cisaillement (M/V) (0,3 m et
0,6 m). L'étude analytique a été réalisée en deux phases. La phase I comportait l’évaluation des
codes de conception et la proposition de méthodes de calcul simplifiées pour les jonctions sans
iv Résumé
et avec armatures de cisaillement. L'évaluation des équations de poinçonnement disponibles
dans les dispositions de conception à l’aide des PRF, ACI 440.1R-15; CSA S806-12; and JSCE-
97, est effectuée en comparant leurs prévisions aux résultats expérimentaux des jonctions testées
et d’autres spécimens dans la littérature. La phase II s'est concentrée sur une analyse 3D non
linéaire par éléments finis (FEA) à l’aide du logiciel ANSYS pour simuler le comportement des
jonctions testées. Ensuite, une étude paramétrique complète a été réalisée pour étudier les
paramètres clés influençant la résistance au cisaillement de telles jonctions. Les résultats des
essais ont montré que le dernier mode de jonction avec et sans armatures de cisaillement était la
rupture par poinçonnement sans aucun signe d’écrasement du béton ou de rupture par glissement
des barres d’armature. Cependant, la présence d’armatures de cisaillement constituées d’étriers
en PRFV s'est avérée être un signe avant-coureur d’une rupture. Les armatures de cisaillement
constituées d’étriers en PRFV prolongés de 4,25d ont eu un effet significatif sur l'amélioration
de la résistance au cisaillement, sur la capacité de déformation et ont conduit à un mode de
rupture par poinçonnement adouci, avec une déformabilité considérable. Le béton à haute
résistance a directement contribué à améliorer la résistance au poinçonnement, la réponse
charge-flèche, la rigidité initiale avec des fissures moins nombreuses et plus étroites par rapport
aux spécimens construits avec du béton de résistance normale. Entre-temps, l’augmentation du
rapport M/V pour les jonctions en béton normal et en béton à haute résistance s’est traduite par
des contraintes de poinçonnement importantes, entraînant une réduction de la résistance et une
limitation de la capacité de déformation, avec une rupture par poinçonnement fragile. D'autre
part, les résultats numériques de la simulation par éléments finis ont permis de prédire de
manière adéquate les réponses expérimentales pour les jonctions de rive en PRFV testées avec
et sans armatures de cisaillement et de confirmer la précision du modèle par éléments finis. Sur
la base des résultats, deux méthodes simplifiées de calcul sont proposées pour estimer la
résistance au poinçonnement des jonctions de rive avec et sans étriers de cisaillement en PRFV.
Les modèles ont montré de bonnes prédictions, mais prudentes par rapport aux résultats
expérimentaux et aux résultats disponibles dans la littérature. Les recommandations présentées
dans le présent document peuvent soutenir les travaux des comités techniques nord-américains
chargés de l’élaboration des normes et des dispositions de conception des jonctions dalle-poteau
en béton armé de PRFV soumises à une charge verticale et à un moment non équilibré.
v Résumé
Mots clés : Jonctions dalle-poteau de rive, poinçonnement, moment non équilibré, barres en
PRFV, étriers, armatures de cisaillement, béton à haute résistance, FEM, codes de conception,
résistance au cisaillement.
vi
ACKNOWLEDGEMENT
First and foremost, thanks to Almighty ALLAH to whom I attribute all my knowledge and
success in my life.
The author would like to express his gratefulness to his research director, Prof. Brahim
BENMOKRANE, for his inspiration, motivation, guidance, and constructive criticism. It is due
to his confidence in me, as well as his seemingly boundless patience that I have been able to do my
best work; for this I am truly thankful. I cannot thank you enough for the limitless meetings, late-
night conversations and technical brainstorming. This is beside the hand-by-hand work with
dedication and devotion throughout this research program. Many thanks also go to my jury Prof.
Adel EL-SAFTY, Prof. PV VIJAY, and Prof. Nathalie ROY.
The author is grateful to our group technical staff; Mr. Jérôme LACROIX and Mr. Steven
MACEACHERN for their technical assistance in the experimental program during the
laboratory work. The author also would like to thank all his colleagues in Prof. Benmokrane
research group especially Dr. Fareed ELGABBAS and Dr. Ahmed ABDELDAYEM for their
assistance and encourage.
I gratefully acknowledge scholarship granted to me by the Canada Research Chair in Advanced
Composite Materials for Civil Structures and Natural Sciences and Engineering Research
Council of Canada (NSERC-Industry Research Chair program). The author also would like
to acknowledge Pultrall Inc. (Thetford Mines, Québec) which generously provided the FRP
materials for the project.
I would like to express my deep appreciation and thanks to my father, my brothers, my sister
and my wife’s family, for their unlimited love, support, encouragement, duas, and prayers.
Finally, my words stand helpless, and cannot express my deep love and appreciation to my wife
(Eman) for her continuous encouragement, steadfast support and typing of the manuscript. I
cannot present this work without expressing my love to my little daughter (Hana) who
enlightened my life with her smile.
October 2019
Ahmed Salama
vii
TABLE OF CONTENTS
ABSTRACT i
RÉSUMÉ iii
ACKNOWLEDGEMENT vi
TABLE OF CONTENTS vii
LIST OF TABLES xi
LIST OF FIGURES xii
CHAPTER 1 INTRODUCTION 1
1.1. General Background 1
1.2. Objectives and Scope 3
1.3. Methodology 4
1.4. Organization of Dissertation 5
CHAPTER 2 LITERATURE REVIEW 7
2.1. Introduction 7
2.2. Steel RC Edge Slab Column Connections 7
2.2.1. General Background 7
2.2.2. Mode of Failures 9
2.2.3. Factors Affecting Edge Connections Behavior 12
2.2.3.1. Flexural Reinforcement Ratio 12
2.2.3.2. Shear Reinforcement 13
2.2.3.3. Moment-to-Shear Ratio (M/V) 14
2.2.3.4. Concrete Compressive Strength 15
2.3. FRP Composite Materials 16
2.3.1. FRP Constituents 17
2.3.2. Manufacturing Process 18
2.3.3. Mechanical Properties 18
2.3.3.1. Tensile Strength 18
2.3.3.2. Compression Strength 20
2.3.3.3. Flexural Strength 20
2.3.3.4. Shear Strength 21
2.3.3.5. Bent Portion Strength 21
2.4. FRP RC Edge Slab Column Connections 22
CHAPTER 3 EXPERIMENTAL PROGRAM 33
3.1 Introduction 33
3.2 Test Matrix 33
3.3 Material Properties 40
3.4 Specimens Construction 42
3.5 Design of Test Specimens
45
3.6 Test-Setup and Procedure 49
3.7 Instrumentations
3.8 53
viii Table of Contents
CHAPTER 4 ARTICLE 1: EFFECTIVENESS OF GFRP STIRRUPS AS SHEAR
REINFORCEMENT IN GFRP-RC EDGE SLAB–COLUMN CONNECTIONS
57
4.1 Introduction 59
4.2 Research Significance 61
4.3 Experimental Program 61
4.3.1 Overall Specimen Configuration and Design 61
4.3.2 Material Properties 66
4.3.3 Instrumentation 68
4.3.4 Experimental Setup 69
4.3.5 Test Procedure 70
4.4 Test Results 73
4.4.1 Overall Response and Cracking Pattern 73
4.4.2 Mode of Failure and Envelope 75
4.4.3 Vertical Load–Deflection Characteristics 76
4.4.4 Moment–Rotation Relationships 79
4.4.5 Flexural Reinforcement and Concrete Strains 79
4.4.6 Shear-Reinforcement Strains 83
4.4.7 Ultimate Strength 85
4.4.8 Deformability and Energy Absorption 85
4.5 Discussion 86
4.5.1 Influence of Stirrup Extension 86
4.5.2 Influence of GFRP Stirrup Type 87
4.6 Proposed Design Provisions and Predications 88
4.6.1 Slabs without Shear Reinforcement 88
4.6.2 Slabs with Shear Reinforcement 89
4.6.3 Ultimate-Capacity Predications 90
4.7 Conclusion 93
4.8 Acknowledgments 94
4.9 List of Symbols 95
CHAPTER 5 ARTICLE 2: BEHAVIOR OF CONCRETE EDGE COLUMN-SLAB
CONNECTIONS REINFORCED WITH GFRP BARS SUBJECTED TO
DIFFERENT MOMENT-TO-SHEAR FORCE RATIOS
97
5.1 Introduction 99
5.2 Experimental Program 101
5.2.1 Material Properties 101
5.2.2 Test Matrix and Parameters 103
5.2.3 Test Setup and Procedure 106
5.2.4 Instrumentation 108
5.3 Test Results and Observations 109
5.3.1 Cracking and Mode of Failure 109
5.3.2 Vertical Load-Deflection Behavior 111
5.3.3 Moment–Rotation Relationships 112
5.3.4 Strains in Flexural Reinforcement and Concrete 116
ix
5.4 Discussion 121
5.4.1 Influence of Reinforcement Type 121
5.4.2 Influence of Moment-to-Shear Force Ratio (M/V) 121
5.4.3 Influence of Concrete Strength 122
5.5 Punching Shear Design Equations 122
5.6 Comparison Between Predicted and Test Results 125
5.7 Summary and Conclusion 126
5.8 Acknowledgments 127
CHAPTER 6 ARTICLE 3: EFFECT OF GFRP SHEAR STIRRUPS ON THE
STRENGTH OF TWO-WAY GFRPRC EDGE SLABS: EXPERIMENTAL AND
FINITE-ELEMENT INVESTIGATIONS
128
6.1 Introduction 130
6.2 Research Significance 132
6.3 Summary of Experimental Program 133
6.3.1 Test Connections and Procedure 133
6.3.2 Material Properties 136
6.3.3 Experimental Setup and Instrumentation 137
6.4 Test Results and Discussion 139
6.4.1 General Cracking Pattern and Failure Mode 139
6.4.2 Ultimate Capacity and Load–Deflection Characteristics 140
6.4.3 Flexural Reinforcement and Concrete Strains 144
6.4.4 Shear-Reinforcement Strains 144
6.5 Finite-Element Simulations 146
6.5.1 Material Properties 146
6.5.2 Model Geometry, Loading and Boundary Conditions 149
6.5.3 Model Verification 151
6.6 Parametric Study 152
6.6.1 Effect of Stirrup Extension from the Column Face 152
6.6.2 Effect of Stirrup Diameter 154
6.6.3 Effect of Spacing Between Stirrups 155
6.7 Proposed Approach 156
6.8 Summary and Conclusions 160
6.9 Acknowledgements 161
CHAPTER 7 CONCLUSIONS AND RECOMMENDATIONS 162
7.1 Summary 162
7.2 Conclusions 162
7.2.1. GFRP– RC Edge Slab-Column Connections with GFRP Stirrups Shear
Reinforcement 162
7.2.2. GFRP–RC Edge Slab-Column Connections without Shear Reinforcement
164
7.3 Recommendations for Future Work
166
7.4 Résumé
7.5
166
7.5 Conclusions 167
x Table of Contents
7.5.1. Jonctions PRV–RC Bord Dalle-colonne avec Étriers PRV Renfort de
Cisaillement 167
7.5.2. Jonctions PRV–RC Bord Dalle-Colonne sans Armatures de Cisaillement
170
7.6 Recommandation pour des Travaux Futurs 171
BIBLIOGRAPHY 172
APPENDIX 182
xi
LIST OF TABLES
Table 3.1 – Flexural and shear reinforcement details 36
Table 3.2 – Tensile properties of the reinforcing bars and shear reinforcement 41
Table 4.1 – Details of test specimens 66
Table 4.2 – Tensile properties of the reinforcing bars and shear reinforcement 67
Table 4.3 – Summary of the test results 78
Table 4.4. Tested-to-predicted punching-shear capacity 92
Table 5.1– Tensile Properties of The Reinforcing Bars 102
Table 5.2 – Details of Test Connections 105
Table 5.3 – Summary of Test Results 115
Table 5.4 – Punching Shear Design Equations 124
Table 5.5 – Punching Shear Capacity Prediction 126
Table 6.1 – Details of test connections 134
Table 6.2 – Tensile properties of the reinforcing bars and shear reinforcement 137
Table 6.3 – Summary of the test and FEA results 142
Table 6.4 – Results of finite element parametric study 158
Table 6.5 –Tested-to-predicted punching shear capacities using the simplified proposed equation 159
xii
LIST OF FIGURES
Figure 1.1 – Punching shear failure in Ville St. Laurent parking garage (Julie et al. 2014) 2
Figure 2.1 – Flat plate structure applications (Salama 2016) 8
Figure 2.2 – Shear stress distribution due to shear and unbalanced moment: (a) Critical shear
section; (b) High M/V ratio; (c) Low M/V ratio (Sherif 1996) 10
Figure 2.3 – Punching shear failure under high M/V ratio of 800 mm: (a) Schematic detail; (b)
Photo (Sherif 1996) 11
Figure 2.4 – Punching shear failure under low M/V ratio of 350 mm: (a) Schematic detail; (b)
Photo (Sherif 1996) 11
Figure 2.5 – Shear reinforcement types: (a) Closed stirrups, (b) Shear studs, (c) Shear bands, (d)
U-shaped stirrups (e) Single leg stirrups, (f) Lattice reinforcement (Salama 2016) 13
Figure 2.6 – Pultrusion process (www.strongwell.com, 2018) 18
Figure 2.7 – Typical stress strain for steel and FRP bars (Ahmed 2009) 19
Figure 2.8 – Bends in FRP bars reinforcement (Arafa 2017) 22
Figure 2.9 – Geometry and reinforcement for edge connections (El-Gendy and El-Salakawy
2016) 25
Figure 2.10 – Deflection response of specimens (El-Gendy and El-Salakawy 2016) 26
Figure 2.11– Details of GFRP shear reinforcement (Mostafa and El-Salakawy 2018) 29
Figure 2.12 – Details of shear reinforcement (Mostafa and El-Salakawy 2018) 30
Figure 2.13 – Test setup (Mostafa and El-Salakawy 2018( 31
Figure 3.1 – Overall dimensions of test edge connections (Unit: mm) 34
Figure 3.2 – Flexural reinforcement details of specimens with shear reinforcement 37
Figure 3.3 – Arrangement of GFRP stirrups shear reinforcement 38
Figure 3.4 – Flexural reinforcement details of specimens without shear reinforcement 39
Figure 3.5 – GFRP bars and shear stirrups reinforcement 41
Figure 3.6 – Assembly of the slab and column cages to the formwork 43
Figure 3.7 – Assembly and alignment of column formwork 44
Figure 3.8 – Casting the test specimen 44
Figure 3.9 – Curing of concrete 45
Figure 3.10 – Lifting test specimen for testing 45
Figure 3.11 – Design specimen location relative to prototype structure 46
Figure 3.12 – Elevation view of test setup 51
Figure 3.13 – Plan view of test setup 51
Figure 3.14 – overview of test setup 52
Figure 3.15 – Stain gauges instrumentation for flexural reinforcement 54
Figure 3.16 – Stain gauges instrumentation for shear reinforcement 55
Figure 3.17 – String potentiometers and concrete gauges instrumentation 56
xiii
Figure 4.1– Typical slab geometry and reinforcement details: (a) Concrete dimension; (b)
Bottom mesh configuration; (c) Top mesh configuration; (d) Sec (A-A) (Note: 1
mm = 0.0394 in.)
64
Figure 4.2 – Shear stirrups configuration: (a) Closed stirrups arrangement (G-CS-1.75d); (b)
Closed stirrups arrangement (G-CS-4.25d); (c) Spiral stirrups arrangement (G-SS-
4.25d); and (d) Typical dimensions of bent bars and stirrups (Note: 1 mm = 0.0394
in.)
65
Figure 4.3 – B5 test method: (a) B5 test specimens; (b) Typical mode of failure at bend portion 68
Figure 4.4 – Instrumentation details 71
Figure 4.5 – Test setup 72
Figure 4.6 – Cracking patterns and punching-shear failure surface for the tested specimens 74
Figure 4.7 – Inclined shear cracks and failure envelope on the two parts of cut sections 75
Figure 4.8 – Vertical load–deflection relationships: (a) Perpendicular to the free edge; (b)
Parallel to the free edge; and (c) Moment–rotation relationships (Note: 1 mm =
0.0394 in.; 1 kN = 0.2248 kip; 1 kN.m = 8.86 kip.in)
80
Figure 4.9 – Vertical load–strain relationships: (a) Reinforcement strain perpendicular to the
free edge; (b) Reinforcement strain parallel to the free edge; (c) Concrete strain
(Note: 1 kN = 0.2248 kip)
81
Figure 4.10 – Distribution of flexural-reinforcement strains in both directions (Note: 1 mm =
0.0394 in.) 82
Figure 4.11 – Vertical strain distribution in vertical legs of stirrups 84
Figure 5.1– GFRP bars, connection reinforcement cage, and column-reinforcement details 103
Figure 5.2 – Connections concrete dimensions and reinforcement configuration 104
Figure 5.3 –Test setup and schematic 107
Figure 5.4 – Instrumentations (Note: All dimensions in mm) 109
Figure 5.5 – Cracking patterns and punching-shear failure surface for the tested connections 113
Figure 5.6 – Shear cracks progression along the sawed sections and the free edge 114
Figure 5.7 – Vertical load–deflection relationships 114
Figure 5.8 – Moment–rotation relationship 116
Figure 5.9 – Vertical load-strain relationships 118
Figure 5.10 – Flexural reinforcement-strain distribution in the perpendicular direction to the free
edge 119
Figure 5.11 – Flexural reinforcement-strain distribution in the parallel direction to the free edge 120
Figure 6.1– Slab geometry and concrete dimensions 134
Figure 6.2 – Typical reinforcement details and stirrup layout for slabs with and without shear
reinforcement 135
Figure 6.3 – Test setup and instrumentation 138
Figure 6.4 – Final punching-shear failure surface (in bold) on slab tension side and free edge
and saw-cut section 140
Figure 6.5 – Comparison between FEA and test results in terms of vertical-load deflection 141
Figure 6.6 – Comparison between FEA and test results in terms of vertical-load reinforcement
bars, concrete, and stirrup strains perpendicular to the free edge 143
xiv List of Figures
Figure 6.7 – Average stirrup strain in vertical legs from 0.25d to 1.25d 145
Figure 6.8 – Strain profile of the vertical legs of the stirrups for slabs with shear reinforcement 146
Figure 6.9 – Stress–strain relationships used in the FE model 148
Figure 6.10 – Load-deflection response with different shear transfer coefficients 149
Figure 6.11 – Geometry and reinforcement details of ANSYS model 150
Figure 6.12 – Mesh convergence study for G-CS-4.25d 151
Figure 6.13 – Deformed shapes of simulated connections 153
Figure 6.14 – Cracking progression at different loading levels for connection G-CS-1.75d 154
Figure 6.15 – Parametric study vertical load–deflection results 156
1
CHAPTER 1
INTRODUCTION
1.1. General Background
Reinforced concrete flat plate structures are defined as uniform thicknesses slabs supported
directly on columns without drop panels or column capitals. They are used commonly in parking
structure as main structural systems. Other applications of flat plate structures are multi-story
industrial buildings, warehouses, office buildings, public halls, and offshore structures. Flat
plate structures provide architectural flexibility, more clear space, easier formwork and shorter
construction time. In spite of their advantages, the ultimate strength of such structures is
governed by the ultimate capacity of their connections. However, their connections are
vulnerable to local brittle failure in the column periphery, known as a punching-shear failure.
Punching failure can arise in such system when the column with a surrounding portion of the
slab is pushed through the slab under the transfer of shear or combined shear and unbalanced
moments. The combination of shear and unbalanced moment is inevitable at edge and comer
column-plate connections and may occur at interior column-plate connections as the result of
unequal spans, unequal loads on adjacent panels, or as a result of lateral loads (Shahab 1997).
Unbalanced moments transferred between slabs and columns produces additional shear stresses
leads to minimizing the strength of slab-column connection and increasing the likelihood of
brittle punching failure. In addition, such failure is more critical at edge columns owing to the
presence at the free edge of a smaller resisting section combined with a large bending moment
(Dilger and shatila). To protect slab-column connections from such failures, caution is clearly
needed in shear strength calculation and attention should be given to increase the punching shear
strength (Hassan 2013).
Many parking structures in northern climates are deficient due corrosion of steel reinforcement
and delamination of the concrete at the level of the top mat of reinforcement. Some conditions,
such as, significant temperature fluctuations, use of deicing salts, and chlorides have created
harsh environment conditions and make the hazard more severe. This can lead to a premature
punching shear failure and redistribution of the forces to adjacent supports, causing additional
2 Chapter 1: Introduction
failures and possibly resulting in progressive collapse of the slab (Julie et al. 2014). There have
been several cases of progressive collapse due to punching shear failure and steel corrosion
problems include a parking garage collapse in Ville St. Laurent, Québec in 2008 (Fig 1.1), Hôtel
de Ville parking garage deterioration in Québec, Canada, in 2010 (Hassan et al. 2013), and La
Chancelière parking garage deterioration in Québec, Canada, in 2011 (Benmokrane et al. 2012).
Various solutions have been implemented to mitigate the accelerated deterioration of parking
structures resulted from corrosion problems as using galvanized-steel bars and epoxy-coated
steel bars. None of these techniques, however, has been proven to be cost-effective or a long-
term solution. On the other hand, using fiber reinforced Polymer (FRP) bars as internal
reinforcement for concrete structures in aggressive environment has emerged as an innovative
solution to eliminate corrosion problems. Glass FRP (GFRP) reinforcing bars have recently
gained wide acceptance as a viable construction material for sustainable new constructions due
to the lower costs compared to the other FRP types.
GFRP reinforcing bars advantages paved the way to successful field applications as concrete
reinforcement, especially in concrete parking structures. The implementation of GFRP bars in
parking structures ago with an extensive research project conducted at the University of
Sherbrooke. The experimental work presented in this dissertation extends that extensive
research project. The first phase of this project has been completed (Dulude et al. 2013; Hassan
et al. 2013a, b; and Hassan et al. 2014 a, b). A total of 30 GFRP-RC interior slab-column
Punching failure
(b) Catastrophic collapse of flooring slabs (a) Corrosion of steel reinforcement
Figure 1.1 – Punching shear failure in Ville St. Laurent parking garage (Julie et al. 2014)
3
connections were tested under concentric loading. This phase contributed to first field
implementation of GFRP bars in flat slab parking structures in a demonstration area of 350 m2
at Hôtel de Ville parking garage (Quebec, Canada, 2010). In addition to this achievement, it
helped in designing the world’ first flat-slab parking garage totally reinforced with GFRP bars:
La Chancelière parking garage (Québec, Canada, 2011) (Benmokrane et al. 2012).
That notwithstanding, very limited research has been conducted on edge slab-column
connections reinforced with FRP bars or grids (Zaghloul 2007, El Gendy and El-Salakawy 2016,
Mostafa and El-Salakawy 2018). There is also the potential for FRP-shear reinforcement in the
form of stirrups, shear studs, or shear bands to improve the punching-shear strength of two-way
slabs reinforced with GFRP bars (Hassan et al. 2014 a, b; El-Gendy and El-12 Salakawy 2016;
Mostafa and El-Salakawy 2018). To the authors’ knowledge, no experimental or analytical
investigations have been conducted to examine the effectiveness of GFRP-stirrup as shear
reinforcement in GFRP edge slab-column connections. In addition, no research has been
conducted to investigate the effect of different M/V ratios on GRRP-reinforced edge connections
constructed with HSC. This has been the main impetus to carry out the current study to fill the
gap of knowledge and provide information about these effects on the behavior of GFRP edge
slab column connections. Then design provisions and recommendations for engineers in
designing FRP edge slab-column connections were established.
1.2. Objectives and Scope
Experimental and analytical investigations on full-scale GFRP-RC edge slab–column
connections with and without GFRP shear stirrups reinforcement under combined vertical shear
and unbalanced moment were conducted. The punching shear strength and behavior of such
connections is the main scope of this study.
Basically, the objectives of the current study can be summarized as follows:
1. Study the effectiveness of the GFRP stirrups, considering the effects of GFRP-stirrup
type and extension within the slab in a crucifix layout around the column faces;
4 Chapter 1: Introduction
2. Investigates the punching strength of normal and high strength GFRP edge slab-column
connections tested under different M/V ratios;
3. Evaluate the accuracy of the available punching-shear equations in different FRP codes
and guides under shear force and unbalanced moment transfer;
4. Propose design provisions as an extension to CSA S806-12 and ACI 440.1R-15 to
account the contribution of FRP shear stirrups and predict the ultimate capacity of such
connections;
5. Perform a finite element parametric study using ANSYS software to expand the range of
investigated parameters affecting the punching shear strength of GFRP edge slab-
column connections with shear stirrups reinforcement ; and
6. Establish new punching-shear design equation to reasonably predict the ultimate shear
strength for edge slab column connections with shear reinforcement on the basis of the
finite element results.
1.3. Methodology
To achieve the foregoing objectives, a set of test specimens that comprised nine full scale
specimens were fabricated and tested under combined vertical shear and unbalanced moment
up to failure. The test specimens represented edge slab-column connections from a prototype of
flat-plate parking structure with 5 × 5 m2 square panels. One reinforced was reinforced with
steel bars as a control specimen, five were reinforced with GFRP bars in flexural, and the
remaining three were reinforced with GFRP bars and shear stirrups in different configurations
and reinforcement ratios according to the studied parameters. The total ultimate factored loads
on the prototype, including the slab weight, was estimated according to national building code
of Canada (NBCC 2015). The prototype is analysed using Equivalent Frame Method in CSA
A23.3-14 to determine the straining action on the selected connection. Then, the flexural design
was conducted according to the CSA A23.3-14 for steel RC connection and the CSA S806 for
GFRP RC edge connections, considering the requirement for structural integrity reinforcement
in CSA A23.3-14. Given the absence of shear reinforcement provisions in the CSA S806-12;
however, similar philosophies that are being used in the companion code, CSA A23.3-14, were
adopted.
5
Analysis of the experimental results in terms of strength, deformability, slab–column rotation,
concrete strains, and flexural and shear-reinforcement strains facilitate a better understanding of
the behavior of GFRP edge slab–column connections with GFRP stirrups. Evaluation of the
influence of shear stirrups type and extension was discussed. The experimental results were also
analyzed, identifying the effect of different moment -to-shear ratios on the behavior of normal
and high strength edge connections without shear reinforcement in terms of crack pattern, failure
mode, deformability, cumulative energy absorption, ultimate strength. Documentation of the
strain distribution in flexural reinforcement bars was also presented.
The experimental measurements captured the strain distribution in shear stirrups along
perpendicular and parallel directions to the free edge of the slab to assist in a reasonable
estimation of their contribution to punching shear capacity. As a result, a new design provisions
as an extension to CSA S806-12 and ACI 44.1R-15 equations was proposed to account the
contribution of FRP shear stirrups and predict the ultimate capacity of such connections.
Evaluation of the ultimate capacity of tested edge connections without shear reinforcement
according to the ACI 44.1R-15, CSA S806-12 codes and JSCE-97 punching shear equations
was also introduced. Finally, Three-dimensional non-linear finite element analysis (FEA) is
used to simulate tested edge slab-column connections with shear stirrups reinforcement using
ANSYS software. The results from the finite element analysis validated against the experimental
results to confirm the accuracy of the finite element model. Then, a comprehensive finite
element parametric study is presented to expand the range of investigated parameters
influencing the shear capacity of such connections. Based on the results, a simplified design
approach is proposed to estimate the punching capacity for FRP-RC edge connections with shear
reinforcement.
1.4. Organization of Dissertation
The dissertation consists of seven chapters. The contents of each chapter can be summarized as
follows:
6 Chapter 1: Introduction
Chapter 1 of this dissertation presents background information on the research topic, the work
objectives and the adopted methodology.
Chapter 2 introduces a literature review reporting the pertinent studies on FRP-RC edge slab
column connections to this work in a chronological order. Some aspects such as failure modes
and the most decisive parameters that affect the FRP slab-column connections’ behavior are
presented.
Chapter 3 gives the details of the experimental program and the testing procedure. The
geometry and reinforcement details of the test specimens, shear reinforcement configuration,
test setup and procedure, and the instrumentation details are presented.
The subsequent three chapters respectively correspond to three technical papers have submitted
for publication in scientific journals:
Chapter 4: (Article 1) Salama, A. E., Hassan, M., and Benmokrane, B., 2018 (Published)
“Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP-RC Edge
Slab–Column Connections,” ACI Structural Journal, V. 116, No. 5.
Chapter 5: (Article 2) Salama, A. E., Hassan, M., and Benmokrane, B., 2019 (Reviewed)
“Behavior of Concrete Edge Column-Slab- Connections Reinforced with GFRP
Bars Subjected to Different Moment-to-Shear Force Ratios,” Journal of
Composites for Construction, ASCE.
Chapter 6: (Article 3) Salama, A. E., Hassan, M., and Benmokrane, B., 2019 (Accepted)
“Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRPRC Edge Slabs:
Experimental and Finite-Element Investigations,” Journal of Structural
Engineering, ASCE.
Chapter 7 presents a general conclusion of the results obtained from the experiments and
analyses with respect to the problems and observations discussed throughout the dissertation in
addition to recommendations for future work.
1
7
CHAPTER 2
LITERATURE REVIEW
2.1. Introduction
In this chapter, a survey of relevant previous works related to this research study is presented.
A review for the behavior of steel edge slab column connections under moment and shear is
first presented. Emphasis is given on the identifications of failure modes and main factors that
affect the behavior. Afterwards, it presents a brief summary about FRP material constituents,
manufacturing, and properties as well as previous studies pertinent to the subject under
investigation.
2.2. Steel RC Edge Slab column connections
2.2.1. General Background
Reinforced concrete flat plates are commonly used as a main structural system in the buildings
of North America and Europe since the beginning of the 20th century. Compared to beam-slab
floor structure, the main advantages that can be rendered by flat slabs are reduction of floor
height, easy construction and formwork and reduction of the construction cost. Slabs without
column capitals and/or drop panels appeared in the 1950s. These slabs developed high shear
stresses near the column and thus they were considered as vulnerable to the punching shear
failure. The first flat slabs were designed by George M. Hill in 1901, however, the most famous
contributors were C.A.P. Turner (1869-1955) in USA and R. Maillart (1872-1940) in
Switzerland. Flat plate structures are employed in the construction of many multi-story
buildings; such as parking garages, offices, hotels, and apartments (Fig. 2.1)
8 Chapter 2: Literature Review
Figure 2.1 – Flat plate structure applications (Salama 2016)
In flat plate structure, relatively large shear stresses are generated around the column periphery
resulted from vertical shear forces or vertical shear forces combined with unbalanced moments
transferred between the slab, that are sufficient to cause a local brittle failure around the column,
known as a punching-shear failure. The unbalanced moment transfer occurs at edge slab column
connections subjected to gravity loads due to the discontinuity of the slab. The existence of the
unbalanced moment produces more shear stresses led to minimizing the strength and ductility
of the connection. When designing edge slab column connections, the lack of symmetry of the
portion of slab resisting this punching action and the large unbalanced moment to be resisted,
must also be considered. Therefore, edge slab column connections behavior is generally
dominated by punching shear stresses from shear and moment and its punching shear capacity
constitutes a major concern in their design. Numerous experimental and analytical
investigations have been devoted to study the behavior of edge steel RC slab-column
(a) Hotel building (b) Office building
(c) Parking structures (d) Commercial building (Dubai Tower)
9
connections under shear and moment. Based on these studies; failure modes, punching shear
behavior as well as the main parameters affecting the behavior and ultimate shear strength were
identified. These issues will be discussed in the following subsections.
2.2.2. Mode of Failures
An edge slab-column connection transferring vertical shear and unbalanced moment may fail
by flexure, punching or a combination of both modes. A slab with low flexural reinforcement
ratio will fail in a ductile manner by developing complete yield lines (Park and Gamble 1980).
If the slab shear strength is reached in a critical section, the slab will fail in diagonal tension
near the side of the column where the vertical shear stresses are the highest. This will result in
the column punching through the slab and the top flexural reinforcement splitting off the
concrete cover near the side of the column.
Figures 2.3 and 2.4 show cracking patterns on the tension sides and along the free edge of
specimens with shear reinforcement failing in punching shear under high and low eccentricities,
respectively (Sherif 1996). On the tension side, the radial and circumferential flexure cracks
appear first as the top flexural steel start to yield in the column vicinity, especially the bars
crossing the column. The diagonal shear cracks will form at about 50 to 70% of the ultimate
load, near the column side where shear stresses are maximum. The shear cracks will appear near
the inner corners of the column and then towards the free edge.
The eccentricity, M/V ratio, of the shear force from critical section centroid near the column, is
usually high edge. Thus, the shear stresses produced by the moment on the critical section near
the free edge are larger and opposite to the stresses caused by the vertical shear force (Figure
2.2a). Therefore, the net vertical shear stresses on the critical section near the free edge are in
the opposite direction to the applied vertical force. This causes the shear cracks across the free
edge will propagate from the tension sides of the slab towards the compression side (Figure 2.3).
For a critical section near the column subjected to low eccentricity, the direction of the vertical
shear stresses on the critical section near the free edge will be in the direction of applied shear
force (Figure 2.2b). Thus, the cracks across the free edge will propagate from compression side
of the slab towards the tension side of the slab (Figure 3.4). Test results demonstrated that the
formation of these inclined cracks across the free edge are usually dominant the form of final
10 Chapter 2: Literature Review
punching surface regardless the value of eccentricity. It should be noted that this crack
propagation is the same in the case of slabs without shear reinforcement.
The third mode of failure is the combination of flexure and punching; this is the case for slabs
with well anchored shear reinforcement. The main role of shear reinforcement is to control the
opening of the diagonal shear crack and consequently allow more load to be carried by the
concrete and the transverse reinforcement. Thus, more flexural steel can yield before failure and
the ductility of the connection is enhanced. The transverse reinforcement will increase the
ductility by allowing more flexural steel to yield. Punching may happen after extensive yielding
of flexural reinforcement in the column vicinity, or as a secondary phenomenon after the flexure
failure.
Figure 2.2 – Shear stress distribution due to shear and unbalanced moment: (a) Critical shear
section; (b) High M/V ratio; (c) Low M/V ratio (Sherif 1996)
B
A D
C
c2+d
Critical section
C.g of critical section
CCD cAB
c1+d/2
V
Mo
B
A D
C
(a) (b) (c)
11
Figure 2.3 – Punching shear failure under high M/V ratio of 800 mm: (a) Schematic detail; (b)
Photo (Sherif 1996)
Figure 2.4 – Punching shear failure under low M/V ratio of 350 mm: (a) Schematic detail;
(b) Photo (Sherif 1996)
Tension side
(a)
Tension side
Free edge
(b)
Tension side
(a)
Tension side
Free edge
(b)
12 Chapter 2: Literature Review
2.2.3. Factors Affecting Edge Slab Column Connections Behavior
The experimental database compiled from previous experimental and analytical researches
revealed that the punching shear behavior of edge slab column connections was governed by
many factors such as flexural reinforcement ratio, shear reinforcement, M/V, and concrete
strength. Summary about the effect of each parameter is briefly presented in the following
subsections.
2.2.3.1. Flexural Reinforcement Ratio
There is an agreement that flexural reinforcement ratio is one of the most crucial parameters
that affects the punching shear strength, ductility and mode of failure of slab column
connections. Marzouk et al 1992 studied experimentally the effect of flexural reinforcement
ratio (ranging between 0.6 to 2.4%) on punching shear capacity for high strength interior slabs
with thickness ranging from 120 and 150 mm. They concluded the punching shear capacity
increased by 63 % for slabs with 150 mm thickness when the reinforcement ratio was increased
by threefold while, increased by 78% with an increase in reinforcement ratio from 0.9 to 2.3%
for the slabs with 120-mm thickness. (Stein et al.2007) studied experimentally the effect of the
flexural reinforcement ratio and Concluded that increasing the flexural reinforcement ratio
controls flexural cracks so, the mode of failure changes from ductile flexural mode to brittle
punching shear failure. Stein et al 2007 reported that the two main modes of failure of slab
column connections are flexure and punching failures. Rizk et al 2011 tested ten full-scale
interior slab-column connections with different reinforcement ratios to examine the effect of
reinforcement ratio on punching shear capacity. Rizk et al. (2011) reported that increase of
reinforcement ratio from 0.52% to 2.17% increases maximum punching shear capacity by 40%
and punching capacity is not linearly proportional to the reinforcement ratio. The importance of
including the effect of flexural reinforcement ratio on punching shear capacity equations is well
recognized by many researchers. However, in current North American codes didn’t consider the
flexure reinforcement ratio as a variable in the design equations that predict punching shear
capacity. The best power function for the reinforcement ratio is one third power based on
extensive experimental analytical studies (Richart 1948, Regan and Bræstrup 1985; Gardner
1990; Takahashi et al. 1992; Sherif and Dilger 2000; Dilger 2000).
13
2.2.3.2. Shear Reinforcement
The use of shear reinforcement is an efficient solution that enhances both the ductility and
punching shear. There are many types of shear reinforcement as closed stirrups, shear studs,
shear bands, U-shaped stirrups, single leg stirrups, lattice reinforcement to avoid punching shear
failure. These types have been tested seeking to evaluate their efficiency. Figure 2.5 shows the
different types of shear reinforcement. The efficiency of shear reinforcement refers to many
aspects such as the used type in addition to the ratio, distribution, spacing, anchorage which is
usually critical in thin flat plates. Previous studies concluded that shear stirrups, is not fully
effective, because it does not reach its yield strength before slab failure (Kinnunen and Nylander
(1960), Franz (1963), Wantur (1969), Carpenter, et al (1970). On the other hand, Shear Stud
provides ease in installation process around column zone; fully anchorage at top and bottom that
develop yield in studs before failure and consequently increase ultimate capacity and ductility
of the connection (Dilger et al 1978; Seible et al 1980; Dilger and Ghali 1981; Mokhtar et al
1985; Elgabry and Ghali 1987; Birkle and Dilger 2008; El Salakawy 1998; Heinzman et al
2012). Stein et al (2007) concluded that when the flexural capacity exceeds the punching shear
capacity, the ultimate capacity of the connection will increase and the failure mode changes
from brittle punching shear failure into ductile failure mode.
Figure 2.5 – Shear reinforcement types: (a) Closed stirrups; (b) Shear studs; (c) Shear bands;
(d) U-shaped stirrups; (e) Single leg stirrups; (f) Lattice reinforcement (Salama 2016)
(a) (b) (c)
(d) (e) (f)
14 Chapter 2: Literature Review
The work conducted by Mortin and Ghali (1991) is one of the early investigations that studied
effect of shear studs on the behavior of edge connections under shear and moment. Mortin and
Ghali (1991) reported tests on six edge connections loaded in shear and moment. Four of them
contained stud shear reinforcement and two had no shear reinforcement. The tests showed a
considerable improvement in shear strength and ductility when studs were provided. Increases
in strength between 43 and 64 percent were noticed. Deflections at failure for specimens with
studs were twice as much as those with no shear reinforcement. The two specimens with no
shear reinforcement failed in punching. On the other hand, all four specimens with stud
reinforcement failed in flexure. The stud reinforcement changed the failure mode from brittle
punching shear failure to the more ductile flexural failure. Besides, Elgabry (1991) studied
experimentally the effect of shear stud configuration on five full scale interior slab column
connections under gravity loads associated with unbalanced moment. They concluded that
increase in punching shear capacity up to 200% depended on shear stud configuration. El-
Salakawy et al. )2000) investigated the influence of shear stud existence on the behavior of
reinforced concrete edge slab column connections with openings in order to present and discuss
the results of large-scale tests on slabs with shear stud reinforcement and compare these test
results with those of tests on identical slabs but without shear reinforcement. The slabs had
dimensions of 1540 × 1020 ×120 mm with square exterior column stub of side length 250 mm
extending 700 mm above and below the slab. All specimens were subjected to a constant M/V
of 0.3 m. El-Salakawy et al. (2000) concluded that using shear studs increases stiffness; shear
capacity; and ductility of connections and the opening located at the side of the column affects
the behavior less than the opening located in front of the column.
2.2.3.3. Moment-to-Shear Ratio (M/V)
Previous investigations on steel RC slab column connections have confirmed that increasing the
M/V ratio decreases the ultimate capacity of the connection (Zaghlool and Rawdon de Paiva
1973; Marzouk et al. 1996, 2000; El-Salakawy et al. 1998; Ozden et al. 2006). The work
conducted by Rosenthal (1959) is one of the early investigations that studied this parameter.
Rosenthal (1959) reported the results of tests on simply supported circular reinforced concrete
slabs. Rosenthal (1959) interior slab-column connections, three of these specimens were loaded
eccentrically to produce the combined effect of shear and moment acting on the connections.
For one of the latter three specimens, which were found to have failed in punching, a clear
15
unsymmetrical crack pattern was observed, accompanied by a 15% reduction in the connection
capacity. This reduction was attributed to the effect of the moment induced in the connection by
the eccentrically applied axial load. El-Salakawy et al. (1998) studied experimentally the effect
of high M/V ratio on punching shear for eight full scale edge slab column connections reinforced
with shear studs. The shear studs were arranged in six lines around the column as shown in
Figure 2.12. El Salakawy et al. 1998 concluded that the mode of failure is changed from ductile
flexural failure to more brittle flexural failure because of higher stresses for specimens subjected
to high M/V ratio of 0.66 m, besides increase in punching shear capacity outside shear reinforced
zone. Edge slab column connections subjected to high M/V ratio the shear stresses at the free
edge reverse their direction . Consequently, the inclined cracks at the free edge propagate
approximately perpendicular to the case of low M/V ratio (El-Salakawy et al. 1998).
2.2.3.4. Concrete Compressive Strength
Very limited researches have been devoted to study the influence of high strength concrete on
the punching shear capacity of slab column connections under moment and shear. Marzouk et
al. (1992) tested seventeen interor slabs with different grades of concrete where , fifteen slabs
with high strength and two with normal strength . Based on the test results, a mechanical model
was adopted and developed for high-strength concrete slab applications. The formulation takes
into account the actual behavior of the high-strength concrete and steel. The proposed model
gives a fairly good agreement between the predicted and experimental punching loads. Marzouk
et al. (1998) tested six slabs with compressive strength varying from 35 to 75 MPa; the test
result showed 7 to 15% increase in the shear strength when the concrete compressive strength
was increased by 114%. In addition, these pervious investigations concluded that using the cubic
root of the concrete compressive strength to predict the punching resistance of the slab-column
connections generally yielded better results than the square root expression used in North
American codes.
Ozden et al (2006) carried out a comprehensive experimental program involving twenty-six
circular slab column connections, twelve six fabricated with normal strength concrete while the
others constructed with high-strength concrete. The connections were tested under concentric
and eccentric loads. The slab plates had a 1500 mm diameter circular geometry and 120 mm
16 Chapter 2: Literature Review
thickness with a concentric 200 mm square central column stub, extending above and below the
slab. The results indicate that concrete strength has a direct influence on the punching behavior
and punching capacity of concrete slabs. The initial and post cracking stiff nesses of HSC
specimens tested were higher than those of NSC specimens.CSA-A23.3-04 (CSA 2004)
expressions result in conservative punching shear capacity predictions for concentrically loaded
slabs and provide good agreement with the experimentally observed punching shear capacities
for eccentrically loaded slabs.
2.3. FRP Composite Materials
In the last decades, steel corrosion is one of the major factors that leads to the accelerated
deterioration for concrete infrastructures such as parking garages and bridges. This is typically
due to significant temperature fluctuations, deicing salts, and chlorides have created harsh
environment conditions accelerating the corrosion of steel. Solutions have been proposed to
reduce the potential for corrosion and related degradation such as using galvanized-steel bars
waterproofing membranes, epoxy-coated steel bars. None of these techniques, however, has
been proven to be cost-effective or a long-term solution. The added cost of repairing deteriorated
structures with replacement costs commonly more than twice the original cost of construction,
led to the adoption of stricter specifications in some building codes and more stringent limits of
chloride ions in construction materials. It also stimulated the recent major research efforts in
design and construction techniques to improve the durability of reinforced concrete (Arafa
2017).
The use of fiber-reinforced polymer (FRP) bars provides a suitable solution for eliminating the
potential of corrosion and the related deterioration. In addition, FRP can result in significant
benefits related to the service life and reduce maintenance costs of concrete structures. Other
advantages include high-strength and stiffness to-weight ratios, chemical attack resistance,
thermal expansion control and electromagnetic neutrality. Due to the lower costs of glass FRP
(GFRP) compared to the other FRP types, GFRP bars have been used widely in concrete bridge
decks (Nanni and Faza 2002; Benmokrane et al. 2006), bridge barriers (El-Salakawy et al. 2003;
Matta and Nanni 2009, bridge piers (De Luca et al. 2010) and recently parking garages ( Ahmed
17
et al 2017, Hassan et al. 2013 a,b). A brief summary for FRP material Constituents,
manufacturing process and properties is presented in the following subsections.
2.3.1. FRP Constituents
FRP products are composite materials consisting of reinforcing fibers impregnated with a matrix
(resin). The fibers provide the mechanical strength and stiffness to the composite, while the
resins transfer shear stresses between the fibers, protect the fibers from mechanical abrasion,
and prevent the fibers from buckling. In order to provide the reinforcing function, the fiber-
volume fraction should be more than 55 percent for FRP bars and rods and 35 percent for FRP
grids (ISIS Product Certification #1, 2006).
Fibers
The most commonly used fibers for FRPs are aramid, carbon, glass, and recently basalt fibers.
The performance of fibers is affected by their length, cross-sectional shape and chemical
composition. Since glass FRP (GFRP) is more economical than the available types (carbon and
aramid) of FRP bars, it is more attractive for the construction industry. GFRP characterized
with high strength-to-weight ratio, low cost, electromagnetic neutrality, and chemical resistance.
Nevertheless, the disadvantages are relatively low tensile modulus, sensitive to abrasion, and
relatively low fatigue resistance. Glass fibers are classified as fiber drawn from an inorganic
product of fusion that has cooled without crystallizing. The types of glass fibers commonly
used are E-glass, S-glass and C-glass. E-glass has the lowest cost among all commercially
available reinforcing fibers, which is the reason for its widespread use in the FRP industry (ISIS
2007).
Matrix (Resin)
The selection of the proper matrix (resin) significantly affects the final mechanical properties of
the FRP product. In order to exploit the full strength of the fibers, the matrix should be able to
develop a higher ultimate strain than the fibers (Phillips, 1989). There are two types of polymeric
matrices widely used for FRP composites; namely, thermosetting and thermoplastic. However,
thermosetting polymers are used more often than thermoplastic in FRP industry. They are low
18 Chapter 2: Literature Review
molecular-weight liquids with very low viscosity, and their molecules are joined together by
chemical cross-links. Hence, they form a rigid three-dimensional structure that once set, cannot
be reshaped by applying heat or pressure.
2.3.2. Manufacturing Process
There are three common manufacturing techniques for FRP materials: pultrusion, braiding, and
filament winding. Pultrusion is a common technique for manufacturing straight FRP bars. In
this technique, Continuous strands of reinforcing material are drawn from creels, through a resin
tank, where they are saturated with resin, and then through a number of wiper rings into the
mouth of a heated die as shown in Figure 2.6. Before the FRP bars are cut to the required lengths,
the bars surface must be treated in the form of spirals or with sand coating to create rough surface
that creates a strong bond with concrete (ISIS 2007).
Figure 2.6 – Pultrusion process (www.strongwell.com, 2018)
2.3.3. Mechanical Properties
2.3.3.1. Tensile Strength
When loaded in tension, FRP bars do not exhibit any plastic behavior (yielding) before rupture.
The tensile behavior of FRP bars consisting of one type of fiber material is characterized by a
19
linearly elastic stress-strain relationship until failure with a general lack of ductility, very high
tensile strength and relatively low modulus of elasticity (Figure 2.7). The tensile strength and
stiffness of an FRP bar are dependent on several factors. The most significant factors are fiber
type and fiber-volume fraction that is defined as the ratio of the volume of fiber to the overall
volume of the bar over the unit length. The rate of curing, the manufacturing process, and the
manufacturing quality control also affect the mechanical characteristics of the bar (ACI 440.1R-
15 and Wu 1990).
Figure 2.7 – Typical stress strain for steel and FRP bars (Ahmed 2009)
Unlike steel, the unit tensile strength of an FRP bar can vary with diameter. For example, GFRP
bars from three different manufacturers show tensile strength reductions of up to 40% as the
diameter increases proportionally from 0.375 to 0.875 in. (9.5 to 22.2 mm) (Faza and GangaRao
1993b). On the other hand, similar cross section changes do not seem to affect the strength of
twisted CFRP strands (Santoh 1993). The sensitivity of AFRP bars to cross section size has been
shown to vary from one commercial product to another. For example, in braided AFRP bars,
there is a less than 2% strength reduction as bars increase in diameter from 0.28 to 0.58 in. (7.3
to 14.7 mm) (Tamura 1993). The strength reduction in a unidirectionally pultruded AFRP bar
with added aramid fiber surface wraps is approximately 7% for diameters increasing from 0.12
to 0.32 in. (3 to 8 mm) (Noritake et al. 1993). The FRP bar manufacturer should be contacted
for particular strength values of differently sized FRP bars.
0
200
400
600
800
1000
1200
1400
1600
1800
0. 0.5 1.0 1.5 2.0 2.5 3.0
Carbon
Aramid FRP
Glass FRP
Steel
Strain
(%)
20 Chapter 2: Literature Review
2.3.3.2. Compression Strength
The ACI 440.1R-15 do not recommended to rely on FRP bars to resist compressive stresses,
while the CSA S806-12 neglect the compressive contribution of FRP longitudinal reinforcement
is design. Nevertheless, very limited research has been devoted to study the behavior of FRP
bars under compression load. Wu 1990 reported that tests on FRP bars with a length-diameter
ratio from 1:1 to 2:1 have shown that the compressive strength is lower than the tensile strength.
The compressive modulus of elasticity of FRP bars depends on length-to-diameter ratio; bar size
and type; and other factors, such as boundary conditions. In the reported results from
compression tests, it is generally agreed that compressive stiffness ranges from 77 to 100% of
the tensile stiffness (Bedard. 1992, Chaallal and Benmokrane 1993, Tavassoli et al. 2015), while
the compressive strength is around 50% of the tensile strength. Experimental test results (De
Luca et al. 2009; ; Issa et al. 2011, Deiveegan and Kumaran 2009) on the behavior of concrete
columns entirely reinforced with glass fiber RC polymer (GFRP) reinforcement have also
demonstrated the feasibility of such structural element.
2.3.3.3. Flexural Strength
The behavior of FRP RC sections is different compared to sections reinforced with traditional
steel reinforcement. This is due to the different mechanical behavior between the two types of
reinforcements. FRP bars exhibit linear stress-strain behavior up to failure without any yielding.
Therefore, tension failure in FRP RC section is sudden and catastrophic; hence, it should be
avoided (Jaeger et al. 1997, Theriault and Benmokrane 1998). On the other hand, compression
failure of FRP RC sections offers more favorable response, as concrete ductility is utilized in
giving ample warnings before failure (Nanni 1993).
Most of current codes and guidelines require FRP RC section to be design for compression
failure. According to ACI 440.1R-15, a large amount of FRP reinforcement to be provided in
the tension zone of flexural members in order to obtain compression failure mode which is the
most ductile failure mode, as well as, for controlling crack width and deflection. The CSA S6-
14 and CSA S806-12 , on the other hand, recommends that the moment of resistance of flexure
member cross section reinforced with FRP should be at least 50% greater than the cracking
moment, to avoid brittle failure.
21
2.3.3.4. Shear Strength
As identified by Joint ACI-ASCE Committee 445 (ACI-ASCE 1998), cracked reinforced
concrete members resist the applied shear stresses by the following five mechanisms: (1) shear
stresses in uncracked concrete; (2) aggregate interlock; (3) dowel action of the longitudinal
reinforcing bars; (4) arch action; and (5) residual tensile stresses transmitted directly across the
cracks. Aggregate interlock results from the resistance to relative slip between the two rough
interlocking surfaces of the crack, much like frictional resistance. As long as the crack is not too
wide, this action can be significant (Razaqpur et al. 2001). Dowel forces generated by
longitudinal bars crossing the crack partially resist shearing displacements along the crack.
Arching action occurs in deep members or in members having shear span-to-depth ratio less
than 2.5 (Razaqpur et al. 2004). The residual tension in cracked concrete is reported to be present
for cracks less than 0.15 mm in width (ACI-ASCE Committee 445-98).
Due to the relatively low modulus of elasticity of FRP bars, concrete members reinforced with
FRP will develop wider and deeper cracks than members reinforced with steel. Deeper cracks
decrease the contribution to shear strength from the uncracked concrete due to the lower depth
of concrete in compression. Wider cracks, in turn, decrease the contributions from aggregate
interlock and residual tensile stresses. Additionally, due to the relatively small transverse
strength of FRP bars and the relatively wider cracks, the contribution of dowel action may be
negligible. Eventually, the overall shear capacity of concrete members reinforced with FRP bars
as flexural reinforcement is lower than that of concrete members reinforced with steel bars.
2.3.3.5. Bent Portion Strength
Currently-available FRP reinforcing bars are fabricated using thermosetting resin matrices and
consequently cannot be bent on site. Bends and hooks, when required, must be produced by the
bars’ manufacturer during the fabrication process. It is possible to obtain bends and hooks in
virtually any geometry from current FRP rebar manufacturers (Figure 2.8), although minimum
bend radius is typically larger than for steel bars due to significant weakening of FRP bars
around tight corners. Typical minimum allowable bend radius for FRP bars are 3.5 to 4 times
the bars’ diameter and these bends are accompanied by up to 50 percent reduction in the tensile
strength of the bar at the bend (ISIS 2007).
22 Chapter 2: Literature Review
Many studies have reported a significant reduction in the tensile strength of bent FRP bars and
stirrups at the location of the bend. For instance, Shehata et al. (2000) reported that the bend
strength generally decreases with decreasing bend radius and can be as low as 35% of the tensile
capacity of straight portions of the bar. Other investigation conducted by Morphy et al. (1997)
on 16 specimens with different types of CFRP stirrups, it was recommended limiting the
strength of CFRP stirrups to 50% of the ultimate straight bar capacity for design. The CSA
S806-12 recommends that bend portion strength shall be taken equal to 40% of the straight
portion tensile strength while the ACI 440.1R-15 gives the following equation for bend portion
strength estimation (SI units):
𝑓𝑓𝑏 =(0.05𝑟𝑏/𝑑𝑏+0.3)𝐸𝑓𝑣
1.5≤ 𝑓𝑓𝑢 (2.1)
where ffb is the bend portion strength, rb is the bend portion’s radius, db is the bar diameter, ffu is
the ultimate tensile strength for straight portion.
2.4. FRP RC Edge Slab Column Connections
Recent years have seen a great interest in testing concrete slab-column connections reinforced
with GFRP bars. In addition, there has been a growing effort to improve design guidelines for
concrete structures reinforced with FRP, especially with respect to punching shear equations.
However, there is a need for more experimental work that systematically studies the effect of
some factors, such as the different shapes of shear reinforcement; HSC edge connections under
different M/V ratios; column aspect ratio and shear perimeter-to- slab depth ratio, openings on
the punching shear strength of FRP edge slab column connections.
Figure 2.8 – Bends in GFRP bars reinforcement (Arafa 2017)
23
Because of the elastic nature of FRP up to failure, the contribution of shear resisting mechanisms
in FRP-reinforced edge slab column connections is believed to be different from that in steel-
reinforced concrete beams. For instance, FRP reinforced concrete members typically develop
wider and deeper cracks than those in concrete members reinforced with steel. Because of such
deeper cracks, the contribution of the uncracked concrete compression zone, dowel action, and
aggregate interlock to punching shear strength is reduced. Moreover, the dowel action for FRP
bars is always less than that of steel bars because of its lower transverse strength (El-Sayed et
al. 2006).
The use FRP bars in RC slab column connections can extend the service life, reduce
maintenance cost and improve-life cycle cost efficiency. Moreover, FRP bars may also reduce
construction costs by eliminating the need for membrane and pavement items (Benmokrane et
al. 2006). The direct implementation of FRP instead of steel bars, however, is not possible due
to the differences in the mechanical and bond properties compared to steel bars. This results
development of wider and deeper cracks affected the shear strength from the uncracked concrete
compression zone below the neutral axis (N.A) depth and the contribution of aggregate interlock
to decrease which, in turn, the ultimate punching-shear capacity to decrease. A brief summary
for the implemented works, ordered chronologically, is given as following.
Zaghloul 2007 was the first who conducted a study to investigate the behavior of CFRP
reinforced edge slab column connections subjected to shear and unbalanced moment . The test
includes 10 half-scale slab-column edge connections in which three connections reinforced with
steel bars and seven reinforced with CFRP NEFMAC grids. All tested specimens were
reinforced with top and bottom meshes of CFRP grids or steel bars . It was found that increasing
the reinforcement ratio by 46% increased the ultimate capacity by 21% without an increase in
the post-cracking stiffness. Two connections were assigned to study the effect of CFRP shear
reinforcement on the punching shear behavior of such connections. A typical CFRP shear rails
consisted of four legs 90 mm apart were used. The rails were placed orthogonally parallel to the
column faces. For the interior connection, it was found that the shear reinforcement increased
the ultimate capacity by 24.6 and 30.4% when the first leg of the rail was located at a distance
of 0.5d and 0.85d from the column face, respectively. For the edge connection, the increase was
24 Chapter 2: Literature Review
only 9% with the first leg of the rail located 0.5d from the column face. Also, it was reported
that the shear reinforcement increased the deformability of the connections.
The second attempt was done by El-Gendy and El-Salakawy (2016) by investigate the behavior
of edge slab column connections reinforced internally with GFRP bars. The test connections
included two series with three connections each. The connections of Series 1 investigated the
effect of a new type of GFRP shear reinforcement on the punching shear behavior of slab-
column edge connections, while those of Series 2 investigated the effect of M/V. For Series 1,
one connection did not have shear reinforcement, while the other two connections had ribbed-
deformed GFRP shear studs with headed ends at different radial spacing (120 and 80 mm). For
Series 2, three different M/V ratios were applied to the connections (0.2, 0.4, and 0.6 m). The
typical dimensions of the slabs were 2,800 × 1,550 × 200 mm with a 300-mm square column
extending above and below the slab. Details of connections tested by El-Gendy and El-Salakawy
(2016) shown in Figure 2.9.
The results indicated that, as shown in Figure 2.10, the punching shear capacity of the specimens
decreased as the M/V ratio increased. Increasing the M/V ratio from 0.2 (SC-XX-L)to 0.4 (SC-XX-
M) and 0.6 m (SC-XX-H) decreased the punching capacity by 7 and 33%, respectively, and the
ultimate deflections by 21 and 62%, respectively. The headed ends of the shear studs provided
adequate anchorage, which allowed the studs to reach their recommended design strains with no
apparent signs of slippage. Thus, the studs were capable of controlling the propagation of diagonal
shear cracks, which increased the loading capacities of the connections. The presence of studs
spaced at 120 mm (0.75d) changed the mode of failure to a mixed flexural-punching mode, while
reducing the spacing to 80 mm (0.50d) allowed the connection to reach its full flexural capacity.
Connections RD-75-M (studs spaced at 120 mm, 0.75d) and RD-50-M (studs spaced at 80 mm,
0.50d) showed 34 and 46% higher capacity than connection RD-XX-M (without shear studs). Also,
connections RD-75-M and RD-50-M showed a considerable ample warning before failure with
ultimate deflections of 48 and 75 mm, respectively. These values are 55 and 142% higher than that
of connection RD-XX-M (38 mm), respectively.
25
Figure 2.9 – Geometry and reinforcement for edge connections (El-Gendy and El-Salakawy 2016)
232
19
2
300 1250
16
00
10
00
20
0
10
00
4-20M
10M stirrups @150 mm
GFRP No. 20
16
0
Straight bars
bars
GFRP No. 20
1550
28
00
GFRP No. 20
Bent bars
X X
Sec (X-X)
54
4
54
4
Support line
Outer critical section
80
80
240
544
54
4
Support line
Outer critical section
120
120
240
26 Chapter 2: Literature Review
Figure 2.10 – Deflection response of specimens (El-Gendy and El-Salakawy 2016)
In an attempt to quantify the effect of other types shear reinforcements, sand coated studs and
corrugated bars (refer to Fig. 2.11), as well as high strength concrete, Mostafa and El-Salakawy
(2018) conducted punching shear tests on 7 GFRP-RC edge slab-column connections with and
without shear reinforcement. The test connections were divided into two series. Series 1
included three high-strength concrete (HSC) connections, investigating the effect of the flexural
reinforcement ratio (0.90, 1.35, and 1.80%); and Series 2 included four normal-strength concrete
(NSC) connections, investigating the effect of the GFRP shear-reinforcement type (headed studs
or corrugated bars) and pattern (six or eight lines of shear reinforcement). The flexural details
are the same of the test specimens tested by El-Gendy and El-Salakawy with changing the
concrete type, types of shear reinforcements, and shear reinforcement layouts. Shear
reinforcement layout of connections tested by Mostafa and El-Salakawy (2018) shown in Figure
2.12.
As shown in Figure 2.13, all the connections were tested in an upside-down position, in
comparison with the position of a real structure, with the vertical column load applied
downward; consequently, tension cracks appeared on the bottom surface of the slab. Stiff steel
I-beams were used to simply support the connections at three edges through the 20-mm-wide
steel bearing plates, and the fourth edge was left free. Neoprene strips were placed between the
slab and the bearing plates to allow a uniform load distribution along the supported edges. Three
(a) Effect of using GFRP shear studs (b) Effect of M/V ratio
27
heavy steel angles were placed on top of each supported edge of the slab to prevent any slab
movement. C-clamps were used to tighten the steel angles to the supporting I-beams, while the
two corners of the slab were kept free to lift. A hydraulic actuator and two hydraulic jacks, all
attached to a rigid steel frame, were used to apply the vertical shear force and the lateral forces
causing the unbalanced moment, respectively. The actuator and one hydraulic jack were placed
at the tip of the upper column, and the other hydraulic jack was placed at the tip of the lower
column. To maintain a M/V ratio of 0.4 m during the test, the loads were applied simultaneously
in a monotonic mode with small increments (10 and 2.3 kN for the vertical and horizontal loads,
respectively). The loading was paused every 20 kN to mark the propagation of cracks.
The main findings of this investigation can be summarized as follows:
• The HSC connections without shear reinforcement failed in a brittle punching shear
mode characterized by a sudden drop in the load accompanied by column penetration
through the slab.
• The flexural reinforcement ratio had a considerable effect on the punching shear capacity
and the post-cracking stiffness of the HSC connections. Increasing the flexural
reinforcement ratio by 50 and 100% increased the punching shear capacity by 7 and 15%
and the post-cracking stiffness by 65 and 129%, respectively. This increase in the post-
cracking stiffness resulted in a decrease in the deflection at service by 35 and 67%,
respectively.
• The use of HSC enhanced the uncracked stiffness and the punching shear capacity of the
connections and decreased the deflection at service. Doubling the concrete compressive
strength from 40 to 80 MPa resulted in 83 and 10% increases in the uncracked stiffness
and the punching shear capacity.
• With the use of eight lines of shear reinforcement, both the GFRP headed studs and
corrugated bars managed to control the propagation of shear cracks and prevented the
brittle punching shear failure in the column vicinity. However, in reducing the shear
reinforcement ratio by the use of six lines of shear reinforcement, only the headed studs
were able to fully control the shear cracks and to prevent the brittle punching shear
failure. A minimum shear reinforcement ratio of 0.4% is recommended to ensure
28 Chapter 2: Literature Review
flexural failure. Further investigation is required to examine the efficiency of corrugated
bars with larger bar diameters.
• The use of shear reinforcement enhanced the deformability and the punching capacity
of the connections. The connections N-0.9-S8, N-0.9-C8, N-0.9-S6, and N-0.9-C6 had
60, 41, 68, and 15% higher deformability; 66, 75, 62, and 17% higher deflection at
failure; and 26, 23, 27, and 8% higher capacity, respectively, than the counterpart
connection N-0.9-XX* without shear reinforcement.
29
Figure 2.11– Details of GFRP shear reinforcement (Mostafa and El-Salakawy 2018)
(b) Corrugated bars
(a) Headed bars
(c) Connections N-0.9-S8 and N-0.9-C8
(d)
30 Chapter 2: Literature Review
(a) Connection N-0.9-S8 (b) Connection N-0.9-C8
(c) Connection N-0.9-S6 (d) Connection N-0.9-C6
Figure 2.12 – Details of shear reinforcement (Mostafa and El-Salakawy 2018)
31
Figure 2.13 – Test setup (Mostafa and El-Salakawy 2018)
2.5. Summary
The available literature on steel-RC edge slab-column connections and their strength is quite
large. On the other hand, very limited research has been devoted to the problem of shear-moment
transfer at GFRP-RC edge slab-column connections. These investigations have been directed to
investigate some variables affecting the punching capacity as discussed in this chapter. The main
variables affecting the punching capacity are the M/V ratio, concrete strength, FRP flexural
reinforcement type and ratio, and shear reinforcement type. In this regard, this study aims at
Block
32 Chapter 2: Literature Review
investigating the punching-shear behavior of GFRP-RC edge slab-column connections
reinforced with and without FRP shear stirrups reinforcement, which contributes to understand
the general behavior of such connections. In addition, tests are needed to examine and modify
the current design equations in ACI 440.1R-15 and CSA S806-12 to insure safe and practical
design of such connections with FRP shear stirrups. The test parameters in the current
experimental program are described in the following chapter.
33
CHAPTER 3 EXPERIMENTAL PROGRAM
3.1. Introduction
The details of the experimental program that includes nine large-scale edge slab-column
connections are presented in this chapter. The design, construction and testing of the specimens
at the Structural Engineering Laboratory at the University of Sherbrooke are discussed in detail.
3.2. Test Matrix
Nine full-scale edge slab-column connections were fabricated and tested to failure under
combined vertical load and unbalanced moment. Of the nine specimens, one specimen was
reinforced with conventional steel bars and served as a control specimen; five were reinforced
with GFRP bars in flexural, and the remaining three were reinforced with GFRP bars and shear
stirrups. The design and details have been conducted according to according to CSA A23.3-14
and CSA S806-12 for test connections. It should be noted that since there is no design provision
for FRP shear reinforcement in the CSA S806-12, similar methodologies that are being using in
the companion code was adapted and followed. All slabs measured 2500 mm in length, 1350
mm in width, and 200 mm in thickness with a 300 mm square column stub protruding 700 mm
above and below the slab surfaces. Figure 3.1 shows the concrete dimensions of the test
specimens. The slabs’ thickness satisfied the CSA A23.3-14 Clause 13.2.3 requirement for the
minimum thickness. The test matrix was designed to investigate the influence of the following
parameters on the punching shear behavior and strength of edge slab connections:
1. GFRP stirrups type (closed and spiral);
2. Stirrups extension (1.75d and 4.25d);
3. Flexural reinforcement ratio (1.04% and 1.55%);
4. Reinforcement type (GFRP and steel);
5. Concrete strength (normal and high-strength concretes); and
34 Chapter 3: Experimental Program
6. Different M/V ratios (0.3 m and 0.6 m).
Figure 3.1 – Overall dimensions of test edge connections (Unit: mm)
The first specimen G was designed to have high flexural reinforcement ratio. The flexural
tension reinforcement in the bottom side consisted of 10 and 20 No. 20 bars in the short and
long directions. Whereas, the flexural tension reinforcement in the compression (top) side
consisted of 7 and 10 No. 15 bars in the short and long directions with at least two bars passing
through the column core to satisfy the requirement for structural integrity reinforcement in CSA
A23.3 (2014).Three specimens; G-CS-1.75d, G-CS-4.25d and G-SS-4.25d were reinforced
identically in flexure to G; however, with different types of transverse-reinforcement systems
and extension from the column faces. Figure 3.2 and Figure 3.3 show the flexural and shear
reinforcement details of the tested specimens with shear reinforcement, respectively. It should
be mentioned that these three specimens were designed to have high amounts of flexural and
transverse reinforcement such that punching-shear failure would be expected to occur prior
flexural failure. Two connections (G-CS-1.75d and G-CS-4.25d) were reinforced in shear with
No. 10 closed GFRP stirrups extended to 1.75d and 4.25d away from the column face,
respectively, where d is the slab effective depth equal to 160 mm. These connections were
designed to fail outside and within the punching-shear zone to evaluate the effect of stirrup
extension on the punching behavior and to quantify the concrete contribution (vc) outside the
250
70
0
200
Position of steel tie rods to enable
slab anchorage and setup fixing
1350
70
0
300
250
x
y
35
punching-shear zone. The third connection (G-SS-4.25d) was reinforced No.10 spiral GFRP
stirrups extended to 4.25d away from the column face to study the influence of stirrup type on
the punching strength and deformation capacity and to compare its behavior with the counterpart
slab (G-CS-4.25d) with discrete closed stirrups. The shear-reinforcement stirrups were arranged
in a cruciform pattern according to ACI 318-14 and CSA A23.3-14. The number of peripheral
lines of shear reinforcement varied between four and nine in both directions among the
specimens; the spacing between the consecutive lines was 0.5d. The first perimeter was offset
d/4 from the column face for all slabs with shear reinforcement, as specified in CSA A23.3-14.
Four other specimens, G-N-0.3, G-H-0.3, G-N-0.6, and G-H-0.6, were constructed using normal
and high strength concretes and tested under different M/V ratios ranged between 0.30 to 0.6 to
investigate the effect of different M/V ratios on the behavior. These specimens were reinforced
in flexure without shear stirrups as shown in Figure 3.4. Each specimen was reinforced in the
short and long directions, respectively, with 7 and 14 No. 20 bars as a flexural tension
reinforcement in the bottom side and 5 and 8 No. 15 bars in the compression (top) side. Two
bars in the compression side passing through the column core to satisfy the requirement for
structural integrity reinforcement in CSA A23.3-14. The steel RC edge connection (S-N-0.3)
served as a control specimen for G-N-0.3, so both had identical reinforcement configurations
and ratios. In all test specimens, the tension reinforcement (bottom) in the long direction had
double bent ends to provide the required anchorage and avoid any unexpected mode of failure,
such as slippage failure rather than punching failure. The anchorage length was equal to the
development length specified in CSA S806-12 and CSA A23.3-14 for GFRP and steel edge
connections, respectively. It should be mentioned that connection G-N-0.3 was compared to
connection G to study the effect of different flexural reinforcement on the behavior and strength.
Each slab was monolithic with square column stub, which was designed to transfer shear force
and lateral moment to the slab without any premature column failure. The nominal concrete
cover both on the top and bottom faces of the slabs was 21 mm. Table 3.1 shows the
reinforcement details of all tested specimens.
36 Chapter 3: Experimental Program
Table 3.1 – Flexural and shear reinforcement details
Test
Specimen
f’c,
(MPa)
f 't ,
(MPa)
Flexural-
Reinforcement Ratio Stirrup Layout Parameters
Bottom Top ρfv,
(%) Shape
ds,
(mm)
So;
(mm)
Sfv;
(mm) Extent
ρb, (%) ρt, (%)
G 41.4 3.6 1.55 0.65 0.90 ------ ------ ------ ---- ----
G-CS-1.75d 47.6 3.9 1.55 0.65 0.90 Closed 9.5 0.25d 0.5d 1.75d
G-CS-4.25d 51.3 3.9 1.55 0.65 0.90 Closed 9.5 0.25d 0.5d 4.25d
G-SS-4.25d 52.5 3.5 1.55 0.65 0.90 Spiral 9.5 0.25d 0.5d 4.25d
S-N-0.3 39.2 3.73 1.09 0.34 ------ ------ ------ ---- ---- ----
G-N-0.3 37.1 3.73 1.04 0.34 ------ ------ ------ ---- ---- ----
G-H-0.3 85.8 6.54 1.04 0.34 ------ ------ ------ ---- ---- ----
G-N-0.6 38.8 3.56 1.04 0.34 ------ ------ ------ ---- ---- ----
G-H-0.6 86.0 6.54 1.04 0.34 ------ ------ ------ ---- ---- ----
fcˊ= concrete compressive strength; ftˊ = concrete tensile strength; sfv = stirrup spacing; ρb = average tensile flexural
reinforcement ratio within effective widths; ρt = average compression flexural reinforcement ratio within effective
widths; ρfv = shear-reinforcement ratio at a perimeter of 0.5d from column face = (ns*Afv /Sfv bo); ds = stirrup
diameter.
37
Figure 3.2 – Flexural reinforcement details of specimens with shear reinforcement
250 7
00
Position of steel tie rods to enable
slab anchorage and setup fixing
1350
70
0
300
250
x
y
57
5
P1
57
5
P2
Vu
200
Straight bars
bars
GFRP No. 20
27
3
7@
11
4
5 @152 170
1350
25
00
11
10
GFRP No. 20
Bent bars
3@
93
269
(a) Concrete dimensions (b) Bottom mesh configuration
304 456
Straight bars
GFRP No. 15
27
3
170
1350
25
00
11
10
GFRP No. 15
Straight bars
269
34
2
45
6
3@
93
3
(c) Top mesh configuration
300 1050
16
00
700
20
0
6@
10
0
GFRP No.15
6-25M
10M stirrups
GFRP No. 20
16
0
(d) Sec (X-X) Unit: mm
A A
X X
61
61
40
40
90
90
38 Chapter 3: Experimental Program
Figure 3.3 – Arrangement of GFRP stirrups shear reinforcement
B B
4.7
5d
650 290
9@
80
40
410
GFRP closed stirrups
9@80 40
C C
4.7
5d
650 290
9@
80
40
410
GFRP spiral stirrups
GFRP spiral stirrups
9@80 40
2.2
5d
40
4@
80
A A
410 330 610
GFRP closed stirrups
4@80 40
GFRP closed stirrups
Section (A-A) Section (B-B) Section (C-C) Unit: mm
(a) G-CS-1.75d (b) G-CS-4.25d (c) G-SS-4.25d
GFRP closed stirrups
39
Figure 3.4 – Flexural reinforcement details of specimens without shear reinforcement
Y
Y
Straight bars
bars
GFRP No. 20
27
3
5@
17
5
4@218 170
1350
25
00
11
88
GFRP No. 20
Bent bars
X X
12
4
Y
Y
Straight bars
bars
GFRP No. 15
27
3
35
0
2@436 170
1350 2
50
0
11
88
GFRP No. 15
Bent bars
X X
12
4
52
5
300 1050
16
00
70
0
20
0
6@
10
0
GFRP No.15
6-25M
10M stirrups
GFRP No. 20
16
0
150 1100
GFRP No.15
GFRP No. 20
20
0
Sym.
Axis
40
40
90 90 130 88 130 88
(a) Bottom mesh configuration (b) Top mesh configuration
(d) Sec. (Y-Y) Unit: mm (c) Sec. (X-X)
40 Chapter 3: Experimental Program
3.3. Material Properties
All specimens were cast using ready-mixed normal and high concrete with a targeted 28-day
concrete compressive strength of 35 MPa and 75 MPa, respectively. The slab and the bottom
and top column stubs were cast monolithically on the same day. Table 3.1 also gives the actual
concrete compressive (fcˊ) and tensile (ftˊ) strengths based on the average of at least three 100
× 200 mm cylinders for each of the compression and splitting tests on the day of testing. The
concrete compressive strength ranged from 37.1 to 52.5 MPa, whereas the tensile strength
ranged from 3.5 to 6.54 MPa. Two types of reinforcing bars were used as flexural
reinforcements; sand-coated GFRP and deformed steel bars. Sand-coated GFRP bars of Grade
II and III compliant with CSA S807-15, were used in all GFRP specimens. The GFRP bars were
manufactured by combining the pultrusion process with an in-line sand-coating process for the
bar surface. This sand coating was designed to improve bonding between the GFRP bars and
surrounding concrete. The bottom flexural reinforcement bars were bent and straight GFRP bars
No.20 (#20) in the direction perpendicular and parallel to the free edge, respectively. Straight
GFRP bars of size No.15 (#15) were used as top flexural reinforcement in both orthogonal
directions. The tensile properties of the straight and bent GFRP bars were determined from
testing five representative specimens according to ASTM D7205M (2011) and the B.5 test
method in ACI 440.3R-12, respectively. Deformed steel bars 15M and 20M (Type 44W) were
used in top and bottom reinforcements for the reference connection. The column stub was
reinforced with steel bars of 25M and 10M as longitudinal and transverse reinforcements,
respectively. The steel-bar properties were provided by the manufacturer. Discrete No. 10 closed
and rectilinear sand-coated spiral GFRP stirrups were used as shear reinforcement. The tensile
strengths of the straight and bent portions of the stirrups were determined by testing five
representative specimens according to ASTM D7205M (2011) and the B.5 test method in ACI
440.3R-12, respectively. Table 3.2 summarizes the tensile properties of the used reinforcing
bars. Figure 3.5 depicts the GFRP bars and shear-reinforcement stirrups.
41
Table 3.2 – Tensile properties of the reinforcing bars and shear reinforcement
Bar Designationa
Nominal
Cross-
Sectional
Areaa
(mm2)
Ultimate
Tensile
Strength
(MPa)
Elastic
Tensile
Modulus
(GPa)
Ultimate
Tensile Strain
(%)
GFRP straight flexural bars
No. 15 GFRP bar 199 1323 ±12 64.8±0.5 2.04 ±0.05
No. 20 GFRP bar 285 1334 ±85 64.9±0.6 2.06 ±0.13
GFRP bent flexural bars
No. 20 straight portion 285
1210±63 53±0.48 2.28±0.15
No. 20 bent portion ffvb b= 490±44 ------ ------
GFRP-stirrup shear reinforcement
No. 10 straight portion 71
967±39 45.7±0.5 2.12±0.08
No. 10 bent portion ffvb b= 489±38 ------ ------
Steel bars
10M 100 fy c= 420 200 ɛy = 0.21
20M 300 fy c= 460 200 ɛy = 0.23
25M 500 fy c= 470 204 ɛy = 0.23 a According to CSA S807 (2015). b ffvb = ultimate tensile bend strength obtained from the B.5 test method (ACI 440.3R 2012) c fy steel yielding strength and εy steel yielding strain, as provided by the manufacturer.
Figure 3.5 – GFRP bars and shear stirrups reinforcement
No.20 GFRP bent bars
No.20 GFRP s aight barstr
No.15 GFRP bars
Spiral stirrups (No.10 GFRP) Closed stirrups (No.10 GFRP)
42 Chapter 3: Experimental Program
3.4. Specimens Construction
The cages were assembled in the Structural Laboratory at the University of Sherbrooke and then
moved for casting at Les Coffrages Carmel, inc. upon completion. A wooden formwork was
manufactured by Les Coffrages Carmel, inc. from plywood plates of 19 mm thickness. The top
and bottom column stubs were fabricated in the wooden formwork 700 mm beyond the slab.
The formwork was supported on Thirteen aluminum I beams of 4 m long, 9 beams in the long
direction and 3 beams in the short direction, which were supported in turn on steel supports.
Before installing the reinforcing cages, the vertical level of the column was adjusted, and the
formwork was lubricated to provide ease in formwork removal. The construction started with
mounting the steel column cage without top column stub stirrups in the wooden formwork. Then
the instrumented slab cages were placed in the formwork and the stirrups of the top column stub
were installed (Figure 3.6) followed by the installation of the wooden formwork of the top
column stub (Figure 3.7). Two 10 mm-diameter holes were cast close to the slab edges to enable
anchorage during testing by fixing PVC pipe at those locations. Two vertical steel hooks were
placed at 450 mm from the free edge of the slab to carry the slabs after removing from the
formwork.
Batch plant delivered ready-mixed concrete and slump test was performed for each delivered
mix. The orientation of the specimens during casting was the same as during testing. The column
stub was cast simultaneously with the slab (Figure 3.8). The concrete was internally vibrated,
and the surface of the concrete slab was adjusted when casting had been completed. Nine plastic
standard cylinders of 100 x 200 mm were moulded for each delivered mix to determine concrete
compressive strength and splitting tensile strength. One day after casting, the cylinders and the
external sides of the formworks were stripped and then the slabs, column stubs and the concrete
cylinders were covered with moist burlap (Figure 3.9). After one week, the specimens were
moved out from the formwork, and transported to the Structural Laboratory at the University of
Sherbrooke for testing using 10-ton capacity crane (Figure 3.10).
43
Figure 3.6 – Assembly of the slab and column cages to the formwork
(a) S-N-0.3 (b) G-N-0.3, G-H-0.3, G-N-0.6, G-H-0.3
(c) G-CS-1.75d (d) G-CS-4.25d
44 Chapter 3: Experimental Program
Figure 3.7 – Assembly and alignment of column formwork
Figure 3.8 – Casting the test specimen
(c) Surfacing the slab surface
(b) Casting the slab
(d) Connection just after casting
(a) Casting the column stub
45
Figure 3.9 – Curing of concrete
Figure 3.10 – Lifting test specimen for testing
3.5. Design of Test Specimens
The test specimens represented edge slab-column connections from a prototype of flat plate
parking structure. The prototype consisted of four-square panels with 5 m long in both
directions. Figure 3.11 depicts the position of the test specimens relative to a prototype slab. All
slabs had identical geometries of 2500 × 1350 × 200 mm with a 300-mm square column stub
protruding 700 mm above and below the slab surfaces. The slabs were simply supported on a
2000 × 1150 mm perimeter on the bottom face of the slab. The prototype structure was analysed
using Equivalent Frame Method in CSA A23.3-14 to determine the straining action on the
selected connection and the M/V ratio (Appendix). Then, the flexural design was conducted
according to the CSA A23.3-14 for steel RC connection and the CSA S806-12 for GFRP RC
46 Chapter 3: Experimental Program
edge connections. Each specimen was simply supported on three edges, simulating lines of
contra flexure in the prototype floor, and monolithic with a column at the middle of the fourth
edge. The lines of contra flexure were assumed to be 0.2L away from the column centerlines,
where L is the span between the column centerlines. The prototype had a gravity live service
load of 2.40 kN/m2, a super-imposed dead load of 1.0 kN/m2 and a self-weight of 4.80 kN/m2,
resulting in a M/V ratio of 0.3 m.
Figure 3.11 – Design specimen location relative to prototype structure
20
0
3
2
1
A B C 5m 5m 5m
5m
5
m
5m
2.5
m
1.35 m
Design
specimen
47
The predicted shear strength for the investigated GFRP edge connections without shear
reinforcement was calculated based on the available punching-shear equations provided in CSA
S806-12, ACI 440.1R-15, and JSCE-97. These equations are forms of the original equations for
steel that have been modified to account for the difference in mechanical properties between
FRP and steel reinforcement, especially the lower modulus of elasticity.
ACI 440.1R-15
The punching-shear stress provided by concrete (vc) for two-way slabs reinforced with FRP bars
or grids is simply the ACI 318-14. Punching-shear equation for steel-reinforced slabs modified
to account for the shear transfer in two-way slabs. The vc equation for steel modified by the
factor ([5/2] k) accounts for the axial stiffness of the FRP reinforcement through the neutral-
axis-depth term (kd), as shown in Eq. (3.1).
𝑣𝑐 = 4
5 𝑘 √𝑓𝑐
′ (3.1a)
𝑘 = √2𝜌𝑓 𝑛𝑓 + (𝜌𝑓 𝑛𝑓)2 − 𝜌𝑓𝑛𝑓 (3.1b)
Where: 𝑛𝑓 =𝐸𝑓
𝐸𝐶⁄ , 𝐸𝑐 = 4700 √𝑓𝑐
′
where fc' = concrete compressive strength (MPa); bo,0.5d = perimeter of the critical section for
slabs at a distance of effective depth (d)/2 from the column face (mm); k = neutral-axis depth
to reinforcement depth ratio (mm); and ρf = average of the FRP reinforcement ratio in both
directions.
CSA S806-12
vc can be calculated as the smallest of Eq. (3.2) to (3.4), which are essentially the CSA A23.4-
14 equations with modifications to account for FRP bars instead of steel. A critical perimeter
nearest a column equal to 0.5 times the effective depth (0.5d) from the column face was taken
𝑣𝑐 = 0.028 λ ∅𝑐 (1 +2
βc) (𝐸𝑓 𝜌𝑓 𝑓𝑐
′ )13
(3.2)
𝑣𝑐 = 0.147 λ ∅𝑐 (0.19 +αs d
𝑏𝑜;0.5𝑑) (𝐸𝑓 𝜌𝑓 𝑓𝑐
′ )13
(3.3)
48 Chapter 3: Experimental Program
𝑣𝑐 = 0.056 λ ∅𝑐 (𝐸𝑓 𝜌𝑓 𝑓𝑐′ )13
(3.4)
where λ= concrete density factor (1 for normal weight and 0.85 for semi-lightweight); ∅c = concrete
resistance factor (0.65); βc = ratio of long side to short side of column; αs = 4 for interior columns, 3 for
edge columns, and 2 for corner columns; and fc' shall not exceed 60 MPa. If d exceeds 300 mm, the vc
obtained from the equations shall be multiplied by (300/d)0.25
.
JSCE-97
vc can be calculated as given in Eq. (3.5).
𝑣𝑐 = 𝛽𝑑 𝛽𝑝 𝛽𝑟 𝑓𝑝𝑐𝑑 /𝛾𝑏 (3.5a)
𝛽𝑑 = (1000/𝑑)0.25 ≤ 1.5 , (3.5b)
𝛽𝑝 = (100𝜌𝑓𝐸𝑓/𝐸𝑆)1
3 ≤ 1.5 , (3.5c)
𝛽𝑟 = 1 + 1/(1 + 0.25 𝑢𝑜/𝑑) , (3.5d)
𝑓𝑝𝑐𝑑 = 0.2√𝑓𝑐′ ≤ 1.2
(3.5e)
where uo =perimeter of reaction area of supporting column; ρf = average flexural reinforcement
ratio in both orthogonal direction; γb = partial safety factor equal to 1.3 or 1.5 for concrete
strengths below and above 50 MPa, respectively, that was set to 1.0 to get an un factored
prediction of capacity; fpcd = concrete compressive strength (MPa), and d = effective slab depth
(mm).
Due to the lack of provisions in CSA S806-12 and ACI 440.1R-15 for calculating ultimate
capacity of FRPRC two-way slabs with FRP shear reinforcement, we opted to propose design
provisions as an extension to CSA S806-12 and ACI 440.1R-15. Regarding steel-reinforced
two-way slabs with shear reinforcement, ACI 318-14 and CSA A23.3-14 require that the shear
stresses be checked either inside or outside the shear-reinforced zone. The critical shear section
inside the shear-reinforced zone is located at d/2 from the column faces, while the critical section
outside the shear reinforcement lies at d/2 from the outermost shear reinforcement. Within the
shear reinforced zone, the factored shear-stress resistance, computed as (vc + vs), where vc and
49
vs are the summations of concrete and shear-reinforcement contributions to the shear strength
inside the punching zone. Design codes, ACI 318-14 and CSA A23.3-14, calculated the concrete
contribution inside and outside the region reinforced with shear stirrups as 50% of the punching-
shear strength of slabs without shear reinforcement. Accordingly, the concrete contribution
inside and outside the shear-reinforced zone for FRP-reinforced two-way slabs is proposed to
have a value equal to 50% of the least of Eqs. (3.2) to (3.4) according to CSA S806-12 or Eq.
(3.1) according to ACI 440.1R-15.
In order to calculate the FRP-stirrup contribution, steel stirrups equation has been modified by
replacing, fy (yielding strength) with a specific stress (ffv) at a limiting strain value (εfv) of 5000
or 4000 μs according to CSA S806-12 and ACI 440.1R-15, respectively, where ffv equals εfv
multiplied by the FRP-stirrup modulus of elasticity (Efv). It should be noted that the ffv should
be less than the stress corresponding to the failure of the stirrup corners or bends as determined
with the appropriate procedure in accordance with ACI 440.1R-15 and CSA S806-12. The
proposed design equations can be summarized as follows.
Proposed design provisions for CSA S806-12 with the shear-reinforced zone
𝑣𝑐 𝑖𝑛𝑠𝑖𝑑𝑒 = 𝑣𝑐𝑜𝑢𝑡𝑠𝑖𝑑𝑒 = 0.028𝜆𝜙𝑐(𝐸𝑓𝜌𝑓𝑓𝑐′)1
3 (3.6)
𝑣𝑓𝑣 =𝜙𝑓𝐴𝑓𝑣(0.005𝐸𝑓𝑣)
𝑏0 𝑆𝑓𝑣 (3.7)
Proposed design provisions for ACI440.1R-15 with the shear-reinforced zone
𝑣𝑐 𝑖𝑛𝑠𝑖𝑑𝑒 = 𝑣𝑐 𝑜𝑢𝑡𝑠𝑖𝑑𝑒 =2
5𝑘√𝑓𝑐
′ (3.8)
𝑣𝑓𝑣 =𝜙𝑓𝐴𝑓𝑣(0.004𝐸𝑓𝑣)
𝑏0𝑆𝑓𝑣 (3.9)
3.6. Test-Setup and Procedure
The specimens were tested in the structural laboratory at the University of Sherbrooke under
monotonic vertical shear force and lateral static unbalanced moment until failure. The test setup
included three main parts: (1) the testing frame, (2) reaction frames, and (3) the supporting bed
and top restrain beams. The testing frame consisted of two main frames and a stiff connecting
steel I-beam on top. A 1500-kN vertical hydraulic jack was installed at the center of the I beam
50 Chapter 3: Experimental Program
to apply a constant vertical load at the top of the concrete column. During testing, a steel pan
with rollers was placed between a vertical jack and the top of upper concrete column to free
horizontal movement of the column during lateral loading while maintaining the vertical load.
Two 1000 kN horizontal hydraulic jacks were installed on two very rigid reaction frames fixed
firmly to the laboratory strong floor to apply lateral loads. The vertical and lateral jacks were
controlled using three manual hydraulic pumps. The loads were monitored with three load cells
on each pump and connected to the data-acquisition system.
The specimens were simply supported on the bottom surface along three sides during testing
with a new fabricated supporting steel bed, which was designed to ensure adequate strength and
stiffness under the testing load of the specimens. The supporting bed consisted of four-square
steel beams [HSS 250 × 150 × 8 mm] supported on four square columns [HSS 152 × 100 × 6
mm] laterally stiffened with back-to-back double steel angles [102 × 102 × 7.9 mm] in both
directions. It is worth mentioning that, before placing the test specimen in the setup, the
supporting bed was prestressed directly on the laboratory strong floor with four 38 mm diameter
steel tie rods to prevent the supporting bed from moving laterally. On the slab top face, three
supported edges were restrained by steel reaction beams to prevent slab lifting. Each end of the
reaction beam was held in position by four steel nuts and plates attached to the steel tie rods. In
addition, 20 mm thick neoprene pads were placed between the slab and supporting bed and
between the slab and top restrain beams along the support lines to simulate slab rotation at the
line of contra flexure and ensure uniform stress distribution along the edges. The test setup
details are depicted in Figure 3.12 to 3.14. The specimens were tested under varied unbalanced
moment (Mun) to vertical load (V) ratios between 0.3 to 0.6 m. The unbalanced moments were
calculated by multiplying the two lateral forces, applied to each column by the distance from
the application point to the center of the slab: 675 mm. The vertical load was applied
monotonically at a load-controlled rate of 5 kN/min, whereas the horizontal forces were
simultaneously applied with the vertical force in small increments to maintain a constant M/V
ratio of 0.3 or 0.6 m throughout the test until failure.
51
Supporting bed
Main steel frame
Main steel frame
Reaction frame
Roller plate Lateral hydraulic jack
Reaction frame
Steel post
Test specimen
Neoprene pads
Stiff connecting steel I-beam
Steel clamps
Test
specimen
4 Steel rods (20mm)
Main steel frame Main steel frame
Top frame
4 Steel rods (38 mm)
2 Steel plates
Stiff connecting steel I-beam
Figure 3.13 – Plan view of test setup
Figure 3.12 – Elevation view of test setup
52 Chapter 3: Experimental Program
Figure 3.14 – Overview of test setup
53
Instrumentation
Strains in the bottom flexural reinforcement (tension side) were measured with 11 electrical
resistance strain gauges [6 mm long] at different locations in both orthogonal directions (Fig.
3.15). The strain gauges were located at a distance of 0, 75, 225, 450, and 750 mm from the
column face on one bar in each direction. In addition, one electrical strain gauge was glued at
the bend location of the GFRP bar at the column location (see Fig. 3.15). The strains in the FRP
stirrups were monitored using six strain gauges mounted at mid-height of the vertical legs of the
FRP stirrups and bend location in each orthogonal direction, as shown in Figure 3.16. In
addition, five concrete electrical strain gauges —labeled C1 to C5—were glued before testing
to the slab's top surface (compression side) at 0 and 200 mm from the column face (see Fig.
3.17).
Sixteen string potentiometers (pots) were used at different locations to measure the
displacements. Eleven pots (P1 to P11) were placed on the top slab face along two orthogonal
directions at a distance of 80, 250, 550, and 850 mm from the column face to measure the slab-
deflection profile while one pot (P15) was located at the column centerline to measure the
central deflection. Two pots (P12 and P16) were installed horizontally on the top and bottom
column ends to measure column lateral displacements. To monitor any possible shifting of the
specimen or test setup, two pots (P13 and P14) were installed in the horizontal loading directions
at the center of slab thickness and frame test setup. All instruments were installed onto rigid
steel frames, separated from the testing frame and attached directly to the laboratory floor, to
prevent any frame deformations from affecting the measurements. Moreover, two linear variable
differential transformers (LVDTs) were placed throughout slab testing to monitor flexural-crack
widths in each direction. The strain gauges, pots, and LVDTs were connected to a data-
acquisition system to record the readings. Figures 3.15 to 3.17 show the position of several
instrumentation details of the test specimen. During the test, crack propagation was marked, and
the corresponding loads were recorded.
54 Chapter 3: Experimental Program
Figure 3.15 – Strain gauges instrumentation for flexural reinforcement
Strain gauges
(a) Slabs with shear reinforcement
Strain gauges
(b) Slabs without shear reinforcement
55
Figure 3.16 – Strain gauges instrumentation for shear reinforcement
B B
4.7
5d
650 290
9@
80
40
410
Strain gauges
GFRP closed stirrups
9@80 40
Strain gauges
C C
4.7
5d
650 290
9@
80
40
410
GFRP spiral stirrups
GFRP spiral stirrups
9@80 40
2.2
5d
40
4@
80
A A
410 330 610
Strain gauges
GFRP closed stirrups
4@80 40
GFRP closed stirrups
Section (A-A) Section (B-B) Section (C-C)
(a) G-CS-1.75d (b) G-CS-4.25d (c) G-SS-4.25d Unit: mm
GFRP closed stirrups
56 Chapter 3: Experimental Program
Figure 3.17 – String potentiometers and concrete gauges instrumentation
C1
P9
P12
P13
P14
P11
P1 P2 P3 P4
P8
P5
P6
Test setup sliding
Lateral top displacement
Lateral Bottom displacement
P16
P10
Vertical Pots
P7
Horizontal pots
C2
C3 C4
C5
Concrete
gauges
P15
57
CHAPTER 4
Article 1: EFFECTIVENESS OF GFRP STIRRUPS
AS SHEAR REINFORCEMENT IN GFRP-RC
EDGE SLAB–COLUMN CONNECTIONS
Foreword
Authors and Affiliation
o Ahmed E. Salama: PhD Candidate, Department of Civil Engineering, University of
Sherbrooke, Quebec, Canada J1K 2R1, E-mail: [email protected]
o Mohamed Hassan: Postdoctoral Fellow, Department of Civil Engineering, University of
Sherbrooke, Quebec, Canada J1K 2R1, E-mail: [email protected].
o Brahim Benmokrane: FACI, is professor of civil engineering and NSERC Research
Chair in FRP Reinforcement for Concrete Infrastructure. He is a member of ACI
Committee 440 FRP Reinforcement and serves as co-chair of Canadian Standard
Association (CSA) committees on FRP structural reinforcing materials for building
design code (CSA S806), and bridge design code (CSA S6).
Corresponding author, E-mail: [email protected].
Paper submitted to ACI structural journal on September 9, 2018
Paper status: Published on September 1, 2019 (DOI: 10.14359/51716757)
Reference: Salama , A. E. , Hassan , M., and Benmokrane, B., 2019, “Effectiveness of GFRP
Stirrups as Shear Reinforcement in GFRP RC Edge Slab–Column Connections,”
ACI Structural Journal, V. 116, No. 5.
58 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
Abstract
Recent years have seen a great interest in testing concrete slab-column connections reinforced
with glass-fiber-reinforced-polymer bars (GFRP-RC). Yet, current FRP codes and guidelines
have not addressed the design of slab-column connections with FRP shear reinforcement.
Results from an experimental investigation aimed at evaluating the effectiveness of glass-fiber-
reinforced-polymer (GFRP) stirrups as shear reinforcement in edge slab–column connections
reinforced with GFRP bars are presented. Four full-sized slabs with and without stirrups as shear
reinforcement were tested to failure under combined vertical load and unbalanced moment. The
effect of the GFRP-stirrup type and extension on the punching shear response of the tested slab–
column connections are analyzed and discussed. In addition, simplified design provisions to
predicate the ultimate shear capacity of the tested specimens are proposed. The test results
revealed that the presence of GFRP shear reinforcement as either closed or spiral stirrups within
the slab around the column perimeter improved the punching-shear response of the tested
connections. The results also indicated that the performance of the spiral stirrups was equivalent
to or better than that of the closed stirrups in reducing the brittleness of the tested specimens
with the same amounts of flexural and shear reinforcement. The proposed design provisions as
extensions to those in CSA S806 design code yielded good yet conservative predictions with an
average Vtest/Vpred of 1.28 ± 0.24 for test specimens with FRP shear stirrups as well as others
with different types of FRP shear reinforcement found in the literature. This represents a step
forward for engineers in designing two-way concrete slabs reinforced with FRP stirrups.
Keywords: Punching Shear, FRP, Flat Slab, Edge Slab, Parking Garages, Design Codes,
Stirrups, Shear Reinforcement, Unbalanced Moment.
59
4.1. Introduction
The construction industry has expressed great demand for innovative and durable structural
members. Glass-fiber-reinforced-polymer (GFRP) reinforcing bars have recently gained wide
acceptance as a viable construction material for sustainable new constructions. Reduced
material costs—coupled with labor savings inherent with its light weight and comparatively
simple installation, its high tensile strength, and immunity to corrosion and chemical attack—
have made GFRP reinforcing bars an attractive alternative to steel reinforcement in concrete
members subjected to severe environmental conditions. Code writing bodies in the USA and
Canada have tasked several technical committees to produce standards and guidelines for
elements reinforced with GFRP, including AASHTO (2009), ACI 440-1R (2015), CSA S806
(2012), and CSA S6 (2014). Field applications over the last years have shown excellent
performance and durability of GFRP-reinforced structures (Benmokrane et al. 2007; Ahmed et
al. 2014, etc.). Only limited work, however, has been conducted on implementing GFRP
reinforcement in two-way concrete flat-slab parking structures (Ahmed et al. 2017).
Reinforced-concrete (RC) two-way flat-slab systems are very popular in construction because
of their functional and economic advantages. Yet this type of structural system is not very
efficient in terms of energy dissipation and is vulnerable to a type of brittle failure known as a
punching-shear failure. When designing edge slab–column connections, the lack of symmetry
of the portion of the slab resisting the punching action and relatively large unbalanced moments
to be transferred between the slab and column may produce significant shear stresses that
increase the likelihood of brittle failure, which must be considered. The avoidance of such a
failure is of paramount importance. Various solutions have been used in the past to mitigate
punching-shear failure at a slab–column connection. This can be achieved by simply (1)
increasing the slab thickness by providing a drop panel or capital or increasing the column
dimensions; (2) using higher-strength concrete; or (3) providing additional shear strength
through shear reinforcement in the form of stirrups, shear studs, shear heads, or shear bands
within the slab around the column perimeter. The latter solution is more effective and practical
than the other two methods in increasing the punching-shear strength and deformation capacity
of slab–column connections (Megally and Ghali 2000), which is one of the primary motivations
of this research.
60 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
Despite the increasing demand to use GFRP reinforcing bars in two-way flat slabs (Dulude et
al. 2013; Hassan et al. 2013 a, b; Gouda and El-Salakawy 2015; Hassan et al. 2017), very limited
research has been conduced on FRP edge slab–column connections (Zaghloul 2007; El-Gendy
and El-Salakawy 2016, 2018; Mostafa and El-Salakawy 2018). Most of the existing studies have
been focused on the behavior of two-way slabs reinforced solely with GFRP bars as flexural
reinforcement. There is also the potential for FRP-shear reinforcement in the form of stirrups,
shear studs, or corrugated GFRP bars to improve the punching-shear strength of two-way slabs
reinforced with GFRP bars (Hassan et al. 2014 a, b; El-Gendy and El-Salakawy 2016; Mostafa
and El-Salakawy 2018).
New types of FRP shear reinforcement for slabs have been tested at the University of
Sherbrooke (Hassan et al. 2014 a, b): sand-coated carbon- and glass-FRP shear reinforcement
in the form of discrete closed and spiral stirrups. The stirrup shear reinforcement proved quite
effective in tests on GFRPRC interior connections. The use of FRP stirrups significantly
increased the punching-shear strength and deformation capacity on average by 27% and 107%,
respectively, particularly when the flexural reinforcement ratio was high. El-Gendy and El-
Salakawy (2016) tested two GFRP edge connections with another type of FRP shear
reinforcement, headed studs, which consisted of ribbed GFRP bars with double heads. The studs
were placed in an orthogonal layout with 0.5d and 0.75d spacing between the rows of studs.
Decreasing the spacing of the shear studs from 0.75d to 0.5d increased the punching-shear
strength by 34% and 46%, respectively, and the maximum deflections by 55% and 142%,
respectively, compared to connections without shear reinforcement. Mostafa and El-Salakawy
(2018) examined two types of GFRP shear reinforcement, specifically, sand-coated double-
headed GFRP studs and corrugated GFRP bars in tests on edge slab–column connections
reinforced with GFRP bars. The test results indicate that both types of shear reinforcement can
be highly satisfactory in preventing brittle punching-shear failure in the column vicinity. The
average increases in the ultimate shear strength were 27% and 16% and the deformation capacity
were 64% and 46% for the shear studs and corrugated GFRP bars, compared to their
counterparts without shear reinforcement, respectively.
Based on these earlier studies, FRP shear reinforcement has demonstrated its ability to develop
substantial increases in punching-shear and deformation capacities, making it an attractive
61
alternative to traditional methods, such as drop panels and column capitals, for the construction
of two-way GFRPRC slabs, especially when there are constraints on slab thickness. It is worth
mentioning that the current North American codes for FRP—ACI 440.1R (2015) and CSA S806
(2012)—do not have provisions for designing GFRP-reinforced connections with FRP shear
reinforcement. This is mainly due to a lack of experimental research, particularly on edge
connections. Given the increase use of FRP as flexural and transverse shear reinforcement in
different structural elements such as beams, beam–column joints, and piles, similar code
provisions are urgently needed for two-way flat-slab structures reinforced with FRP flexural and
shear reinforcement.
This paper presents experimental tests on GFRP edge slab–column connections with the aim of
investigating the influence of GFRP-stirrup type (closed and spiral) and extension inside the
slab around the column perimeter on the punching-shear strength and failure within or outside
the shear-reinforced zone. Detailed measurements on deflections, slab–column rotation,
concrete strains, and flexural- and shear-reinforcement strains facilitate a better understanding
of the behavior of GFRP edge slab–column connections with GFRP stirrups.
4.2. Research Significance
The purpose was to assess the effectiveness of the GFRP stirrups, considering the effects of
GFRP-stirrup type and extension within the slab in a crucifix layout around the column faces.
The paper also establishes design provisions and recommendations for engineers in designing
two-way flat slabs with GFRP stirrups as shear reinforcement. The recommendations herein
may support the work of the North American technical committees engaged in the development
of standards and design provisions for GFRP-RC slab-column connections columns subjected
to combined vertical load and unbalanced moment.
4.3. Experimental Program
4.3.1. Overall Specimen Configuration and Design
In this study, a total of four full-size specimens were constructed and tested to failure under
combined vertical load and unbalanced moment. The test specimens represented edge
62 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
connections from a prototype RC flat-slab structure with 5 × 5 m2 (196.9×196.9 in2) square
panels. Each specimen was simply supported on three edges, simulating lines of contra flexure
in the prototype floor, and monolithic with a column at the middle of the fourth edge. The lines
of contra flexure were assumed to be 0.2l away from the column centerlines, where l is the span
between the column centerlines. All slabs had identical geometries of 2500 × 1350 × 200 mm
(98.4 ×53.1×7.9 in.) with a 300-mm (11.8 in.) square column stub protruding 700 mm (27.6 in.)
above and below the slab surfaces. The slabs were simply supported on a 2000 × 1150 mm (78.7
× 45.3 in.) perimeter on the bottom face of the slab. The nominal concrete cover both on the top
and bottom faces of the slabs was 21 mm (0.83 in.). Figure 4.1 shows the typical geometry and
reinforcement details of the test specimens.
All slabs had identical reinforcement in the tension and compression sides as well as similar
material properties but different types of transverse-reinforcement systems and extension from
the column faces. Each specimen was reinforced in the short and long directions, respectively,
with 10 and 20 No. 20 bars (20 mm (0.79 in.) in diameter) as a flexural tension reinforcement
in the bottom side and 7 and 10 No. 15 bars (15 mm (0.6 in.) in diameter) in the compression
(top) side with at least two bars passing through the column core to satisfy the requirement for
structural integrity reinforcement in CSA A23.3 (2014). The average bottom reinforcement ratio
(ρb) was 1.55%, while the average compression (top) reinforcement (ρt) was 0.68%. Table 4.1
presents the test matrix and characteristics for each specimen.
Specimens with shear reinforcement were designed to have high amounts of flexural
reinforcement such that punching-shear failure would be expected to occur prior to flexural
failure. That would allow for measuring the shear-strength contribution of the GFRP stirrups
and for the shear-reinforcement system to achieve its maximum strength and deformation
capacity. Two connections (G-CS-1.75d and G-CS-4.25d) were reinforced in shear with discrete
four branches of closed GFRP stirrups (No. 10, 10 mm in diameter) extended to 1.75d and 4.25d
away from the column face, respectively, where d is the slab effective depth equal to 160 mm.
Slabs G-CS-1.75d and G-CS-4.25d were designed to evaluate the effect of stirrup extension on
the punching behavior and to quantify the concrete contribution (vc) to shear strength outside
the shear reinforced zone. The third connection (G-SS-4.25d) was reinforced with four branches
of spiral GFRP stirrups (No. 10) extended to 4.25d away from the column face to study the
63
influence of stirrup type on the punching strength and deformation capacity and to compare its
behavior with the counterpart slab (G-CS-4.25d) with discrete closed stirrups. The remaining
slab (G) served as the control with no shear reinforcement. The shear-reinforcement ratio (ρfv)
at the perimeter of 0.5d from the column face was maintained constant at 0.9%.
64 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
Figure 4.1 – Typical slab geometry and reinforcement details: (a) Concrete dimension;
(b) Bottom mesh configuration; (c) Top mesh configuration; (d) Sec (A-A) (Note: 1 mm =
0.0394 in.)
250 7
00
Position of steel tie rods to enable
slab anchorage and setup fixing
1350
70
0
300
250
x
y
57
5
P1
57
5
P2
Vu
200 Straight bars
bars
GFRP No. 20
27
3
7@
11
4
5 @152 170
1350
25
00
11
10
GFRP No. 20
Bent bars
3@
93
269
Strain gauges
(a) (b)
304 456
Straight bars
GFRP No. 15
27
3
170
1350
25
00
11
10
GFRP No. 15
Straight bars
269
34
2
45
6
3@
93
3
(c)
300 1050
16
00
700
20
0
6@
10
0
GFRP No.15
6-25M
10M stirrups
GFRP No. 20 1
60
(d)
A A
A A
61
61
40
40
90
90
65
The shear-reinforcement stirrups were arranged in a cruciform pattern according to ACI 318
(2014) and CSA A23.3 (2014). The number of peripheral lines of shear reinforcement varied
B B
42
3
Outer critical section
4.7
5d
650 290
9@
80
Inner critical section
40
410
Strain gauges
GFRP closed stirrups
9@80 40
Outer critical section
Strain gauges
C C
42
3
Outer critical section
4.7
5d
650 290
9@
80
Inner critical section
40
410
GFRP spiral stirrups
GFRP spiral stirrups
9@80 40
Outer critical section
2.2
5d
40
4@
80
A A
Inner critical section
outer critical section
410 330 610
Strain gauges
GFRP closed stirrups
4@80 40
Outer critical section
GFRP closed stirrups
Section (A-A) Section (B-B) Section (C-C)
(a) (b) (c)
(d)
42
3
GFRP closed stirrups
69
160 360
69 GFRP bent bars No. 20
290
9.5
290
9.5 40 145 145
40
GFRP Closed stirrup No.10 GFRP spiral stirrup No.10
Figure 4.2 – Shear stirrups configuration: (a) Closed stirrups arrangement (G-CS-1.75d); (b) Closed stirrups
arrangement (G-CS-4.25d); (c) Spiral stirrups arrangement (G-SS-4.25d); and (d) Typical dimensions of
bent bars and stirrups (Note: 1 mm = 0.0394 in.)
66 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
between four and nine in both directions among the specimens; the spacing between the
consecutive lines was 0.5d. The first perimeter was offset 0.25d from the column face for all
slabs with shear reinforcement, as specified in CSA A23.3 (2014). Figure 4.2 shows the shear-
stirrup layout and arrangement. Each slab was monolithic with a square column stub, which was
designed to transfer shear force and lateral moment to the slab without any premature column
failure. The column reinforcement consisted of six 25M deformed steel bars (three bars on each
face) with 10M deformed closed steel ties at 100 mm (3.9 in.). Figure 4.1 provides the details
of the reinforcement used in the test specimens.
Table 4.1 – Details of test specimens
Test
Specimen a
fcˊ b,
MPa
ftˊ b,
MPa
Average Flexural-
Reinforcement Ratio Stirrup Layout Parameters
Bottom Top Shape
Width × height,
mm× mm
So,
mm
Sfv,
mm Extent
ρb, % ρt, %
G 41.4 3.6 1.55 0.65 ------ ------ ------ ---- ----
G-CS-1.75d 47.6 3.9 1.55 0.65 Closed 290×145 0.25
d 0.5d 1.75d
G-CS-4.25d 51.3 3.9 1.55 0.65 Closed 290×145 0.25
d 0.5d 4.25d
G-SS-4.25d 52.5 3.5 1.55 0.65 Spiral 290×145 0.25
d 0.5d 4.25d
a G-aa-xd: G for GFRP tension reinforcement, aa for stirrup configuration (CS for closed stirrups; SS for spiral
stirrups); and xd for stirrup distance from the column faces relative to the average effective depth, if any. b Cylinder strength at day of testing [100×200mm cylinders (3.9×7.9 in.)].
1MPa = 145 psi; 1 mm = 0.0394 in.
4.3.2. Material Properties
Concrete—All specimens were cast using normal-weight, ready-mixed concrete with a targeted
28-day concrete compressive strength of 35 MPa and 5% to 8% of entrained air. The slab and
the bottom and top column stubs were cast monolithically on the same day. The concrete
compressive (fcˊ) and tensile strength (ftˊ) of each specimen were determined, on the day of
testing, using six 100 × 200 mm (3.9 × 7.9 in.) concrete cylinders for each of the compression
and splitting tests. The concrete compressive strength ranged from 41.4 to 52.5 MPa (6 to 7.6
ksi), whereas the tensile strength ranged from 3.5 to 3.9 MPa (0.51 to 0.57 ksi). Table 4.1
provides the concrete strengths.
Flexural Reinforcement—Grade II and III sand-coated GFRP bars—classified in CSA S807
(2015) as No. 15 and No. 20—were used as flexural reinforcement in all specimens. Each
specimen was reinforced with layers of straight GFRP bars, except for the tension reinforcement
67
(bottom) in the short direction, which had double bent ends. That was to provide the required
anchorage and avoid any unexpected mode of failure, such as slippage failure rather than
punching failure. Table 4.2 reports the tensile properties of the GFRP bars, which were
determined by testing five representative specimens in accordance with ASTM D7205M (2011)
as shown in Figure 4.3. The tensile properties were calculated with nominal cross-sectional areas.
Transverse shear reinforcement—Discrete No. 10 closed and rectilinear sand-coated spiral
GFRP stirrups [290 mm (11.4 in.) wide × 145 (5.7in.) mm high] were used as shear
reinforcement. The tensile strength and elastic modulus of the straight portions were determined
in accordance with ASTM D7205M using five samples cut from the FRP stirrups. The bend
strength of the GFRP stirrups was determined by testing five specimens according to the B.5
test method (concrete blocks) in accordance with ACI 440.3R-04 (2012). Figure 4.3 also shows
specimen preparation and testing as well as the mode of failure, whereas Table 4.2 presents the
tensile properties of the GFRP stirrups. Figure 4.2 also depicts the FRP bent bars and shear-
reinforcement stirrups used herein.
Table 4.2 – Tensile properties of the reinforcing bars and shear reinforcement
Bar Designation a
Nominal
Cross-Sectional
Area a
(mm2)
Ultimate Tensile
Strength
(MPa)
Elastic Tensile
Modulus
(GPa)
Ultimate Tensile
Strain
(%)
GFRP straight flexural bars
No. 15 GFRP bar 199 1323 ±12 64.8±0.5 2.04 ±0.05
No. 20 GFRP bar 285 1334 ±85 64.9±0.6 2.06 ±0.13
GFRP bent flexural bars
No. 20 straight portion 285
1210±63 53.0±0.48 2.28±0.15
No. 20 bent portion ffvb b= 490±44 ------ ------
GFRP-stirrup shear reinforcement
No. 10 straight portion 71
967±39 45.7±0.5 2.12±0.08
No. 10 bent portion ffvb b= 489±38 ------ ------
Steel bars
10M 100 fy c= 420 200 ɛy = 0.21
25M 500 fy c= 470 204 ɛy = 0.23
a According to CSA S807 (2015). b ffvb = ultimate tensile bend strength obtained from the B.5 test method according to ACI 440.3R (2012). c fy steel yielding strength and εy steel yielding strain, as provided by the manufacturer.
Note:1 MPa = 145 psi; 1 GPa = 145 psi; 1 mm2 = 0.00155 in.2
68 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
Figure 4.3 – B5 test method: (a) B5 test specimens; (b) Typical mode of failure at bend portion
(Note: 1 mm = 0.0394 in.)
4.3.3 Instrumentation
Strains in the bottom flexural reinforcement (tension side) were measured with 11 electrical
resistance strain gauges [6 mm (0.24 in.) long] at different locations in both orthogonal
directions (Fig 4.1). The strain gauges were located at a distance of 0, 75, 225, 450, and 750 mm
(0, 3, 8.9, 17.7, 29.5 in.) from the column face on one bar in each direction. In addition, one
electrical strain gauge was glued at the bend location of the GFRP bar at the column location
(see Fig. 4.1). Strains in the GFRP stirrups were measured through 6 mm (0.24 in) strain gauges
mounted at mid-height of the vertical legs and bend location in each orthogonal direction as
shown in Fig. 2. In addition, five concrete electrical strain gauges [60 mm (23.6 in.) long]—
(a)
a) Preparation of test samples
300 mm 400 mm 300 mm Steel stirrups to
prevent splitting
Steel stirrups to
prevent splitting
C-shaped FRP bent bars (No.20)
C-shaped FRP stirrups (No.10)
Debonding tube
(b)
69
labeled C1 to C5—were glued before testing to the slab's top surface (compression side) at 0
and 200 (7.9 in.) mm from the column face (see Fig. 4.4).
Sixteen string potentiometers (pots) were used at different locations to measure the
displacements. Eleven pots (P1 to P11) were placed on the top slab face along two orthogonal
directions at a distance of 80, 250, 550, and 850 mm (3.1, 9.8, 21.6, 33.5 in.) from the column
face to measure the slab-deflection profile while one pot (P15) was located at the column
centerline to measure the central deflection. Two pots (P12 and P16) were installed horizontally
on the top and bottom column ends to measure column lateral displacements. To monitor any
possible shifting of the specimen or test setup, two pots (P13 and P14) were installed in the
horizontal loading directions at the center of slab thickness and frame test setup. All instruments
were installed onto rigid steel frames, separated from the testing frame and attached directly to
the laboratory floor, to prevent any frame deformations from affecting the measurements. The
strain gauges, and pots were connected to a data-acquisition system to record the readings.
Figures 4.1, 4.2, and 4.4 show the position of several instrumentation details of the test specimen.
During the test, crack propagation was marked, and the corresponding loads were recorded.
4.3.4. Experimental Setup
The specimens were tested in the structural laboratory at the University of Sherbrooke under
monotonic vertical shear force and lateral static unbalanced moment until failure, as shown in
Fig. 4.5. The test setup included three main parts: (1) the testing frame, (2) reaction frames, and
(3) the supporting bed and top restrain beams. The testing frame consisted of two main frames
(labeled number 1 in Fig. 4.5) and a stiff connecting steel I-beam on top. A 1500-kN (337.2
kip.) vertical hydraulic jack was installed at the center of the I beam to apply vertical load at the
top of the concrete column. During testing, a steel pan with rollers (connection 5) was placed
between the vertical jack and the top of upper concrete column to free horizontal movement of
the column during lateral loading while maintaining the vertical load. Two 1000 kN (224.8 kip.)
horizontal hydraulic jacks were installed on two very rigid reaction frames (labeled number 2
in Fig. 4.5) fixed firmly to the laboratory strong floor to apply lateral loads. The vertical and
lateral jacks were controlled using three manual hydraulic pumps. The loads were monitored
with three load cells on each pump and connected to the data-acquisition system.
70 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
The specimens were simply supported on the bottom surface along three sides during testing
with a new fabricated supporting steel bed (labeled number 3 in Fig. 4.5), which was designed
to ensure adequate strength and stiffness under the testing load of the specimens. The supporting
bed consisted of four-square steel beams [HSS 250 × 150 × 8 mm (9.8 × 6 × 0.3 in.)] supported
on four square columns [HSS 152 × 100 × 6 mm (6 × 3.9 × 0.24 in.)] laterally stiffened with
back-to-back double steel angles [102 × 102 × 7.9 mm (4 × 4 × 0.31in.)] in both directions. It is
worth mentioning that, before placing the test specimen in the setup, the supporting bed was
prestressed directly on the laboratory strong floor with four 38 mm (1.5 in.) diameter steel tie
rods to prevent the supporting bed from moving laterally. On the slab top face, the three
supported edges were restrained by steel reaction beams (labeled number 4) to prevent slab
lifting. Each end of the reaction beam was held in position by four steel nuts and plates attached
to the steel tie rods. In addition, 20 mm (0.79 in.) thick neoprene pads were placed between the
slab and supporting bed and between the slab and top restrain beams along the support lines to
simulate slab rotation at the line of contraflexure and ensure uniform stress distribution along
the edges.
4.3.5. Test Procedure
The specimens were subjected to vertical load (V) through the column stub and unbalanced
moment (Mun) through two opposite horizontal loads (P) applied at the tips of column ends. The
unbalanced moments were calculated by multiplying the two lateral loads, applied to each
column by the distance from the application point to the center of the slab: 675 mm (26.6 in.)
[see Fig. 4.1]. The ratio between the unbalanced moment and vertical load (Mun/V) was 0.3 m
(11.8 in.). This value was based on analysis of a typical floor-system prototype under gravity
loads only according to CSA A23.3 (2014). The vertical load was applied monotonically at a
load-controlled rate of 5 kN/min (1.12 kip/min), whereas the horizontal loads were
simultaneously applied with the vertical load in small increments to maintain a constant M/V
71
ratio of 0.3 m (11.8 in.) throughout the test until failure.
C1
P9
P12
P13
P14
P11
P1 P2 P3 P4
P8
P5
P6
Test setup sliding
Lateral top displacement
Lateral Bottom displacement
P16
P10
Vertical Pots
P7
Horizontal pots
C2
C3 C4
C5
Concrete
gauges
P15
Figure 4.4 – Instrumention details
72 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
Figure 4.5 –Test setup
(1) Main steel frames (2) Reaction frames
(3) Square prestressed supporting bed (4) Restrain top frame
(5) Steel pan, roller, and column collar joint (6) Bed connection
(7) Lateral hydraulic jacks (8) Lateral steel post
(9) 4 Steel tie rods (38 M in diameter) (10) Steel clamps
(11) Pot supporting frame (12) Hydraulic pumps and data-acquisition system
(13) Test specimen (14) Neoprene pads [20 mm (0.79 in.) thick]
(11)
(4)
(14)
(5) (2)
(2)
(5)
(2)
(2)
(6)
(3)
(7)
(7)
(10)
(9)
(11)
(1)
(12)
(13)
(8)
(1)
Stiff connecting steel I-beam
(6)
Spacer
73
4.4. Test Results
4.4.1. Overall Response and Cracking Pattern
The tested specimens showed similar cracking propagation on the bottom surface (tension side)
and along the slab’s free edge during the test. Specimens with shear reinforcement, however,
evidenced more intensive cracks with larger punching-shear failure surfaces compared to their
counterpart without shear reinforcement. Figure 4.6 shows the cracking patterns for all the test
specimens in tension and compression and along the free-edge sides. Generally, three typical
kinds of cracks were observed on the tension side, progressing in the following sequence as the
applied loads were increased: 1) Radial flexural cracks (fan-shaped) originated from the inner
slab–column interface and propagated towards the supports. The cracks began to appear at
vertical loads between 51 and 72 kN (11.5 and 16.2 kip) [at about 15% to 16% of the ultimate
loads]. (2) Inclined torsion cracks formed at the inner corners of the columns at about 35° form
the slab edge. The cracks started to appear at between 23% and 25 % of the ultimate loads. They
then propagated upward the slab edge to half of the slab depth at approximately 50% of the
ultimate loads and then further extended until reaching the top of the slab. These cracks were
normally developed at an angle of approximately 90° to the diagonal shear cracks that formed
later when punching occurred. (3) Circumferential (tangential) cracks generated around the
column and crossed over the radial cracks at higher loads approximately at 52% to 60% of the
test-specimen ultimate loads. As the loads increased, the number of such cracks and their widths
in the column vicinity increased. At the same time, new diagonal shear cracks caused by the
shear stresses initiated near the slab free edge from the bottom side and then extended toward
the top of the slabs. These diagonal cracks propagated with small widths until the test specimen
failed. At failure, a major tangential crack was intercepted by the flexural cracks in
approximately perpendicular manner forming the punching cone. Figure 4.6 shows the diagonal
shear cracks at the free edge of the slabs.
74 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
Figure 4.6 – Cracking patterns and punching-shear failure surface for the tested specimens
G-SS-
4.25d
G-SS-
4.25d G-SS-
4.25d
Compression side Tension side
Compression side Tension side
G-CS-
4.25d
G-CS-
4.25d
G-CS-
4.25d
Compression side Tension side
G-CS-
1.75d
G-CS-
1.75d
G-CS-
1.75d
Compression side Tension side
G
G G
75
4.4.2. Mode of Failure and Envelope
Control specimen G, without shear reinforcement, experienced a typical brittle punching-shear
failure without much warning. The punching failure along the slab free edge was characterized
by a main diagonal shear crack inclined to the tension side of the slab at an angle of 29o. Spalling
of the concrete cover on some parts of the tension side as well as fine torsion cracks on the slab
compression side (Fig. 4.6) were also observed. In the case of specimen G-CS-1.75d, with
stirrups extended 1.75d, the FRP stirrups effectively contributed in distributing the shearing
forces to the uncracked concrete outside the shear-reinforced zone. The mode of failure was
punching-shear failure outside the shear zone. Some deformability was, however, achieved
before failure compared to the control specimen, G, without shear reinforcement. The slab free
edge evidenced horizontal splitting cracks over the top of the shear stirrups near the column top
before joining with inclined cracks that developed outside of the shear-reinforced zone. The
G Punching surface
Inclined cracks Column
G-CS-1.75d Punching surface Inclined cracks
Closed stirrups
Closed stirrups Punching surface
Punching surface Closed stirrups
Closed stirrups
Inclined cracks G-CS-4.25d Hz. splitting crack
Column
G-SS-4.25d Hz. splitting crack
Column Spiral stirrups
Inclined cracks
Hz. split. crack Column face Spiral stirrups
Figure 4.7 – Inclined shear cracks and failure envelope on the two parts of cut sections
76 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
angle of the shear crack at the free edge was 25º with respect to the slab tension side. Other
torsion cracks on the slab compression side were also observed.
The extension of the FRP stirrups by 4.25d for specimens G-CS-4.25d and G-SS-4.25d offered
sufficient resistance and larger deformations before final failure. A similar horizontal splitting
crack over the top of the shear reinforcement, as in specimen G-CS-1.75d, was seen at the slab
free edge but extended further away from the column face to the sixth line of stirrups before
joining with inclined cracks. The increase in the deformation capacity and the concrete crushing
in the column vicinity on the compression side of the slabs were considered early warning signs
before the punching-shear failure occurred. As a result, the mode of failure was mixed flexural–
punching-shear failure within the shear-reinforced zone. This behavior has been observed with
interior steel-reinforced slab–column connections reinforced with shear studs (Grander et al.
1996 and Dam et al. 2017).
Figure 4.7 shows sawn sections for all specimens with and without shear reinforcement through
a line perpendicular to the free edge and adjacent to the column. This figure shows a clear view
of the cracks within the slabs. Specimen G had a single shear crack with an inclination angle of
39.5º. The radius of the punching failure surface extended 2.9d [464 mm (18.3 in.)] from the
lower column face. Specimen G-CS-1.75d had a horizontal splitting crack over the top of the
stirrups. This splitting crack became an inclined shear crack beyond the outermost set of shear
stirrups, which confirms that the punching shear occurred outside the shear-reinforced zone.
The angle of the inclined shear crack was about 25º with respect to the slab tension side and the
radius of the failure surface extended 3.9d [624 mm (24.6 in.)] from the bottom column face.
For the other specimens, several inclined shear cracks were observed within the regions
reinforced with shear stirrups as well as horizontal splitting cracks located above the shear
stirrups. The formation of the horizontal splitting cracks near the columns is assumed to have
caused the slight gradual drops in load capacity. Finally, these inclined and splitting cracks
created the failure surfaces. This observation confirmed the occurrence of the mixed flexural–
punching-shear failure.
4.4.3. Vertical Load–Deflection Characteristics
Figure 4.8 plots the applied vertical load versus deflection relationships at 80 mm from the
column face in both directions for all the tested specimens. Table 4.3 provides the maximum
77
applied vertical load (Vu) and corresponding ultimate deflection (ΔVu) for each specimen. In
general, the initial uncracked stiffness for all specimens was similar, regardless of the presence
of shear reinforcement. The slabs with shear reinforcement, however, exhibited slightly higher
post-cracking stiffness compared to their counterparts without shear reinforcement. In the case
of control specimen G and specimen G-CS-1.75d, including limited stirrups around the column
produced similar bilinear load–deflection responses until the punching failure occurred abruptly,
as shown in Fig. 4.8. Specimens G and G-CS-1.75d failed, respectively, at 314 and 370 kN (70.6
and 83 kip) ultimate loads and at 21 and 28 mm (0.83 and 0.31 in.), corresponding to ultimate
deflections along the moment direction. In comparison to specimen G, specimen G-CS-1.75d
achieved 18% and 34% increases in failure load and deflection, respectively.
Specimens G-CS-4.25d and G-SS-4.25d, with shear reinforcement extending 4.25d, showed
different responses compared to G and G-CS-1.75d, specifically gradual failure with
considerable post-peak deformations. The addition of FRP stirrups resulted in flexure
mechanism due to the mobilization of the shear reinforcement before punching-shear failure.
Specimens G-CS-4.25d and G-SS-4.25d failed at ultimate loads of 444 and 486 kN (99.8 and
109.3 kip), respectively, and at corresponding ultimate deflections along the moment direction
of 36 and 46 mm (1.4 to 1.8 in.), respectively. As shown in Fig. 4.8, the load–deflection curves
for the two specimens were similar in both directions. Nevertheless, the load–deflection curves
perpendicular to the free edge expanded horizontally in the opposite direction after the peak (see
Fig. 4.8 a). This might be due to separation of the concrete over the stirrups in top surface of the
slab because of opening the horizontal splitting cracks during the test and the deflection readings
were not affected. The load–deflection curves parallel to the free edge showed post-peak
softening behavior with large deformations (Fig. 4.8 b). The resulting maximum deformations
of G-CS-4.25d and G-SS-4.25d at failure were 1.8 and 2.4 times that of G, respectively. This
confirms the effectiveness of closed and spiral stirrups in achieving substantial deformations
before slab collapse.
78 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
Table 4.3 – Summary of the test results
Specimen
Cracking
LoadUltimate Load Δvu,
mm
Δvu,
mm
Strains at Ultimate Load (µs) Deformabilit
y Factor,
JΔ
Energy Absorption Failure
Modesb
Vcr,
kN
Mcr,
kN.
m
, uV
kN
Mu,
kN.
m
vu, inside,
MPa
vu,
outside,
MPa
Concret
e, µs
Flexural
reinforcementFRP stirrups Due to
deflection
UΔ,
kN.m
Due to
rotatio
n Uθ,
kN.m
┴a // a ┴ a // a ┴
a // a
G 51 16 314 98 2.44 --- 20.5
518.95 784 6432 5387 ----- ----- 12.15 4.23 1.64 P
G-CS-
1.75d53 18 370 115 2.87 1.21 28.0
826.19 979 8661 7683 3918 3402 16.40 6.86 3.44 P *
G-CS-
4.25d63 20 444 133 3.38 0.88 35.8
233.36 2444 13,226 9141 6412 5899 32.59 10.54 6.60 P †
G-SS-4.25d 72 24 486 146 3.70 0.97 46.1
945.29 2696 13,947 9602 7035 6525 36.68 14.34 7.20 P †
a Position perpendicular (┴) or parallel (//) to the free edge. a P (punching failure). * Brittle punching failure occurred outside the shear-reinforced zone.† Flexure- punching failure occurred inside the shear-reinforced zone.
Note: 1 kN = 0.2248 kip, 1 kN.m = 8.86 kip.in., 1 mm = 0.0394 in.
79
4.4.4. Moment–Rotation Relationships
Figure 4.8 c gives the applied unbalanced moment versus column rotation relationships for all
tested specimens. The column rotation was calculated as the ratio of the sum of measured
displacements at the column ends by means of potentiometers P12 and P16 to the distance
between the two loading rams (see Fig. 4.4). As seen in Fig. 4.8c, the measured rotations of the
columns at failure increased with the use of stirrup shear reinforcement. The ultimate rotations
for specimens G, G-CS-1.75d, G-CS-4.25d, and G-SS-4.25d were 0.0182, 0.0352, 0.0444, and
0.0515 radians, respectively. The ultimate moment increased by 17%, 36%, and 49% and
rotation capacities increased by 93%, 144%, and 183% for specimens G-CS-1.75d, G-CS-4.25d,
and G-SS-4.25d, respectively, compared to the control specimen G. It is also important to note
that, in maintaining the same amounts of flexural and shear reinforcement in specimens G-SS-
4.25d and G-CS-4.25d, spiral stirrups performed better than closed stirrups, with the ultimate
moment and rotation capacities increased by 10% and 16%, respectively. On the other hand,
increasing the stirrup extension around the column from 1.75d to 4.25d increased the moment
and rotation capacities of the connection by 16% and 26%, respectively.
4.4.5. Flexural Reinforcement and Concrete Strains
Figure 4.9 plots the applied vertical load versus the flexural tension reinforcement and concrete
strains for all tested specimens. The flexural-reinforcement strains were measured at 75 mm
from the column face perpendicular and parallel to the free edge, whereas the concrete strains
were recorded at the column face with gauge C1 (Fig. 4.4). Table 4.3 reports the maximum
reinforcement and concrete strains. Specimen G, without shear reinforcement, showed the least
tensile strain compared to its counterparts with GFRP-stirrup reinforcement. The maximum
reinforcement strain was 6430 μs, which represents 35% of the ultimate tensile strength. Besides,
the maximum concrete strains around the column region were low and below the concrete
crushing strain of 3500 and 3000 μs, as per CSA S806 (2012) and ACI 440.1R (2015),
respectively. Upon punching-shear failure, however, no concrete crushing in the compression
zone was observed.
80 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
Figure 4.8 – Vertical load–deflection relationships: (a) Perpendicular to the free edge; (b)
Parallel to the free edge; and (c) Moment–rotation relationships (Note: 1 mm = 0.0394 in.; 1
kN = 0.2248 kip; 1 kN.m = 8.86 kip.in.)
Specimens G-CS-1.75d, G-CS-4.25d and G-SS-4.25d, with shear reinforcement, exhibited
higher strains in the GFRP reinforcing bars and higher concrete strains values compared to
control specimen G at ultimate. The maximum reinforcement strains were 8700, 13200, and
13900 μs, respectively, representing 47%, 71%, and 75% of the ultimate tensile strength,
respectively. The maximum recorded concrete strains were 979, 2444, and 2696 μs (< 3000 or
3500) for G-CS-1.75d, G-CS-4.25d, and G-SS-4.25d, respectively. It is important to report that
the mode of failure of specimen G-CS-1.75d was triggered by brittle punching-shear failure
occurring outside the shear-reinforced zone with no signs of concrete crushing in the
compression zone (see Figs. 4.6 and 4.7). In contrast, for specimens G-CS-4.25d and G-SS-
(a) (b)
(c)
81
4.25d, the achieved higher concrete strains indicated concrete crushing in the column vicinity
on the compression side of the slabs, which exhibited the mixed flexure–punching-shear failure.
Figure 4.10 shows the flexural-reinforcement-strain distribution along selected bars at different
load levels. Figure 4.10 shows that the reinforcement strains decayed in both orthogonal
directions toward the supported slab edge until reaching very low strain values at 750 mm from
the column face. This implies that the sand-coated GFRP bars used adequately transferred loads
with no signs of bar slippage or bond failure during the tests.
(a) (b)
(c)
Figure 4.9 – Vertical load–strain relationships: (a) Reinforcement strain perpendicular to the free
edge; (b) Reinforcement strain parallel to the free edge; (c) Concrete strain (Note: 1 kN = 0.2248 kip)
82 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
G G
G-CS-1.75d G-CS-1.75d
G-CS-4.25d G-CS-4.25d
G-SS-4.25d G-SS-4.25d
Figure 4.10 – Distribution of flexural-reinforcement strains in both directions (Note: 1 mm = 0.0394 in.)
83
4.4.6. Shear-Reinforcement Strains
Figure 4.11 depicts the vertical-strain distributions in the stirrups versus the distance from the
column face divided by d at different load levels in both orthogonal directions. As shown, the
stirrup strains decreased as the distance from the column face increased. In all the specimens,
the strains in the stirrups increased rapidly beyond the 80% of the ultimate loads. The maximum
strains were recorded in the FRP stirrups for up to a distance of 0.25d to 1.25d from the column
faces without any apparent signs of rupture in the vertical or bent portions of the stirrups. The
maximum recorded strains at 95% of the ultimate loads in both directions were 7035 and 6412
μs for specimens G-SS-4.25d and G-CS-4.25d, respectively, representing 33% and 30% of the
ultimate tensile strain, respectively. For specimens G-CS-1.75d, G-CS-4.25d, and G-SS-4.25d,
the average strains in the vertical portions of the FRP stirrups in both directions were 2867, 5305,
and 5163 μs, respectively, which represents 53%, 106%, and 103%, of the CSA S806 (2012)
strain limit, respectively, and 72%, 132%, and 129% of the ACI 440.1R (2015) strain limit.
Thus, the FRP shear reinforcement might be designed with a strain value of 4000 or 5000 μs, as
recommended in ACI 440.1R (2015) and CSA S806 (2012) (Hassan et al 2014). Table 4.3 lists
the maximum recorded strains in the FRP stirrups.
It is worth mentioning that the FRP shear stirrups along the moment direction between 1.75d
and 2.25d achieved relatively high strains compared to the measured strains at 0.25d at 95% of
the ultimate loads. The measured strains at 1.75d for G-CS-1.75d, G-CS-4.25d, and G-SS-4.25d
were 2765, 5486, and 4934 µs, respectively, and the strains at 2.25d were 4637 and 3356 µs for
G-CS-4.25d and G-SS-4.25d, respectively. This implies that the FRP stirrups were still active
up to 2.25d. In addition, limiting the extension of the FRP stirrups in specimen G-CS-1.75d
beyond a distance of 1.75d exhibited only limited deformation capacity and occurrence of brittle
punching failure. Therefore, more experimental work is needed to determine a minimum
extension limit of FRP stirrups for FRP-reinforced slab–column connections to overcome brittle
punching failure.
84 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
Figure 4.11 – Vertical strain distribution in vertical legs of stirrups
G-CS-1.75d
G-CS-4.25d G-CS-4.25d
G-SS-4.25d G-SS-4.25d
G-CS-1.75d
85
4.4.7. Ultimate Strength
The failure loads were multiplied by (48/fc' )1/3 to account for variations in concrete strength,
where fc' (MPa) is the compressive concrete strength of each specimen and 48 (7 ksi) is the
average concrete strength for all the tested specimens in MPa. The test results show the effect
of the FRP stirrups as shear reinforcement in increasing not only the punching-shear strength
but also the deformation capacity of the tested specimens, even with the limited amount of
stirrup extension around the column. Specimens G-CS-1.75d, G-CS-4.25d, and G-SS-4.25d
evidenced noticeable increases in the normalized vertical shear force at ultimate load by 12%,
32%, and 43%, respectively, compared to specimen G (without shear reinforcement). Besides,
increasing the stirrup extension around the column from 1.75d to 4.25d increased the normalized
vertical-shear force by 17%. Use of spiral stirrups in specimen G-SS-4.25d showed an increased
normalized ultimate capacity of 9% compared to specimen G-CS-4.25d, with closed stirrups,
with the same amounts of flexural and shear reinforcement and distribution layout.
4.4.8. Deformability and Energy Absorption
A main concern of slab–column connections is the prevention of brittle failure. Thus, the
connection must be able to deform significantly before collapse. In steel-reinforced concrete
members, ductility measures the ability of the structural member to undergo significant large
deformations before failure, which provides a warning of impending failure. Ductility in steel-
reinforced concrete is quantified by the ratio of maximum displacement or rotation to that at
yielding of the steel reinforcement. Unlike steel bars, GFRP bars do not exhibit a yielding
plateau. GFRPRC members, however, could achieve significant deformations before failure due
to the low elastic modulus of GFRP bars. Consequently, the deformability factor (CSA S6 2014)
J∆ was introduced to quantify the deformation property of GFRP-RC structures (Eq. 1), in which
P and ∆ are the vertical load and deflection and the subscripts u and s refer to the ultimate and
service limit states, respectively. The service limit state for GFRP has several definitions, such
as the state corresponding to a concrete compressive strain of 1000 με (CSA S6 2014) or a
tensile strain of 2000 με in the flexural reinforcement (Design Manual No3, 2007). The service
limit state corresponding to a tensile strain of 2000 με was used in this study to compute the
deformability factor (El-Gendy and El-Salakawy 2016). Table 4.3 provides the deformability
86 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
factors for all specimens.
u u
s s
PJ
P
=
(4.1)
As shown in Table 4.3, the deformability factors were substantially enhanced by using GFRP
stirrups as shear reinforcement around the column at each connection. For specimens G-CS-
1.75d, G-CS-4.25d, and G-SS-4.25d, the deformability factors were 1.4, 2.7, and 3 times higher
than that of control specimen G without shear reinforcement. In addition, extending the FRP
stirrups 4.25d from the column face significantly contributed to reducing slab brittleness, thus
increasing slab safety. The deformability factor of G-CS-4.25d was 2 times higher than that of
G-CS-1.75d. On the other hand, specimen G-SS-4.25d, which had spiral stirrups in instead of
the discrete closed stirrups in specimen G-CS-4.25d, showed an increase of 13%.
Energy absorption of the structural member is of prime importance, particularly in areas of
earthquake activity. Two different measurements can be used to evaluate the energy absorption
of slab–column connections using slab deflections (UΔ) or slab–column rotations (Uθ) (Marzouk
et al. 1996). Energy absorption is calculated by integrating the area under the load–deflection
(Fig. 4.8a) or moment–rotation (Fig. 4.8c) curves. Table 4.3 gives the calculated values for all
tested specimens. The energy absorptions by deflection for specimens G-CS-1.75d, G-CS-4.25d,
G-SS-4.25d were about 58%, 149%, and 239% and by rotation were about 110%, 302%, and
339% higher than that of specimen G, respectively. The reported values indicate that, even in
limited amounts, GFRP stirrups can be an efficient means for increasing the strength,
deformation, and rotation capacity, and the energy absorption of edge flat slab–column
connections.
4.5. Discussion
4.5.1. Influence of Stirrup Extension
In general, the presence of GFRP stirrups as shear reinforcement inside the punching-shear zone
significantly improves slab behavior. The strength and deformation capacity of shear-reinforced
slabs are, however, strongly influenced by the characteristics of the shear reinforcing system
(i.e., extension, amount, type, etc.). Increasing the GFRP-stirrup extension from 1.75d to 4.25d
87
was attributed with achieving large punching strength and deformations before stirrup final
failure, regardless of whether closed or spiral GFRP shear reinforcement was used. The GFRP
stirrups offered sufficient resistance and confinement to control the development of large shear
cracks and effectively distributed the shearing forces around the punching-shear zone to fail
inside or outside the shear-reinforced zone. The more significant increase in deformability in
specimens G-CS-4.25d and G-SS-4.25d could be attributed to the fact that, unlike in specimens
G and G-CS-1.75d, flexure mechanism took place, due to the mobilization of shear
reinforcement before punching-shear failure.
The test results indicate that the shear-stress resistance of the concrete contribution decreased
outside the shear-reinforced zone. For example, specimen G-CS-1.75d failed—as intended—
outside the shear-reinforced zone under an ultimate shear-stress resistance of 1.21 MPa (0.18
ksi) [refer to Table 4.3]. The corresponding normalized shear-stress resistance is 1.21 MPa (0.21
ksi), which is 52% less than the normalized shear-stress resistance of 2.56 MPa (3.7 ksi) for
specimen G. It is therefore reasonable to assume the concrete contribution to shear resistance
outside the shear-reinforced zone to be reduced by 50% as recommended in ACI 318 (2014)
and CSA A23.3 (2014). Further experimental tests are needed to examine the effect of GFRP
shear reinforcement with different extensions around the column zone to quantify the concrete-
fraction contribution outside the shear-reinforced zone and determinate the minimum extension
limit of GFRP stirrups.
4.5.2. Influence of GFRP Stirrup Type
The increase in strength and deformation capacity depends somewhat on the shear-
reinforcement system, specifically the good performance of stirrups due to enhanced anchoring.
The spiral stirrups clearly afforded superior response as well as fast, easy installation during
construction compared to the specimens with discrete closed stirrups and the same amounts of
flexural and shear reinforcement. This can be attributed to the better mechanical anchorage of
the spiral stirrups, which enhanced concrete confinement in the compression zone and resulted
in higher capacity and better post-peak behavior. Both GFRP stirrup shear reinforcement
systems can efficiently reduce the brittleness of specimens and provide ample warning before
failure.
88 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
Like steel shear reinforcement, spiral or discrete closed GFRP stirrups with a large amount of
shear reinforcement near the column zone might develop horizontal splitting cracks over the top
of the stirrups, as depicted in Fig. 4.7. This can be attributed to a significant portion of the radial
compressive force occurring in the concrete near the column, which acts in a nearly horizontal
direction and is transmitted to the region around and over the upper part of the shear
reinforcement. This radial compressive force changes its direction. Consequently, tensile
stresses were produced in a horizontal section through the upper part of the shear reinforcement.
In addition, the large amount of shear reinforcement caused an increase in the eccentricity of
the radial compressive force in the concrete, which increased the radial tensile stresses in the
slab’s top surface. This observation coincides with the past experimental findings reported in
the literature by Hassan et al. (2014) and Dam et al. (2017) for FRP and steel slab–column
connections with a large amount of shear reinforcement, respectively.
4.6. Proposed Design Provisions and Predications
4.6.1. Slabs without Shear Reinforcement
The North American codes—that are, ACI 318 (2014) and CSA A23.3 (2014)—compute the
shear stress for steel, vu, using the moment transfer by eccentricity of shear located at a distance
of 0.5d from the column face using the Eq. (4.2).
;0.5
cu v o
uo d c
V Mv
b d J
= + (4.2)
The North American design codes for FRP-reinforced two-way slabs without shear
reinforcement—i.e., CSA S806 (2012) and ACI 440.1R (2015)—are based on the same forms
as steel design codes with modifications to consider the effect of FRP-bar axial stiffness. The
punching-shear resistance provided by concrete (vc) in CSA S806 (2012) [the smallest of Eqns.
4.3-4.5] and ACI 440.1R (2015) [Eq. 4.6] are summarized below.
CSA S806 (2012): without shear reinforcement
( )1
' 32
0.028 1c c f f cc
v E f
= +
(4.3)
89
( )1
' 30.147 0.19sc c f f c
o
dv E f
b
= +
(4.4)
( )1
' 30.056c c f f cv E f = (4.5)
ACI 440.1R (2015): without shear reinforcement
'4
5c cv k f= (4.6a)
( )2
2 f f f f f fk n n n = + − (4.6b)
To date, CSA S806 (2012) and ACI 440.1R (2015) lack provisions for estimating the ultimate
capacity of FRPRC two-way slabs with FRP shear reinforcement. The following section
presents proposed design provisions as an extension to CSA S806 (2012) and ACI 440.1R
(2015) to account for FRP stirrups as shear reinforcement and their properties affecting the
ultimate capacity of FRP-RC slab column connections. It is worth mentioning that the same
procedure in adapting the aforementioned code provisions was originally proposed by El-Gendy
and El-Salakawy (2016) for GFRP-reinforced edge connections reinforced with GFRP ribbed
shear studs.
4.6.2. Slabs with Shear Reinforcement
Regarding steel-reinforced two-way slabs with shear reinforcement, ACI 318 (2014) and CSA
A23.3 (2014) require that the shear stresses be checked either inside or outside the shear-
reinforced zone. The critical shear section inside the shear-reinforced zone is located at 0.5d
from the column faces, while the critical section outside the shear reinforcement lies at 0.5d
from the outermost shear reinforcement. Within the shear reinforced zone, the factored shear-
stress resistance, computed as (vc + vs), where vc and vs are the summations of concrete and
shear-reinforcement contributions to the shear strength inside the punching zone. Design codes
calculated the concrete contribution inside and outside the region reinforced with shear stirrups
as 50% of the punching-shear strength of slabs without shear reinforcement. Accordingly, in
this paper, the concrete contribution inside and outside the shear-reinforced zone for FRP-
reinforced two-way slabs is proposed to have a value equal to 50% of the least of Eqns. (4.3) to
(4.5) according to CSA S806 (2012) or Eq. (4.6) according to ACI 440.1R (2015).
90 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
In order to calculate the FRP-stirrup contribution, Eqns. (4.8) and (4.10) for steel stirrups have
been modified by replacing, fy (yielding strength) with a specific stress (ffv) at a limiting strain
value (εfv) of 5000 or 4000 μs according to CSA S806 (2012) and ACI 440.1R (2015),
respectively, where ffv equals εfv multiplied by the FRP-stirrup modulus of elasticity (Efv). It
should be noted that the ffv should be less than the stress corresponding to the failure of the
stirrup corners or bends as determined with the appropriate procedure in accordance with ACI
440.1R (2015) and CSA S806 (2012). The proposed design equations can be summarized as
follows.
Proposed design provisions for CSA S806 (2012) with the shear-reinforced zone
( )1
' 3, , 0.028c inside c outside c f f cv v E f = = (4.7)
( )0.005f fv fv
fvfvo
A Ev
b S
= (4.8)
Proposed design provisions for ACI440.1R (2015) with the shear-reinforced zone
', ,
2
5c inside c outside cv v k f= = (4.9)
( )0.004f fv fv
fvfvo
A Ev
b S
= (4.10)
4.6.3. Ultimate-Capacity Predications
This section presents an assessment of the accuracy of the current and proposed design equations
(Eqs. 4.2- 4.10) by comparing their predictions with the experimental results and the results
available in the literature for shear-reinforced edge connections. All safety factors and partial
material factors in the equations were taken to be equal to 1.0. Table 4.4 provides the punching-
shear predictions for all tested specimens with and without FRP shear reinforcement. The ACI
440.1R (2015) predications using the current Eq. 4.6 and proposed Eqns. 4.9 and 4.10, as
expected, were consistently very conservative for specimens with and without shear
reinforcement, respectively. For the test specimen without shear reinforcement, the current ACI
440.1R (2015) equation showed an average Vtest /Vpred of 2.15. On the other hand, the proposed
ACI 440.1R (2015) equations gave an average Vtest /Vpred of 1.87 ± 0.25 (a corresponding COV
91
of 24.6%) for test specimens with FRP shear stirrups as well as other shear-reinforced edge
connections reported in the literature. The reason for this is that the concrete-contribution
fraction (vc) involved only the reinforcement ratio in predicting the neutral axis depth
(contribution of the compression area). The Equation (Eq. 4.6) does not consider axial stiffness,
which might make the overall predications excessively conservative. In contrast, CSA S806
(2012) accounts for FRP axial stiffness in the vc. It therefore yielded better predictions.
As shown in Table 4, the current CSA S806 (2012) Eqns. (4.2) to (4.5) and proposed Eqns. (4.7)
and (4.8) gave better predications for test specimens without and with FRP shear stirrups
involving shear-reinforced edge connections reported in the literature. The current CSA S806
(2012) equations gave an average Vtest /Vpred of 1.29 for the test specimen without FRP shear
stirrups. In addition, the proposed CSA S806 (2012) equations showed average Vtest /Vpred values
of 1.28 ± 0.24 (COV of 18.58%) with respect to the test specimens with FRP shear stirrups and
shear-reinforced GFRP-RC edge connections from literature. The proposed design provisions
provide a step forward for engineers in designing two-way FRPRC slabs with FRP stirrups.
More experimental results under eccentric punching shear for interior and edge slab–column
connections are urgently required.
92 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
Table 4.4. Tested-to-predicted punching-shear capacity
Reference Test
Specimen
c,
mm
M/V,
m
RFT.
Type
davg.,
mm
ts,
mm
,
%
Shear
RFT Type
Vu,
kN
Proposed Equations for
CSA S806 (2012)
Proposed Equations for ACI
440.1R (2015)
Vpred, kN
Vu /Vpred
Vpred, kN
Vu /Vpred Insid
e Outside Inside Outside
This study
G S 300 0.31
SG
160 200
1.55 --- 314 244a --- 1.29 146 --- 2.15
G-CS-
1.75dS 300 0.31 1.55 GFRP
stirrups
370 386 303 1.22 282 180 2.06
G-CS-
4.25dS 300 0.30 1.55 444 396 484 1.12 288 286 1.55
G-SS-
4.25dS 300 0.30 1.55 486 397 488 1.22 289 287 1.69
Mostafa and El-
Salakawy (2018)
N-0.9-S8 S 300 0.40 0.85 SG shear
studs
294 352 321 0.92 260 178 1.65
N-0.9-S6 S 300 0.40 0.85 298 286 335 1.04 207 186 1.60
N-0.9-C6 S 300 0.40 0.85 SG C.
bars
253 174 322 1.45 118 179 2.14
N-0.9-C8 S 300 0.40 0.85 286 201 323 1.42 140 180 2.04
El-Gendy and
El-Salakawy (2016)
RD-75-M S 300 0.40 GRD
0.85 GRD
shear
studs
256 154 332 1.66 116 183 2.21
RD-50M S 300 0.40 0.85 273 186 323 1.47 148 179 1.84
Meanc 1.28 Mean c 1.87
SDc 0.24 SD c 0.25
COVc % 18.58 COV c % 13.46
C = shape of column stub and corresponding width; S = square; avg = average flexural tensile reinforcement ratio in both directions; SG = sand-coated glass-fiber; GRD =
ribbed glass-fiber; C = corrugated. a Calculated using Eq. (4.5). b Calculated using Eq. (4.6). c Calculated using the least of Vpred for specimens with shear reinforcement only.
Note: 1 kN = 0.2248 kip, 1 kN.m = 8.86 kip.in., 1 mm = 0.0394 in
93
4.7. Conclusion
On the basis of the test results and discussion presented, the following conclusions were drawn:
• Using either closed or spiral stirrups as shear reinforcement improved the punching behavior
of FRPRC edge slab–column connections. The cracks were more widely distributed
compared to the specimen without shear reinforcement, which failed in a brittle punching-
shear mode.
• The specimens with FRP shear reinforcement extended 4.25d demonstrated a substantial
increase in shear-strength increase over 38%, enhancement of deformation capacity of over
104%, and deformability and energy absorption of over 185%, and 194% (on average) were
observed. This increase might be of interest because it gives significant warning before
punching-shear failure occurs. As a result, these connections fail in mixed flexure–
punching-shear failure.
• The FRP stirrups offered sufficient resistance and confinement to control the development
of large shear cracks and effectively distributed the shearing forces around the punching-
shear zone so that failure occurred inside or outside the shear-reinforced zone.
• In comparison to closed stirrups, spiral stirrups provided better performance as well as fast
and easy installation during construction of the tested specimens for the same amounts of
flexural and shear reinforcement. Specimen G-SS-4.25d, with spiral stirrups, showed an
increase in the punching-shear strength, deformation capacity, and energy absorption of over
9%, 33%, and 36% compared to G-CS-4.25d, respectively. Both systems, however, could
be used to effectively reduce the brittleness of the tested specimens.
• The results indicate that the shear-stress resistance of the concrete contribution decreased
outside the shear-reinforced zone. For instance, specimen G-CS-1.75d failed outside the
shear-reinforced zone under an ultimate shear-stress resistance of 1.21 MPa (0.18 ksi),
which is 52% lower than the normalized shear-stress resistance of 2.56 MPa (0.37 ksi) for
specimen G. Thus, it is reasonable to assume the concrete contribution to shear resistance
outside the shear-reinforced zone be reduced by 50% as recommended in ACI 318 (2014)
and CSA A23.3 (2014). Further experimental tests are needed, however, to examine the
effect of FRP shear reinforcement with different extensions around the column to quantify
this effect on the concrete contribution to the shear resistance.
94 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
• FRP shear stirrups between 1.75d and 2.25d achieved relatively high strains of 4129 and
3748 µs (on average in both directions) at 95% of ultimate load, which implies that the FRP
stirrups were still active up to 2.25d, respectively. In addition, limiting the extension of the
FRP stirrups beyond 1.75d showed only limited deformation capacity and brittle punching
failure occurred. Therefore, more experimental work is needed to determine a minimum
extension limit of FRP stirrups for FRP-reinforced slab–column connections to overcome
brittle punching failure.
• On the basis of the test results, FRP shear reinforcement can be designed with a strain value
of 4000 or 5000 microstrains, as recommended in ACI 440.1R (2015) or CSA S806 (2012),
respectively.
• The simplified approach proposed to predict the ultimate shear capacity of FRP-reinforced
edge slab–column connections with FRP shear reinforcement as an extension to those in
CSA S806 (2012) gave better predications with respect to the experimental test results as
well as the available results in the literature.
• The proposed ACI 440.1R (2015) simplified approach was consistently very conservative
for test specimens with FRP shear stirrups reported in this study and other data available in
the literature. The reason for this is the high level of conservatism of the concrete-
contribution (vc) in ACI 440.1R (2015) (Eq. 6).
• The proposed design provisions provide a step forward for engineers in designing two-way
FRPRC slabs with FRP stirrups. Nevertheless, more experimental results under eccentric
punching shear for interior and edge slab–column connections are urgently required.
4.8. Acknowledgments
The authors wish to acknowledge the financial support of the Tier 1 Canada Research Chair in
Advanced Composite Materials for Civil Structures, Natural Sciences and Engineering Research
Council of Canada (NSERC Industrial Research Chair in Innovative FRP Reinforcement for
Sustainable Concrete Infrastructure), and the Fonds de recherché du Québec – Nature et
Technologies – (FRQ-NT). The assistance of the technical staff of the Structural and Materials
Laboratory in the Department of Civil Engineering at the University of Sherbrooke is also
greatly appreciated.
95
4.9. List of Symbols
d = effective slab depth
db = bar diameter
bo;0.5d = critical perimeter at a distance of 0.5d from the column face
c = distance from the centroid of the critical section to the face of the critical
section (mm)
Ef = modulus of elasticity of FRP bars
Efv = modulus of elasticity of FRP stirrups, straight portion
Es = modulus of elasticity of steel
ftˊ
= split-cylinder tensile strength of concrete fcˊ = concrete-cylinder compressive strength
ffu = ultimate tensile strength of FRP bars
ffv = ultimate tensile strength of the straight portion of FRP stirrups
ffvb = ultimate tensile strength of FRP stirrups at bend location
J = deformability factor
Jc = polar moment of inertia of critical section
Mcr = cracking unbalanced moment at column centroid
Mu = ultimate unbalanced moment at column centroid
Mo = ultimate unbalanced moment at centroid of the critical shear section
nf = modular ratio (Ef/Ec)
ns = numbers of stirrups at a perimeter of 0.5d from the column face
rb = radius of the bend
sfv = stirrup spacing
Vcr = first radial cracking load
Vu = ultimate vertical shear force at column centroid
Vu = ultimate punching-shear load
vu. = ultimate shear stress at 0.5d from column face
βc = ratio of long side to short side of column
γv = fraction of unbalanced moment transferred by eccentricity of shear at slab–
column connection
96 Chapter 4: Effectiveness of GFRP Stirrups as Shear Reinforcement in GFRP RC
ΔVu = ultimate deflection at peak load
εfv = limiting tensile strain in FRP stirrups
Afv = cross-sectional area of the FRP shear reinforcement at a perimeter of 0.5d from
column face
ρb = average bottom flexural-reinforcement ratio
ρt = average top flexural-reinforcement ratio
ρfv = shear-reinforcement ratio at a perimeter of 0.5d from column face = (ns*Afv/Sfv
bo)
97
CHAPTER 5
ARTICLE 2: BEHAVIOR OF CONCRETE EDGE
COLUMN-SLAB CONNECTIONS REINFORCED
WITH GFRP BARS SUBJECTED TO DIFFERENT
MOMENT-TO-SHEAR FORCE RATIOS
Foreword
Authors and Affiliation
o Ahmed E. Salama: PhD Candidate, Department of Civil Engineering, University of
Sherbrooke, Quebec, Canada J1K 2R1, E-mail: [email protected]
o Mohamed Hassan: Postdoctoral Fellow, Department of Civil Engineering, University of
Sherbrooke, Quebec, Canada J1K 2R1, E-mail: [email protected].
o Brahim Benmokrane: Professor of Civil Engineering and NSERC and Tier-1 Canada
Research Chair Professor, Department of Civil Engineering, University of Sherbrooke,
Sherbrooke, Quebec, Canada, J1K 2R1, Tel.: 1-819-821-7758.
Corresponding author, E-mail: [email protected].
Paper submitted to Composite for Construction Journal, ASCE on January 27, 2019
Paper status: Reviewed and revised manuscript submitted on July 17, 2019
Reference: Salama , A. E. , Hassan, M., and Benmokrane, B., 2019, “ Behavior of Concrete
Edge Column-Slab Connections Reinforced with GFRP Bars Subjected to Different
Moment-to-Shear Force Ratios,” Composite for Construction Journal, ASCE.
98 Chapter 5: Behavior of Concrete Edge Column-Slab Connections Reinforced
Abstract
Applications of glass fiber-reinforced-polymer (GFRP) bars as reinforcement for concrete
structures have been growing in recent years. This paper presents test results from an
experimental program conducted to study the punching-shear response of normal-strength
concrete (NSC) and high strength concrete (HSC) edge column-slab connections. Five full-scale
reinforced concrete (RC) edge slab–column connections and tested under vertical shear force
and unbalanced moment until failure. Four of the five connections were reinforced with GFRP
bars as flexural reinforcement; one connection was reinforced with steel bars for comparison.
All of the slabs had identical geometries of 2500 × 1350 × 200 mm with a 300 mm square
column stub protruding 700 mm above and below the slab surfaces. The test parameters were:
(1) flexural-reinforcement type (steel and GFRP bars); (2) concrete strength (NSC and HSC);
and (3) moment-to-shear force ratio (M/V) (0.3 m or 0.6 m). The test results revealed that all
the connections failed by punching shear with no signs of concrete crushing. The HSC directly
enhanced the punching-shear capacity, load–deflection response, and initial stiffness of the
connections. These connections also evidenced fewer and narrower cracks compared to their
counterparts cast with NSC. Increasing the M/V ratio produced significant shear stresses,
thereby reducing the vertical load capacity by 31% and 30% for the NSC and HSC connections,
respectively. The measured punching shear capacities of the tested connections were compared
with the predictions using the available design provisions in Canada, the United States, and
Japan.
keywords: Punching shear; fiber-reinforced polymer; edge column-slab connections; high-
strength concrete; two-way slabs; moment-to-shear force ratio; shear-strength prediction.
99
5.1. Introduction
Glass fiber-reinforced-polymer (GFRP) reinforcing bars have recently gained wide acceptance
as a viable construction material for sustainable new construction. The corrosion resistance of
GFRP bars is a significant benefit for structures in highly corrosive environments such as
parking garages maintained with deicing salts. Steel-reinforced-concrete flat-plate parking
structures in North America are susceptible to accelerated deterioration given the harsh exposure
conditions to which they are subject, including freeze–thaw cycles, wet–dry cycles, and
diffusion of deicing salts. The latter specifically increase the vulnerability of steel bars to
electrochemical corrosion (El-Gendy et al. 2014 and El-gabbas et al. 2016). Moreover, the
increased punching-shear stresses around the column resulting from vertical shear forces or
vertical shear forces combined with unbalanced moments transferred between the slab and
column cause a type of local brittle failure around the column known as punching-shear failure.
This failure is exacerbated in the case of edge column-slab connections due to the unbalanced
moment, which produces more shear stresses, minimizing connection strength and ductility.
Replacing steel with FRP bars can eliminate the corrosion of steel reinforcement, reduce
maintenance costs, and improve the life-cycle cost-effectiveness of structures (Benmokrane et
al. 2012; Ahmed et al. 2017; Hassan et al. 2017).
Past research data has focused mostly on interior connections reinforced solely with FRP bars
subjected to concentric loading alone or a combination of unbalanced moment and shear (El-
Ghandour et al. 2003; Ospina et al. 2003; Lee et al. 2009; Nguyen-Minh and Rovank 2013;
Dulude et al. 2013; Hassan et al. 2013 a,b ; Hassan et al. 2014 a, b, Gouda and El-Salakawy
2015, 2016; Hassan et al. 2017; Hussein and El-Salakawy 2018). Using HSC for interor
connections increased the punching-shear capacity and the initial stiffness compared to NSC,
however, it had little effect on the post-cracking stiffness (Zhang et al. 2005; Hassan et al. 2013;
Gouda and El-Salakawy 2015; Hussein and El-Salakawy 2018). In contrast, increasing M/V
ratio decreased the punching-shear capacity and increased the strains in the reinforcing bars
(Zaghloul 2002; Gouda and El-Salakawy 2016). To date, very limited research has been
conducted on edge slab-column connections reinforced with FRP bars/grids (Zaghloul 2007; El
Gendy and El-Salakawy 2016 , 2018 ; Mostafa and El-Salakawy 2018). El-Gendy and El-
Salakawy (2016) investigated the effect of different M/V ratios on the punching-shear behavior
100 Chapter 5: Behavior of Concrete Edge Column-Slab Connections Reinforced
of GFRP-reinforced edge column-slab connections with NSC. Three full-scale connections were
tested with M/V ratios of 0.2, 0.4, and 0.6 m. They concluded that increasing the M/V ratio
significantly decreased the deformability and shear-force capacity of the connections. Recently,
El Gendy and El-Salakawy (2018) investigated the effect of flexural-reinforcement type (steel
and sand coated) on punching shear capacity of edge column-slab connections having the same
reinforcement ratios. The authors reported that the flexural-reinforcement type had a significant
effect on the punching-shear capacity and post-cracking stiffness of the connections. The
punching-shear capacity and the post-cracking stiffness of the steel connection were increased
by 35% and 200% compared to its counterpart reinforced with same amount of GFRP bars due
to the higher axial reinforcement stiffness of the steel bars.
The use of HSC for construction has been growing in recent years. HSC has higher compressive
and tensile strengths and a higher modulus of elasticity than NSC. Consequently, HSC can
improve punching capacity, allowing greater forces to be transferred through the slab–column
connection. To the authors’ best knowledge, no research has been conducted on the effect of
different M/V ratios on GFRP-reinforced edge column-slab connections constructed with HSC.
In addition, only three HSC edge connections reinforced with GFRP bars have been reported in
the literature (Mostafa and El-Salakawy 2018).They concluded that the use of HSC enhanced
the uncracked stiffness and punching-shear capacity. Doubling the concrete strength from 40 to
80 MPa resulted in an 83% and 10% increase in the uncracked stiffness and ultimate capacity,
respectively, compared to their NSC counterparts. Moreover, ACI 440.1R-15 (ACI 2015) and
CSA S806-12 (CSA 2012) have provided design provisions to calculate the punching-shear
strength of FRP-RC column-slab connections regardless of the type of loading applied to the
connections. These provisions have provided reasonable predictions for edge and interior slab–
column connections subjected to combined vertical shear force and unbalanced moment (El-
Gendy and El-Salakawy 2016, 2018; Gouda and El-Salakawy 2015, 2016; Hussein and El-
Salakawy 2018; Mostafa and El-Salakawy 2018).
The work presented in this paper extends an extensive research project conducted at the
University of Sherbrooke (Quebec, Canada) to develop and implement GFRP bars for two-way
slabs for parking garages and buildings. The first phase of this research program has been
completed (Dulude et al. 2013; Hassan et al. 2013 & 2014 a, b; Hassan et al. 2017). A total of
101
40 GFRPRC slabs were tested under concentric loading. The test results and findings
contributed to the assessment of the first punching-shear equation in CSA S806-12 (CSA 2012).
It also contributed to field implementation of GFRP bars in flat-slab parking structures in a
demonstration area (350 m2) at city-hall parking garage (Quebec, Canada, 2010) and helped in
designing the world’s first flat-slab parking garage totally reinforced with GFRP bars (La
Chancelière parking garage, Quebec City, Canada, 2011) (Benmokrane et al. 2012 and Ahmed
et al. 2017).
This paper presents experimental tests on GFRP-reinforced edge slab–column connections with
the aim of investigating the influence of the reinforcement type, concrete strength, and M/V ratio
on punching-shear strength. Detailed measurements of the deflections, slab–column rotation,
concrete strains, and flexural-reinforcement strains facilitate a better understanding of the
behavior of GFRP-reinforced edge slab–column connections. The punching-shear capacities of
the test connections were predicted by ACI 440.1R-15 (ACI 2015), CSA S806-12 (CSA 2012)
and JSCE-97 (JSCE 1997). The findings of this research will support the work of North
American technical committees engaged in developing standards and design provisions for
GFRP-RC edge slab–column connections made with normal- and high-strength concrete
subjected to different M/V ratios.
5.2. Experimental Program
5.2.1. Material Properties
Reinforcing bars. Two types of reinforcing bars were used as flexural reinforcement in this
study: sand-coated GFRP and deformed steel bars. Sand-coated Grade II and III GFRP bars
compliant with CSA S807-15 (CSA 2015), were used in all the GFRP-reinforced connections.
The GFRP straight bars were manufactured by combining the pultrusion process with an inline
sand-coating process for the bar surface to improve bonding between the GFRP bars and
surrounding concrete (Pultrall, 2016). It should be noted that the straight portions of the GFRP
bent bars were manufactured by pultrusion, whereas the bent portions were manufactured with
a unique fabrication method (Pultrall, 2016). The bottom flexural-reinforcement bars were bent
and straight No. 20 GFRP bars in the direction perpendicular and parallel to the free edge,
respectively. The bent GFRP bars were manufactured with bent ends to provide enough
102 Chapter 5: Behavior of Concrete Edge Column-Slab Connections Reinforced
anchorage close to the edges. Straight No. 15 GFRP bars were used as top flexural reinforcement
in both orthogonal directions. The tensile properties of the straight and bent GFRP bars were
determined by testing five representative specimens according to ASTM D7205-11 (ASTM
2011) and the B.5 test method in ACI 440.3R-12 (ACI 2012), respectively. Deformed 15M and
20M (Type 44W) steel bars were used as top and bottom reinforcement in the reference slab.
The column stub was reinforced with 25M and 10M steel bars as longitudinal and transverse
reinforcement, respectively. The steel-bar properties were provided by the manufacturer. Table
5.1 summarizes the mechanical properties of the reinforcing bars. Figure 5.1 shows a typical
assembled slab cage, GFRP materials, and column reinforcement.
Concrete. All connections were cast with ready-mixed NSC and HSC with target compressive
strengths of 35 and 70 MPa, respectively. The slab and column stub were cast monolithically to
ensure the same material properties for the connection. The concrete compressive strength (fc')
and tensile splitting strength (ft’) for each connection were determined by testing three 100 x
200 mm concrete cylinders on the day of testing. Table 5.2 lists the average concrete
compressive strength on the day of testing for each connection.
Table 5.1– Tensile Properties of the Reinforcing Bars
Bar Designation
Nominal
Cross-
Sectional
Area a
(mm2)
Immersed
Cross-
Sectional
Area,
(mm2)
Ultimate Tensile
Strength b
(MPa)
Tensile
Modulus of
Elasticity c
(GPa)
Ultimate Tensile
Strain
(%)
Straight flexural GFRP bars
No. 15 GFRP bar 199 240 1323 ±12 64.8±0.5 2.04 ±0.05
No. 20 GFRP bar 285 333 1334 ±85 64.9±0.6 2.06 ±0.13
Bent flexural GFRP bars
No. 20 straight portion 285 331
1210±63 53.0±0.48 2.28±0.15
No. 20 bent portion ffvb = 490±44 ------ ------
Steel bars
10M 100 ------ fy = 420 200 ɛy = 0.21
15M 200 ------ fy = 440 198 ɛy = 0.22
20M 300 ------ fy = 460 200 ɛy = 0.23
25M 500 ------ fy = 470 204 ɛy = 0.23 a according to CSA S807-15 (CSA 2015). b and c calculated using nominal cross-sectional areas of the reinforcing bars.
ffvb = ultimate tensile bend strength obtained from the B.5 test method according to ACI 440.3R-12 (ACI 2012)
fy = steel yielding strength, εy = steel yielding strain.
103
Figure 5.1– GFRP bars, connection reinforcement cage, and column-reinforcement details
5.2.2. Test Matrix and Parameters
A total of five full-scale edge slab–column connections were designed, constructed, and tested
up to failure under combined monotonic static vertical load and unbalanced moment. Four
connections (G-N-0.3, G-H-0.3, G-N-0.6, and G-H-0.6) were reinforced with GFRP bars and
one connection was reinforced with steel bars (S-N-0.3) for comparison. The test specimens
represented edge connections in a prototype of flat-plate parking structure with 5 × 5 m2 panels.
The building was assumed to have a live service load of 2.40 kN/m2, a superimposed dead load
of 1.0 kN/m2, and a self-weight of 4.80 kN/m2. The total ultimate factored loads on the floor,
including the slab weight, were estimated according to the NBCC (2015). The GFRP-RC
connections were designed in accordance with Canadian standards CSA S806-12 (CSA 2012)
and CSA A23.3-14 (CSA 2014). The flexural reinforcement ratio of the steel-RC connection
was, however, chosen to be similar to that of the GFRP-RC connections. Each connection was
simply supported on three edges, simulating lines of contra flexure in the prototype floor and
monolithic with a column at the middle of the fourth edge. The lines of contra flexure were
assumed to be 0.2L from the column centerlines, where L is the span between column
centerlines. All slabs had identical geometries of 2500 × 1350 × 200 mm with a 300 mm square
column stub protruding 700 mm above and below the slab surfaces. The slabs were simply
supported on a 2000 × 1150 mm perimeter on the bottom face of the slab. The nominal concrete
(c) Assembled slab cage
Column reinforcement (a)
(b) GFRP bars
No.20 Bent bars
No.15 Straight bars
No. 20 straight bars
104 Chapter 5: Behavior of Concrete Edge Column-Slab Connections Reinforced
cover on both the top and bottom faces of the slabs was 21 mm. Figure 5.2 shows the typical
geometry and reinforcement details of the test connections.
Figure 5.2 – Connections concrete dimensions and reinforcement configuration
Y
Y
Straight bars
bars
GFRP No. 20
27
3
5@
17
5
4@218 170
1350
25
00
11
88
GFRP No. 20
Bent bars
X X
12
4
Y
Y
Straight bars
bars
GFRP No. 15
27
3
35
0
2@436 170
1350
25
00
11
88
GFRP No. 15
Bent bars
X X
12
4
52
5
300 1050
16
00
700
20
0
6@
10
0
GFRP No.15
6-25M
10M stirrups
GFRP No. 20
16
0
150 1100
GFRP No.15
GFRP No. 20
20
0
Sym.
Axis
40
40
90 90 130 88 130 88
a) Bottom mesh configuration b) Top mesh configuration
d) Sec. (Y-Y) Unit: mm c) Sec. (X-X)
300 225 150
75
300 225 150
75
105
Table 5.2 – Details of Test Connections
Connection RFT
Type
dx,
mm
dy,
mm
Flexural Reinforcement M/V
m
fc'
MPa
ft'
MPa Tension (bottom) Compression
(top)
Ratio,%
ρb ρt
S-N-0.3 Steel 169.0 149.0 7 -20M/14 -20M 5 -15M/ 8-15M 1.09 0.34 0.3 39.2 3.73
G-N-0.3 GFRP 169.5 150.5 7 No.20/14 No.20 5 No.15/ 8 No.15 1.04 0.34 0.3 37.1 3.73
G-H-0.3 GFRP 169.5 150.5 7 No.20/14 No.20 5 No.15/ 8 No.15 1.04 0.34 0.3 85.8 6.54
G-N-0.6 GFRP 169.5 150.5 7 No.20/14 No.20 5 No.15/ 8 No.15 1.04 0.34 0.6 38.8 3.56
G-H-0.6 GFRP 169.5 150.5 7 No.20/14 No.20 5 No.15/ 8 No.15 1.04 0.34 0.6 86.0 6.54
dx, dy = effective slab depths in the x and y directions; dx=t ˗ 0.5db ˗21; dy= t ˗ 1.5 db ˗21; ρb, ρt = average tensile and
compression flexural reinforcement ratios within effective widths, respectively; M/V= moment-to-shear force ratio; fc' =
concrete compressive strength and ft'= tensile splitting strength.
The test matrix was designed to investigate the effects of the reinforcement type (steel and
GFRP), concrete strength (NSC and HSC); and varied M/V ratios (0.3 m and 0.6 m) on the
punching behavior and strength of edge-slab connections. All of the slabs had an identical
number of bars on the tension and compression sides (bottom and top). The bottom and top
meshes consisted of 20M or No. 20 (#20) and 15M or No. 15 (#15) steel or GFRP bars,
respectively. It should be mentioned that two bars were passing through the column core to
satisfy the requirement for structural integrity reinforcement in CSA A23.3-14 (CSA 2014). The
average bottom reinforcement ratios were 1.09% and 1.04% for the steel and GFRP connections,
respectively. Table 2 presents the test matrix and characteristics for each connection. The test
matrix consisted of five slabs, four GFRPRC connections (G-N-0.3, G-H-0.3, G-N-0.6, and G-
H-0.6) were constructed using NSC and HSC and tested under M/V ratios of 0.30 m or 0.6 m,
while the remaining slab (S-N-0.3) was reinforced with steel bars and served as a reference for
comparison. The connections were labelled with letters denoting the reinforcement type (G or
S for GFRP or steel bars) and concrete type (N for NSC and H for HSC), followed by the M/V
value (0.3 or 0.6). The column stub was reinforced with six 25M steel bars as longitudinal
reinforcement and 10M transverse steel stirrups spaced at 100 mm. The chosen configuration
satisfactorily avoids the premature failure of the column stub in steel-RC edge connections
during testing (Megally and Ghali 2000).
106 Chapter 5: Behavior of Concrete Edge Column-Slab Connections Reinforced
5.2.3 Test Setup and Procedure
All of the connections were tested in the structural laboratory at the University of Sherbrooke
under combined vertical shear force (V) and unbalanced moment (Mun) until failure. Figure 5.3
shows the test setup and schematic. Vertical shear force was simulated by vertically applying a
downward load through the column with a 1500 kN hydraulic jack, which was installed in the
middle of a rigid steel I-beam supported on two steel portal frames. To facilitate free horizontal
movement of the column during lateral loading, a steel pan with rollers was placed between the
vertical jack and the top of the upper concrete column. Two 1000 kN horizontal hydraulic jacks
were installed on two very rigid reaction frames firmly fastened to the laboratory strong floor to
apply lateral loads. The vertical and lateral jacks were controlled with three manual hydraulic
pumps. The loads were monitored with three load cells on each pump and connected to the data-
acquisition system. The connections were simply supported on the bottom surface along three
sides during testing with the fabricated supporting steel bed. The bottom supporting frame was
braced with eight double angles back to back and prestressed to the laboratory floor with four
38 mm diameter steel tie rods to avoid any lateral movement. On the slab top face, three
supported edges were restrained by steel reaction beams to prevent slab lifting. To simulate slab
rotation at the lines of contra flexure during the entire test, neoprene bearing pads 20 mm thick
and 100 mm wide were placed between the slab and supporting bed and between the slab and
top restraining beams along the support lines.
The connections were tested under two different M/V ratios of 0.3 and 0.6 m. The unbalanced
moments were calculated by multiplying the two lateral forces applied to each column by the
distance from the application point to the center of the slab: 675 mm. The vertical load was
applied monotonically at a load-controlled rate of 5 kN/min, whereas the horizontal forces were
simultaneously applied with the vertical force in small increments to maintain a constant M/V
ratio of 0.3 or 0.6 m throughout the test until failure.
107
Figure 5.3 –Test setup and schematic
Collar
DAQ
Vertical jack
Roller Plate
Horizontal frame
Lateral hydraulic jack
Stiff connecting steel I-beam Main steel frame Main steel frame
Roller plate Steel post
Test connection Horizontal frame
Horizontal frame
Lateral hydraulic jack
Neoprene pads Supporting bed
Top frame
Collar
(b) Schematic drawing
(a) Test setup photo
Stiff connecting steel I-beam
Supporting bed
Top frame
108 Chapter 5: Behavior of Concrete Edge Column-Slab Connections Reinforced
5.2.4 Instrumentation
Extensive instrumentation was used to help understand connection behavior. A total of 11
electrical strain gauges were mounted on the bottom flexural-reinforcement bars in both
orthogonal directions at different positions to monitor the strains during loading. Figure 5.1
shows the different locations of the attached strain gauges on the two selected tension bars from
the column face in each direction. Moreover, five concrete electrical resistance strain gauges
(C1 to C5) were mounted close to the column face to measure concrete strain on the slab
compression side, as shown in Fig. 5.4. A series of linear potentiometers (LPOTs) were mounted
to measure slab deflections and column lateral displacements. Slab deflections were monitored
with 14 vertical LPOTs at different locations along the column centerlines in both orthogonal
directions (Fig. 5.4). Two LPOTs were mounted horizontally at the tips of the upper and lower
column stubs to measure the horizontal column displacement. To monitor any possible shifting
of the connection or test setup, two LPOTs were installed in the horizontal-loading directions at
the center of slab thickness and frame-test setup. All instruments were installed on rigid steel
frames, separated from the testing frame and attached directly to the laboratory floor to prevent
any frame deformations from affecting the measurements. The strain gauges and POTS were
connected to a data-acquisition system to record the readings. During the test, crack propagation
was marked, and the corresponding loads recorded. Figure 5.4 shows the different positions of
the linear potentiometers.
109
Figure 5.4 – Instrumentations (Note: All dimensions in mm)
5.3. Test Results and Observations
5.3.1. Cracking and Mode of Failure
During the test, flexural cracks appeared first on the slab tension side. The loads corresponding
to the appearance of the first crack (cracking load Vcr and unbalanced moment Mcr) as well as
the corresponding deflections (Δcr) were recorded in Table 5.3. The first flexural crack began to
appear at vertical loads from 37.9 to 45.4 kN and from 65.9 to 73.5 kN for the NSC and HSC
connections, respectively. These radial flexural cracks originated in the inner slab–column
interface and propagated towards the supports. Inclined torsion cracks formed at the inner
corners of the columns at about 35° from the slab edge. These cracks started to appear at about
25 % of the ultimate loads, then propagated upward the slab edge to half of the slab depth at
approximately 50% of the ultimate loads. Thereafter, circumferential (tangential) cracks
generated around the column and crossed over the radial cracks at higher loads, while the torsion
cracks continued their way to the compression face of the slab. As the loads increased, the
number of such cracks and their widths in the column vicinity increased. Shear cracks initiated
on the slab tension side and propagated towards the compression side of the slab until failure
occurred. All connections failed abruptly. At failure, a major tangential crack was intercepted
by the flexural cracks in an approximately perpendicular manner, forming the punching cone.
675 675
P1
P2
P3
P5
P4
∆1 ∆2
P16
P15 Column
150 300 300
C2
C1 C3
C4
170
P10 P6
Concrete gauges
80
170
300
300
P1
P2
P3
P4
P7 P8 P9 P11 P12 P13 P14
150 P5
80
C5
200
200
Potentiometers
Column
P17
(a) Plan (a) Elevation Unit: mm
Slab Slab
110 Chapter 5: Behavior of Concrete Edge Column-Slab Connections Reinforced
In all of the slabs, some cracks developed on the compression faces at approximately 60% to
70% of the ultimate failure load. Figure 5.5 shows the typical cracks in the column vicinity on
the tension and compression sides of some tested connections.
Regardless of the reinforcement type, the final mode of failure for all of the connections was
punching shear without any signs of concrete crushing. This failure was characterized by an
immediate drop in the ultimate load, accompanied by the appearance of a clear crack defining
the failure surface. It should be noted that the punching-shear failure occurred in the steel
connection initiated as yielding of steel bars. The induced yielding in the steel bars widened the
shear cracks, which decreased the contribution of the aggregate interlock to the shear strength.
All connections displayed similar crack patterns on the tension surface regardless reinforcement
type and concrete strength on the tension side. Increasing the M/V ratio to 0.6, however,
decreased the number of cracks at failure on the tension side of the GFRP connections,
regardless of the concrete strength. That can be attributed to the increase in shear stresses applied
to shear critical section, which accelerated the incidence of punching-shear failure before the
formation of the significant flexural cracks. El-Gendy and El-Salakawy (2016) made the same
observation based on testing NSC connections under different M/V ratios. On the other hand,
The HSC connections evidenced narrower cracks as well as considerable splitting of the
concrete cover, however, once punching failure occurred. This behavior is similar to that
observed in steel- and FRP-reinforced-concrete connections (Marzouk et al. 1998 and Mostafa
et al. 2018).
To examine the development of the inner diagonal cracks through the slab thickness, some tested
connections were sawed through a line perpendicular to the free edge and adjacent to the
column. Table 5.3 and Figure 5.6 illustrate the inclination angle of the punching cone of the
tested connections. Figure 5.6 shows that the sawn connections had a main diagonal shear crack
starting at the column face and extending to the slab tension side at different inclination angles
(αcone), where αcone is the average angle for the critical shear crack with the slab tension side.
The inclination angle of the critical shear crack (αcone) was significantly affected by the M/V
ratio rather than concrete compressive strength.
An increase in the M/V ratio from 0.3 to 0.6 for NSC and HSC connections resulted in a slightly
steeper shear crack. It can be also observed that the direction of the cracks at the free edge was
111
consistent with the direction of the punching force, particularly when the M/V ratio was small
(i.e. G-H-0.3). The inclined cracks at the free edge, however, ran in the direction opposite to the
punching-shear force as a result of the high unbalanced moment, which produced reversed shear
stresses in the direction opposite to that caused by the vertical shear force (Fig. 5.6b). This
behavior is similar to that observed in steel-reinforced-concrete edge connections (El-Salakawy
et al. 1998, 2000). On the other hand, the inclined shear crack at failure was not significantly
influenced by the reinforcement type or concrete strength.
5.3.2. Vertical Load-Deflection Behavior
Figure 5.7 provides the applied vertical load versus deflection relationships for the tested
connections at 80 mm from the column faces along column centerlines in the perpendicular
direction to the free edge. All of the connections show a typical bilinear load–deflection
response in both orthogonal directions. The first line represents the pre-cracking stiffness, ki,
calculated as the slope of the load–deflection curve before cracking, whereas the second line
illustrates the post-cracking stiffness , kp, calculated as the slope of the load–deflection curve
after cracking. The sudden drop in the applied vertical load in all tested connections after
reaching their maximum capacities confirmed the occurrence of punching-shear failure. As seen
in Fig. 5.7, the load–deflection relationships and connection stiffness were significantly affected
by the test parameters. GFRP-reinforced connection G-N-0.3 exhibited higher deflection values
than of its steel-reinforced counterpart S-N-0.3 at the same load level. The ultimate deflection
of connection G-N-0.3 was 79% higher than connection S-N-0.3. This can be attributed to the
GFRP bars having a lower modulus of elasticity than the steel bars (approximately Ef = 0.25
Es).
Using HSC directly enhanced the uncracked stiffness, ki, of the tested connections as evidenced
in Fig. 5.7b. The pre-cracking stiffness , ki , of G-H-0.3 and G-H-0.6 (HSC) was 103.7 and 101.3
kN/mm, compared to 80.9 and 78.5 kN/mm, respectively, for G-N-0.3 and G-N-0.6. The pre-
cracking stiffness, ki, increased by 29% (on average) in connections G-H-0.3 and G-H-0.6
compared to their counterparts G-N-0.3 and G-N-0.6. The post-cracking stiffness , kp, of the
NSC and HSC connections did not, however, change significantly after cracking. Furthermore,
the ultimate deflection of the HSC connections was 15.5% (on average) higher than that of the
112 Chapter 5: Behavior of Concrete Edge Column-Slab Connections Reinforced
NSC connections. This indicates that using the HSC in the GFRP-reinforced slabs enhanced the
overall response of the test connections and made it possible to achieve significantly higher
deflections at failure (Hassan et al 2013). Increasing the M/V ratio from 0.3 to 0.6 had a
significant impact on the overall performance as well as the ultimate deflection for all of the
GFRP connections. The ultimate deflections for connections G-N-0.6 and G-H-0.6 were 47%
and 46% lower than that of their counterparts G-N-0.3 and G-H-0.3, respectively.
5.3.3. Moment–Rotation Relationships
Figure 5.8 gives the applied unbalanced moment versus column rotation relationships for all
tested connections. The column rotation was calculated as the ratio of the sum of measured
displacements at the column ends by means of potentiometers P12 and P16 to the distance
between the two loading rams (see Fig. 5.4). The ultimate rotations for connections S-N-0.3, G-
N-0.3, G-H-0.3, G-N-0.6, and G-H-0.6 were 0.027, 0.0188, 0.0223, 0.0233, and 0.029 radians,
respectively. As seen in Fig. 5.8, the measured rotations of the columns at failure increased with
as the M/V ratio increased, regardless of the concrete strength. For instance, the rotation
capacities increased by 19% and 25% for connections G-N-0.6 and G-H-0.6 compared to
connections G-N-0.3 and G-H-0.3, respectively. The ultimate moment increased by 35% and
40 % for connections G-N-0.6 and G-H-0.6 compared to connections G-N-0.3 and G-H-0.3,
respectively. On the other hand, using HSC significantly increased the rotation capacities in
connections G-H-0.3 and G-H-0.6 by 24% and 30% compared to their NSC counterparts G-N-
0.3 and G-N-0.6, respectively. It is the worth mentioning that the comparison with steel
connection S-N-0.3 was not possible because the mounted lateral LPOTs stopped reading before
failure.
113
Figure 5.5 – Cracking patterns and punching-shear failure surface for the tested connections
S-N-0.3 S-N-0.3
G-N-0.3 G-N-0.3
G-H-0.3 G-H-0.3
G-N-0.6
G-H-0.6 G-H-0.6
Tension Side
Tension Side
Tension Side
nsion SideTe
ession SideCompr
Compression Side
Compression Side
Compression Side
Compression Side
` G-N-0.6
Tension Side
114 Chapter 5: Behavior of Concrete Edge Column-Slab Connections Reinforced
Figure 5.6 – Shear cracks progression along the sawed sections and the free edge
Figure 5.7 – Vertical load–deflection relationships
G-N-0.6 G-H-0.3 G-H-0.6
G-H-0.3
G-H-0.6
(a) Shear cracks and failure envelope of the sawed connections
(b) Typical shear cracks along the free edge
a) In the Perpendicular direction to the free edge b) Pre-cracking stiffness for connections G-N-0.3,
G-H-0.3, G-N-0.6,G-H-0.6
@80 mm
115
Table 5.3 – Summary of Test Results
Connection Vcr,
kN
Mcr,
kN.m
Δcr,
mm
Vu test,
kN
Mu test,
kN.m
Δvu,
mm
vu test,
MPa
ki,
kN/mm
,pk
kN/mm
αcone
degrees
ɛr max, (μm/m) ɛc max
(μm/m) ┴ a // a
S-N-0.3 45 12 0.36 359 106 15 2.7 112.4 20.6 ̶ 3393 2683 -796
G-N-0.3 40 11 0.55 260 79 26 2.0 80.9 7.7 ̶ 7570 5208 -1302
G-H-0.3 73 22 0.78 306 92 30 2.3 103.7 8.1 21.0 8381 6246 -775
G-N-0.6 38 24 0.44 178 107 13 2.1 78.5 7.9 26.0 8248 4267 -1133
G-H-0.6 66 40 0.89 213 129 15 2.5 101.3 8.0 25.4 8876 4678 -817 a Position perpendicular (┴) or parallel (//) to the free edge
Vcr = cracking vertical shear force at column centroid; Mcr = cracking unbalanced moment at column centroid; Δcr = deflection
corresponding to cracking load; Vu test = ultimate vertical shear force at column centroid; Mu test = ultimate unbalanced moment at the at
column centroid; Δvu = deflection corresponding to ultimate loads; ki = pre-cracking stiffness; kp = post-cracking stiffness; αcone = actual
punching-shear-angle cone in the horizontal direction; ɛr max = ultimate measured reinforcement strain; ɛc max = ultimate measured
concrete strain.
116 Chapter 5: Behavior of Concrete Edge Column-Slab Connections Reinforced
Figure 5.8 – Moment–rotation relationships
5.3.4. Strains in Flexural Reinforcement and Concrete
The applied vertical load versus the maximum flexural reinforcement and concrete strains for
all of the connections have been graphed in Fig. 5.9. The reinforcement strains for each
connection were recorded at 75 mm from the column faces perpendicular and parallel to the free
edge, while the maximum concrete strain was measured at the column face by gauge C1 (Fig.
5.4). Table 5.3 reports the maximum reinforcement and concrete strains. Connection S-N-0.3,
reinforced with steel bars, exhibited no signs of yielding before the occurrence of punching-shear
failure. On the other hand, the maximum reinforcement strain in the GFRP-reinforced
connections were 7570, 8381, 8248, 8876 µm/m, representing 40%, 44, 43%, and 46% of the
guaranteed ultimate tensile strength for connections G-N-0.3, G-N-0.6, G-H-0.3, and G-H-0.6,
respectively. Furthermore, the maximum measured concrete strains at the column face were
below the specified concrete crushing strains of 3500 and 3000 µm/m according to CSA S806-
12 (CSA 2012) and ACI 440.1R-15 (ACI 2015), respectively. The attained reinforcement and
concrete-strain values were consistent with the incidence of the punching failure, without
concrete crushing, on the compression zone or GFRP-reinforcement rupture.
Figures 5.10 and 5.11 show the reinforcement-strain distribution along the selected tension
reinforcing bars at different loading stages in the perpendicular and parallel directions to the
free edge, respectively. As expected, the tension-reinforcement strains in the column vicinity
117
were high owing to the combined shear stresses resulting from the vertical shear force and the
unbalanced moment. These strains were lower away from the column vicinity toward the
supported slab edge until reaching very low strain values at 750 mm from the column face in
both orthogonal directions. This implies that the sand-coated GFRP bars adequately transferred
loads with no signs of bar slippage or bond failure during the tests. Apparently, due to the low
axial stiffness of GFRP bars, the reinforcement strains in the GFRP-reinforced connection G-
N-0.3 were higher than in its steel-reinforced counterpart S-N-0.3, although similar strain
profiles were observed until failure. This is consistent with the same observations in many
studies (Hussein et al. 2004; Hassan et al. 2013; El-Gendy and El-Salakawy 2016). On the other
hand, increasing the M/V ratio yielded higher reinforcement strains in the GFRP bars along the
perpendicular direction to the free edge than those measured strains in the GFRP bars in the
parallel direction to the free edge. In contrast, the HSC connections revealed lower concrete
strains than the NSC connections.
118 Chapter 5: Behavior of Concrete Edge Column-Slab Connections Reinforced
Figure 5.9 – Vertical load-strain relationships
a) In the perpendicular direction to the free edge b) In the parallel direction to the free edge
C) Maximum concrete strain around the column
@ column face
@ 75 mm @ 75 mm
119
Figure 5.10 – Flexural reinforcement-strain distribution in the perpendicular direction to
the free edge
S-N-0.3 G-N-0.3
G-H-0.6
G-N-0.6
G-H-0.3
120 Chapter 5: Behavior of Concrete Edge Column-Slab Connections Reinforced
S-N-0.3
G-H-0.6
G-N-0.3 G-N-0.6
G-H-0.3
Figure 5.11 – Flexural reinforcement-strain distribution in the parallel direction to the free
edge
121
5.4. Discussion
5.4.1. Influence of Reinforcement Type
The GFRP- and steel-reinforced connections with the same reinforcement ratio exhibited similar
responses in terms of crack pattern, mode of failure, and punching-shear failure surface,
regardless of reinforcement type. Table 3 reports the vertical shear force and bending moment
at ultimate and the corresponding ultimate punching-shear stress calculated at 0.5d from the
column face for the tested connection. The results in Table 3 show that the GFRP-reinforced
connection with the same reinforcement ratio as its steel-reinforced counterpart evidenced 28%
lower punching-shear stress at failure. This was related to the smaller dowel action and lower
modulus of elasticity of the GFRP reinforcing bars compared to the steel bars. Using a GFRP-
reinforcement ratio equal to the steel-reinforcement ratio yielded a smaller neutral-axis depth,
higher strains, and deeper, wider cracks at the same load level. Thus, both the contributions of
the uncracked concrete and aggregate interlock decreased, which, in turn, yielded lower
punching-shear capacity.
5.4.2. Influence of Moment-to-Shear Force Ratio (M/V)
During a lateral-load exposure or slab discontinuity, the unbalanced moment transferred
between the slabs and columns could produce significant shear stresses that increase the
likelihood of brittle failure. Regardless of the concrete strength, increasing the M/V ratio
significantly affected the slab punching-shear strength, deformation capacity, and energy
absorption for all of the NSC and HSC connections. Increasing the M/V ratio from 0.3 to 0.6
(G-N-0.3 to G-N-0.6, fabricated with NSC) yielded a 31% decrease in the ultimate capacity. A
similar was noted between the HSC connections, with G-H-0.6 showing a 30% decrease in
ultimate capacity compared to G-H-0.3. This can be attributed to the higher shear stresses due
to combined vertical shear force and high unbalanced moment. It is worth mentioning that the
M/V ratio had a comparable effect on the GFRP connections constructed with NSC and HSC.
Ozden et al. (2006) reported the same findings for interior steel-reinforced NSC and HSC
connections tested under different M/V ratios.
122 Chapter 5: Behavior of Concrete Edge Column-Slab Connections Reinforced
5.4.3. Influence of Concrete Strength
Using HSC enhanced overall slab behavior and, consequently, increased the ultimate punching-
shear capacity of the connection. The higher concrete strength helped enhance the contribution
of the compressive block above the neutral axis after cracking, which yields higher punching-
shear strength. The ultimate punching-shear strength of G-H-0.3 and G-H-0.6 was 17.6% and
19.3% higher than that of their counterparts G-N-0.3 and G-N-0.6, respectively. In comparison
to the NSC connections, the HSC connections evidenced final punching failure associated with
considerable spalling of the concrete cover in the failure area around the column. This can be
attributed to the brittleness of the HSC, which allowed the cracks to propagate through the
course aggregate particles (Gouda and El-Salakawy 2015). Furthermore, the HSC connections
recorded lower concrete strains than the NSC connections. This relates to the high tensile
strength, which delays slab cracking, and the higher modulus of elasticity helped reduce induced
strains. On the other hand, the HSC connections yielded lower strains in the GFRP bars at early
loading stages than their NSC counterparts. At higher loading stages, the induced strains were
slightly higher than that of their NSC counterparts.
5.5. Punching Shear Design Equations
The design of edge slab–column connection always includes sustainable unbalanced moment
due to the existence of gravity load, wind, earthquake, or other lateral forces in the structure.
Consequently, the factored shear stress is a combination of a vertical shear force and an
unbalanced moment transferred from the slab to the column. The maximum factored shear
stress,vu, is calculated at a distance d/2 from the column face according to the design provisions
in ACI 318-14 (ACI 2014) and CSA A23.3-14 (CSA 2014) for slabs without shear
reinforcement.
𝑣𝑢 =𝑉𝑢
𝑏𝑜; 0.5𝑑 𝑑+𝛾𝑣 𝑀𝑜
𝐽𝑐 𝑐 (5.1)
where vu = ultimate shear stress at 0.5d from the column face; bo;0.5d = critical shear perimeter
at 0.5d from the column face; γv = fraction of unbalanced moment transferred by shear
eccentricity; d = effective slab depth; Mo = ultimate unbalanced-moment centroid of the critical
123
shear section; c = distance from the centroid of the critical shear section to the face of shear
critical section; and Jc = polar moment of inertia of the critical shear section as per Eq. (5.2).
3 3
21 12
3 6c o
b d b dJ b d c= + − (5.2)
where b1 and b2 = width of the critical section for the shear measured parallel and perpendicular
to the direction of the unbalanced moment, respectively
The current design equations for FRP slabs without shear reinforcement are relatively similar to
those for steel-reinforced slabs with some modifications accounting for the mechanical
properties of FRP bars, especially the lower modulus of elasticity of FRP bars. In this section,
the punching-shear capacities of the tested edge slab–column connections were predicted using
the punching-shear equations in FRP design provisions, ACI 440.1R-15 (ACI 2015), CSA S806-
12 (CSA 2012), and JSCE-97 (JSCE 1997), as listed in Table 5.4. In addition, a recent model
proposed by Hassan et al. (2017) for estimating the punching-shear capacity of GFRP-RC
interior connections (Table 5.4) was examined for the tested GFRP-RC edge connections. The
predictions yielded by these equations were compared to the experimental results to evaluate
their accuracy in predicting the punching-shear capacity of the tested connections.
124 Chapter 5: Behavior of Concrete Edge Column-Slab Connections Reinforced
Table 5.4 – Punching Shear Design Equations
Reference Equation
JSCE-97 (JSCE 1997)
𝑣𝑐 = 𝛽𝑑 𝛽𝑝 𝛽𝑟 𝑓𝑝𝑐𝑑1
𝛾𝑏 (1a)
𝛽𝑑 = (1000/𝑑)0.25 ≤ 1.5 , (1b)
𝛽𝑝 = (100𝜌𝑓𝐸𝑓/𝐸𝑆)1
3 ≤ 1.5 , (1c)
𝛽𝑟 = 1 +1
1+0.25𝑢𝑜𝑑
, (1d)
𝑓𝑝𝑐𝑑 = 0.2√𝑓𝑐′ ≤ 1.2
(1e)
where βd = coefficient to consider the effective depth; βp = factor to consider
difference in the modulus of elasticity between FRP and steel bars; Es = modulus of
elasticity of steel; Es = modulus of elasticity of FRP bars; uo = perimeter of reaction
area of supporting column; γb = partial factor of safety equal to 1.3 or 1.5 for concrete
strengths below and above 50 MPa, respectively, which was set to 1.0 to get an
unfactored prediction of capacity; fpcd = design compressive strength of concrete
(MPa); fcˊ= concrete compressive strength (MPa); and d = effective slab depth (mm).
CAN/CSA S806-12 (2012)
The least of the following equations:
𝑣𝑐 = 0.028λ ∅𝑐 (1 +2
βc) (𝐸𝑓 𝜌𝑓 𝑓𝑐
′ )1
3
(2)
𝑣𝑐 = 0.147 λ ∅𝑐 (0.19 +αs d
bo;0.5d) (𝐸𝑓 𝜌𝑓 𝑓𝑐
′ )1
3 (3)
𝑣𝑐 = 0.056 λ ∅𝑐 (𝐸𝑓 𝜌𝑓 𝑓𝑐′ )
1
3
(4)
where βc = ratio of long side to short side of the column; ϕc = concrete resistance
factor (0.65); λ = concrete density factor (1 for normal weight); ρf = reinforcement
ratio of FRP bars; αs = factor equals 4 for interior columns, 3 for edge columns, 2
for corner columns; bo,0.5d = perimeter of critical shear section located at d/2 from
the column face (mm).
ACI 440.1R (2015)
𝑣𝑐 = 4
5 𝑘 √𝑓𝑐
′ (5)
where 𝑘 = √2𝜌𝑓 𝑛𝑓 + (𝜌𝑓 𝑛𝑓)2 − 𝜌𝑓𝑛𝑓 ; nf = ratio of modulus of elasticity of FRP
bars to modulus of elasticity of concrete (Ef / Ec); Ec = modulus of elasticity of
concrete (𝐸𝑐 = 4700 √𝑓𝑐′).
Hassan et al. (2017)
𝑣𝑐 = 0.065 λ ∅𝑐 (0.65 +4d
bo;0.5d) (𝐸𝑓 𝜌𝑓 𝑓𝑐
′ )13 (125
𝑑)
16
where (125
𝑑)
1
6 = size effect factor for column-slab connection with effective depth
greater than 300 mm.
125
5.6. Comparison Between Predicted and Test Results
Table 5.5 presents the ratio between the tested and predicted punching-shear capacity. All safety
factors and partial material factors in the equations were taken to be equal to 1.0. The punching-
shear predictions listed in Table 5 show that the punching-shear equations of JSCE-97 (JSCE
1997) and CSA S806-12 (CSA 2012) equations reasonably predicted the punching-shear
capacities of the tested connections with average of Vu test /VJSCE = 1.28 ± 0.13 and Vu test /VCSA
= 1.27 ± 0.04, respectively. These equations include the effect of FRP axial stiffness by
replacing the flexural-reinforcement ratio (ρs) with (ρf Ef /Es), which gives good predications.
However, the punching-shear design equation adopted in ACI 440.1R-15 (ACI 2015)
underestimates the punching-shear capacity with average of Vu test /VACI = 2.13 ± 0.09. The ACI
440.1R-15 (ACI 2015) equation has some shortcomings due to retaining the reinforcement ratio
only in predicting the depth of the neutral axis and dropping the FRP axial stiffness. In contrast,
the Hassan et al. equation (2017) overestimated the punching-shear capacity with average of Vu
test /VHassan = 0.88 ± 0.06. This can be attributed to the type of loading and connection, as the
Hassan et al. equation was based primarily on concentric punching-shear tests that were
conducted on interor slab–column connections.
CSA S806-12 (CSA 2012) limits the applicability of its equation to a maximum concrete
strength of 60 MPa. However, using the CSA S806-12 (CSA 2012) equations for the HSC, G-
H-0.3 and G-H-0.6 with a concrete compressive strength of 85.83 and 86 MPa, respectively,
yielded average of Vu test /VCSA = 1.19 ± 0.08. Thus, the CSA S806-12 (CSA 2012) punching-
shear equation proved to be more effective for concrete strengths higher than 60 MPa. Further
investigations are needed, however, to quantify the concrete compressive-strength limit in the
CSA S806-12 (CSA 2012) equation.
126 Chapter 5: Behavior of Concrete Edge Column-Slab Connections Reinforced
Table 5.5 – Punching Shear Capacity Prediction
5.7. Summary and Conclusion
This study assessed the performance and punching-shear strength of NSC and HSC edge slab–
column connections reinforced with GFRP bars subjected to low and high M/V ratios. Based on
the experimental results and discussion, the following conclusions were drawn:
• The tested connections experienced punching-shear failure as the final mode without any
signs of concrete crushing. This failure was characterized by an immediate drop in the
ultimate load, accompanied by the appearance of a clear crack defining the failure surface.
• Using HSC significantly enhanced the punching-shear capacity, deflection, and initial
stiffness of the GFRP-reinforced connections. The punching-shear capacity, deflection, and
initial stiffness of the HSC connections were 18.5%, 15.5%, and 29% (on average) higher
than that of the GFRP-reinforced connections constructed with NSC, respectively. The post-
cracking stiffness, however, was similar to the NSC GFRP-reinforced connections.
• Increasing the M/V ratio from 0.3 m to 0.6 m for the NSC and HSC connections resulted in
slightly steeper shear cracks. The inclined cracks at the free edge ran in opposite direction
to the punching-shear force as a result of the reversed shear stresses caused by highly
unbalanced moment.
• Increasing the M/V ratio transferred between the slabs and columns produced significant
shear stresses that increased the likelihood of brittle failure and resulted in a reduction in the
vertical-load capacity by approximately 31% and 30% for the NSC and HSC connections,
respectively.
• The JSCE-97 (JSCE 1997) and CSA S806-12 (CSA 2012) reasonably predicted the
punching capacities of the tested connections with average of Vu test /VJSCE = 1.28 ± 0.13 and
Connection Vu
(kN)
CSA S806-12
(CSA2012)
ACI 440-15
(ACI 2015)
JSCE-97
(JSCE 1997)
Hassan et al.
(2017)
VCSA
(kN)
Vu test /VCSA
VACI
(kN)
Vu test /VACI
VJSCE
(kN) Vu test /VJSCE
VHassan
(kN)
Vu test /VHassan
G-N-0.3 260 210 1.24 121 2.15 228 1.14 286 0.91
G-H-0.3 630 245 1.24 152 2.01 228 1.34 379 0.81
G-N-0.6 178 140 1.27 80 2.22 150 1.19 191 0.93
G-H-0.6 213 162 1.31 100 2.13 150 1.42 249 0.85
Average 1.27 2.13 1.28 0.88
SD 0.04 0.09 0.13 0.06
127
Vu test /VCSA = 1.27 ± 0.04, respectively. The ACI 440.1R-15 (ACI 2015) equation, however,
underestimated, giving average of Vu test /VACI = 2.13 ± 0.09. In contrast, the Hassan et al.
equation (2017) overestimated the capacity of the tested connections with an average of Vu
test /VHassan = 0.88 ± 0.06.
• Using the actual concrete strengths of 85 and 86 MPa for the HSC connections (G-H-0.3
and G-H-0.6) in the CSA S806-12 (CSA 2012) equation better estimated the ultimate
capacity (Vu test /VCSA = 1.19 ± 0.08) than using the 60 MPa concrete-strength limit as per
CSA S806-12 (CSA 2012). Further research, however, is needed with a wide range of
concrete strengths.
5.8. Acknowledgments
The authors would like to express their special thanks and gratitude to the Natural Science and
Engineering Research Council of Canada (NSERC), the NSERC Research Chair in Innovative FRP
Reinforcement for Concrete Structures, the Tier-1 Canada Research Chair in Advanced Composite
Materials for Civil Structures, the Fonds Québécois de la Recherche sur la Nature et les
Technologies (FQRNT), the Canadian Foundation for Innovation (FCI), and the technical staff of
the structural laboratory in the Department of Civil Engineering at the University of Sherbrooke.
128
CHAPTER 6
ARTICLE 3: EFFECT OF GFRP SHEAR
STIRRUPS ON THE STRENGTH OF TWO-WAY
GFRPRC EDGE SLABS: EXPERIMENTAL AND
FINITE-ELEMENT INVESTIGATIONS
Foreword
Authors and Affiliation
o Ahmed E. Salama: PhD Candidate, Department of Civil Engineering, University of
Sherbrooke, Quebec, Canada J1K 2R1, E-mail: [email protected]
o Mohamed Hassan: Postdoctoral Fellow, Department of Civil Engineering, University of
Sherbrooke, Quebec, Canada J1K 2R1, E-mail: [email protected].
o Brahim Benmokrane: Professor of Civil Engineering and NSERC and Tier-1 Canada
Research Chair Professor, Department of Civil Engineering, University of Sherbrooke,
Sherbrooke, Quebec, Canada, J1K 2R1, Tel.: 1-819-821-7758.
Corresponding author, E-mail: [email protected].
Paper submitted to Structural Engineering Journal, ASCE on February 11, 2019
Paper status: Accepted on October 2, 2019
Reference: Salama , A. E. , Hassan, M., and Benmokrane, B., 2019, “Effect of GFRP Shear
Stirrups on the Strength of Two-Way GFRPRC Edge Slabs: Experimental and
Finite-Element Investigations,” Structural Engineering Journal, ASCE.
129
Abstract
Glass-fiber-reinforced-polymer (GFRP) reinforcing bars have recently gained wide acceptance
as a viable construction material for sustainable new constructions. Yet current codes and
guidelines have not addressed the design of GFRP-reinforced-concrete edge-slab–column
connections with FRP stirrups as shear reinforcement. This paper summarizes the experimental
results for full-sized edge-slab–column connections reinforced with GFRP bars and stirrups.
The effectiveness of the GFRP stirrups and their extension from the column face on the
performance of the tested connections are examined. In addition, a nonlinear 3D finite-element
analysis (FEA) is used to perform an in-depth investigation. Then, a comprehensive parametric
investigation is presented on edge connections with different stirrup sizes, extensions located at
different distances from the column, and different spacings. The test results reveal that the
presence of GFRP stirrups as shear reinforcement in the slab around the column perimeter
improved the punching-shear response. In addition, the FEA results are in good agreement with
the experimental results in terms of ultimate load, cracking patterns, strains in the reinforcement
and concrete, and load–deflection relationships, thereby confirming the accuracy of the finite-
element model. The results confirm that the punching-shear resistance decreased with increasing
stirrup spacing and increased with increasing stirrup size and extension from the column. Based
on the numerical-simulation results, a simple design approach to predicate the ultimate capacity
of the tested connections is proposed. The model yielded good yet conservative predictions with
respect to the experimental results as well as the available results in the literature.
Keywords: Punching shear, two-way flat slabs; edge connections; GFRP reinforcement;
stirrups; finite-element analysis (FEA); shear reinforcement; strength, design codes.
130 Chapter 6: Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRP
6.1. Introduction
Two-way reinforced-concrete (RC) flat-slab systems are very popular in construction because
of their functional and economic advantages. This structural system is vulnerable to a type of
brittle failure known as punching-shear failure. One essential consideration when designing
edge-slab–column connections is the lack of symmetry of the slab portion resisting the punching
action combined with a large unbalanced moment at the free edge. Unbalanced bending
moments transferred between the slab and column might produce significant shear stresses that
increase the possibility of brittle failure. Avoiding such a failure is of paramount importance.
Various solutions have been implemented to mitigate punching-shear failure at slab–column
connections. Examples are simply (1) increasing the slab thickness, adding a drop panel or
capital, or increasing the column dimensions; (2) using higher-strength concrete; or (3)
providing additional shear strength through shear reinforcement in the form of stirrups, shear
studs, shear heads, or corrugated bars in the slab around the column perimeter. The latter
solution is more effective and practical than the other two methods to increase the punching-
shear strength and deformation capacity of slab–column connections (Megally and Ghali 2000;
Lips et al. 2012) which is one of the primary motivations of this research.
Glass-fiber-reinforced-polymer (GFRP) reinforcing bars have recently gained wide acceptance
as a viable construction material for sustainable new constructions. The noncorrodible nature of
GFRP bars is a significant benefit for reinforced-concrete elements in harsh environments such
as parking garages treated with de-icing salts. Past research data has mostly focused on interior
connections entirely reinforced with GFRP bars under the transfer of shear or combined shear
and unbalanced moments (Lee et al. 2009; Dulude et al. 2013; Hassan et al. 2013a, b; Hassan et
al. 2014a, b; Gouda and El-Salakawy 2016; Hassan et al. 2017). There is, however, very limited
research on FRP edge-slab–column connections reinforced with shear reinforcement (Zaghloul
2007, El Gendy et al. 2016, Mostafa et al. 2018). GFRP shear reinforcement as stirrups, shear
studs, and corrugated bars have proved effective in enhancing slab strength and deformation in
tests on interior GFRPRC and edge-slab–column connections subjected to concentric loading
alone or shear–moment transfer (Lee et al. 2009; Dulude et al. 2013; Hassan et al. 2013a, b;
Hassan et al. 2014a, b; El-Gendy and El-Salakawy 2015; Mostafa and El-Salakawy 2018).
131
Hassan et al (2013a) tested new types of discrete closed and spiral FRP shear stirrups in interior
connections. Their use of FRP shear stirrups significantly increased the punching-shear strength
and deflection, on average, by 27% and 107%, respectively. Their findings also revealed that
FRP shear stirrups controlled the propagation of shear cracks and that the full flexural
mechanism could be attained. El-Gendy and El-Salakawy (2015) tested another type of FRP
shear reinforcement called headed studs. The average increases in punching-shear strength and
deformation capacity for edge connections were 40% and 98%, respectively. Mostafa and El-
Salakawy (2018) examined the effects of sand-coated double-headed GFRP studs and GFRP
corrugated bars in tests on edge connections reinforced with GFRP bars. The test results indicate
that both types of shear reinforcement were highly satisfactory in preventing brittle punching-
shear failure in the column vicinity. The ultimate shear strength and deformation capacity
increased by 27% and 16% and by 64% and 46%, respectively, (on average) for the connections
with shear studs and corrugated bars, compared to their counterparts with no shear
reinforcement.
The punching-shear behavior of two-way slabs is complex with a large number of parameters
that cannot be fully covered solely with an extensive experimental investigation. Therefore, in
addition to experimental investigations, finite-element analysis (FEA) is important in simulating
structural elements and providing insight into their behavior. Furthermore, FEA can depict crack
progression, deflections, and failure mechanisms as well as record more information for
unknown test measurements. To the authors’ best knowledge, no tests have yet been done on
GFRP edge-slab connections with GFRP stirrups as shear reinforcement. In addition, neither
ACI 440.1R (2015) nor CAN/CSA S806 (2012) address the design of GFRP-slab–column
connections with FRP shear reinforcement due to the limited research on such connections.
The experimental work presented in this paper extends an extensive research program carried
out at the University of Sherbrooke to design and implement GFRP bars in parking structures.
The first phase of this project has been completed (Dulude et al. 2013; Hassan et al. 2013a, b;
Hassan et al. 2014a, b; Hassan et al. 2017). A total of 30 GFRP-RC slabs were tested under
concentric loading. The test results and findings contributed to the assessment of the first
punching-shear equation in CAN/CSA S806 (2012). They also contributed to field applications
for implementing GFRP bars in flat-slab parking structures (Hôtel de Ville parking garage, QC,
132 Chapter 6: Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRP
Canada) and helped in designing the world’s first flat-slab parking garage (La Chancelière
parking garage, Qc, Canada) entirely reinforced with GFRP bars (Ahmed et al. 2016). This
paper summarizes the experimental results on GFRP-reinforced edge-slab–column connections
with discrete closed GFRP stirrups. The presence of GFRP shear stirrups in the column
periphery and their extension from the column face are examined. A nonlinear 3D finite-element
modeling was constructed using the ANSYS commercial FEA program (ANSYS User’s Manual
2018) to simulate the behavior of the tested connections. The model developed was validated
against the experimental results and an extensive parametric study was conducted to investigate
the critical parameters influencing the shear capacity of such connections, i.e., FRP-stirrup
extension, stirrup size, and spacing between stirrups. Lastly, a simplified design approach is
proposed to estimate the punching capacity of edge connections reinforced with shear stirrups
based on the FE results. The proposed approach was verified against the experimental results
and those available in the literature.
6.2. Research Significance
Field applications in recent years have demonstrated the excellent performance and durability
of GFRP-reinforced structures. Code-writing bodies in the US and Canada have tasked several
technical committees with producing standards and guidelines for elements reinforced with
GFRP. ACI 440.1R (2015) and CAN/CSA S806 (2012) do not address the design of such GFRP-
reinforced slab–column connections with FRP shear reinforcement due to very limited research.
This paper presents pioneering test results from full-sized GFRPRC edge-slab–column
connections with GFRP stirrups tested under combined vertical shear and unbalanced moment.
The purpose was to assess the effectiveness of the GFRP stirrups, taking into account the effect
of the GFRP-stirrup extension within the slab in a cruciform layout around the column faces. A
nonlinear FEA was used as a powerful tool to capture slab responses, followed by a
comprehensive parametric study to investigate the key parameters influencing the shear capacity
of such connections. The paper also establishes design provisions and recommendations for
engineers in designing FRP-RC slab–column connections with GFRP shear stirrups.
133
6.3. Summary of Experimental Program
6.3.1. Test Connections and Procedure
Three full-scale edge-slab-column connections were constructed and tested to failure under
eccentric shear stresses. The test connections represented edge connections from a prototype of
GFRP-RC flat-plate parking structure with 5 × 5 m2 square panels. This prototype was designed
for flexure in accordance with Canadian standards CAN/CSA S806 (2012) and CAN/CSA
A23.3 (2014). The total ultimate factored loads on the floor, including the slab weight, were
estimated in accordance with National Building Code of Canada (NBCC 2015). All slabs had
identical geometries of 2500 × 1350 × 200 mm with a 300-mm square column stub protruding
700 mm above and below the slab surfaces. Each connection was simply supported on three
edges and monolithic with a column at the middle of the fourth edge. Figure 6.1 shows the
overall slab geometry. The lines of contra flexure were assumed to be 20% from the span between
the column centerlines. All test connections were reinforced with sand-coated GFRP bars as
flexural reinforcement. Two of the connections were reinforced with GFRP shear stirrups
around the punching-shear zone; one had no shear reinforcement for comparison purposes.
Table 6.1 provides the characteristics of each connection . The stirrups were arranged in a
cruciform pattern with a constant spacing of d/2, where d is the slab effective depth equal to 160
mm. The first line of stirrups was located at d/4 from the column face for all connections with
shear reinforcement. Two connections (G-CS-1.75d and G-CS-4.25d) were reinforced in shear
with closed GFRP stirrups (No. 10) extending 1.75d and 4.25d away from the column face to
evaluate the effect of stirrup extension on the punching strength and behavior and to compare
its behavior in the control slab (G). It is worth mentioning that none of the current FRP design
codes and guidelines (CAN/CSA S806 2012 and ACI 440.1R 2015) have addressed the design
of slab–column connections with FRP shear reinforcement. A preliminary design for the amount
of shear stirrups in connections—G-CS-1.75d and G-CS-4.25d—was determined using a
proposed model for interor connections reinforced with FRP stirrups (Hassan et al. 2014).
Figure 6.2 shows the shear-stirrup layout and arrangement. All connections were tested under a
vertical shear force (V) applied to the face of the upper column stub and an unbalanced moment
(Mun) through two opposite horizontal loads (P) applied at the tips of the column ends. The
moment-to-shear ratio, Mun/V, was 0.3 m based on analysis of the prototype flat-plate structure
134 Chapter 6: Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRP
using the equivalent frame method according to CAN/CSA A23.3 (2014). The vertical load was
applied monotonically at a load-controlled rate of 5 kN/min, whereas the horizontal loads were
simultaneously applied with the vertical force in small increments to maintain a constant Mun/V
of 0.3 m throughout the test until failure.
Figure 6.1– Slab geometry and concrete dimensions
Table 6.1 – Details of test connections
Slaba f’c
b,
MPa
Bottom Tensile Reinforcement Top Compression Reinforcement Shear Reinforcement Stirrup
┴c // c
ρb,
(%) ┴c // c
ρt,
(%) db ,
mm Afv
rb,
mm
So;
mm
Sfv;
mm Extent
G 41.4 20 No. 20 10 No. 20 1.55 10 No. 15 7 No. 15 0.65 ----- --- ----- ------ ---- ----
G-CS-1.75d 47.6 20 No. 20 10 No. 20 1.55 10 No. 15 7 No. 15 0.65 9.5 71 38.1 0.25d 0.5d 1.75d
G-CS-4.25d 51.3 20 No. 20 10 No. 20 1.55 10 No. 15 7 No. 15 0.65 9.5 71 38.1 0.25d 0.5d 4.25d a G-aa-xd: G for GFRP tension reinforcement, aa for stirrup configuration (CS for closed stirrups); and xd for stirrup distance from the
column faces relative to the average effective depth, if any. b Cylinder strength on the day of testing (100×200mm cylinders). c Position perpendicular (┴) or parallel (//) to the free edge.
So = distance between column face and first line of shear stirrups and Sfv = spacing between consecutive lines of shear stirrup.
250
700
200
Support line
1350
700
300
250
300 1050
1600
700
200
6@
100
GFRP No.15
6-25M
10M stirrups
GFRP No. 20
160
150 1100
GFRP No.15
GFRP No. 20
200
Sym.
Axis
)a) Concrete dimension )c) Section (Y-Y) )b) Section (X-X)
135
Figure 6.2 – Typical reinforcement details and stirrup layout for slabs with and without shear
reinforcement
Straight bars
ars
GFRP No. 20
273
7@
114
5 @152 170
2500
GFRP No. 20
Bent bars
279
269
273
(a) G
456
342
304 456 170
1350
269
Bottom mesh
Top mesh
GFRP No. 15
Straight bars
GFRP No. 15
Straight bars
B B
4.2
5d
8@
80
40
Strain gauges
GFRP closed
stirrups
8@80
1.7
5d
40
3@
80
A A
Strain gauges
GFRP closed
stirrups
3@80 40
GFRP closed
stirrups
Section (A-A) Section (B-B)
(b) G-CS-1.75d (c) G-CS-4.25d
GFRP closed
stirrups
8@80 3@80 40 40
40
X X
Y
Y
136 Chapter 6: Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRP
6.3.2. Material Properties
The test connections were cast with a ready-mixed normal-weight concrete with a targeted 28-
day compressive strength of 35 MPa. The concrete compressive of each connection was
determined on the day of testing with three 100 × 200 mm concrete cylinders. The concrete
compressive strength (fc’) ranged from 41.4 to 52.5 MPa. Table 6.1 presents the concrete
strengths of the test connections. The sand-coated GFRP bars and stirrups were manufactured
with the pultrusion process (Pultrall Inc. 2018). Sand-coated Grade II and III GFRP bars as
classified in CSA S807 (CSA2015) as sizes No. 15 and No. 20, respectively, were used as
flexural reinforcement in all tested connections. Each connection was reinforced with straight
GFRP bars, except for the tension reinforcement (bottom) in the short direction, which had
double bent ends to provide adequate anchorage and avoid any unexpected slippage mode of
failure. Each slab was monolithic with a square column stub, which was designed to transfer
shear force and lateral moment to the slab without any premature column failure. The column
reinforcement consisted of six 25M deformed steel bars (three bars on each face) with 10M
deformed closed steel ties at 100 mm. The tensile properties of the GFRP bars were determined
by testing five samples according to ASTM D7205M (2011). Table 6.2 presents the tensile
properties of the flexural bars, which were calculated based on nominal cross-sectional areas.
Sand-coated discrete closed GFRP stirrups (No. 10) were used as shear reinforcement. The
stirrups had an overall depth of 145 mm, width of 290 mm, and bent radius (rb) of 38.1 mm. The
tensile properties of the straight portions of the GFRP stirrups were determined according to
ASTM D7205M (ASTM 2011). The bent strength of the FRP stirrups and bent bars were
determined with the B.5 test method in accordance with ACI 440.3R-04 (2004). Table 6.1
presents the bent strength of the GFRP stirrups and bent bars.
137
Table 6.2 – Tensile properties of the reinforcing bars and shear reinforcement
6.3.3. Experimental Setup and Instrumentation
All test connections were tested under combined vertical shear force (V) and unbalanced
moment (Mun) until failure. The vertical shear force was applied using a 1500 kN hydraulic jack
while two 1000 kN horizontal hydraulic jacks were installed on two rigid reaction frames to
apply the lateral loads. To free horizontal movement of the column during application of the
lateral loads, a steel pan with rollers was placed between the vertical jack and the top of the
upper concrete column. Figure 6.3 shows the test setup. All test connections were simply
supported on the bottom surface along three sides during testing with a new fabricated
supporting steel bed. This supporting bed was prestressed directly on the laboratory strong floor
with four 38 mm diameter steel tie rods before placing the test connection to avoid any lateral
movement that might be expected. On the slab top face, steel reaction beams restrained the three
supported edges to prevent slab lifting. To allow for slab rotation at the lines of contra flexure
during the entire test, 20 mm thick neoprene pads were placed between the slab and supporting
bed and between the slab and top restraining beams along the support lines. The test connections
were equipped with extensive external and internal instrumentation to aid in understanding
connection behavior. The flexural-reinforcement strains in both orthogonal directions were
measured with 11 electrical resistance strain gauges (see Fig. 6.2). The strains in the GFRP
Bar Designation
Nominal
Cross-
Sectional
Areaa
(mm2)
Immersed
Cross-
Sectional
Area,
(mm2)
Ultimate Tensile
Strength b
(MPa)
Tensile
Modulus of
Elasticity c
(GPa)
Ultimate Tensile
Strain
(%)
Straight flexural GFRP bars
No. 15 GFRP bar 199 240 1323 ±12 64.8±0.5 2.04 ±0.05
No. 20 GFRP bar 285 333 1334 ±85 64.9±0.6 2.06 ±0.13
Bent flexural GFRP bars
No. 20 straight portion 285 331
1210±63 53.0±0.48 2.28±0.15
No. 20 bent portion ffvb = 490±44 ------ ------
Steel bars
10M 100 ------ fy = 420 200 ɛy = 0.21
25M 500 ------ fy = 470 204 ɛy = 0.23 a according to CSA S807-15 (CSA 2015). b and c calculated using nominal cross-sectional areas of the reinforcing bars.
ffvb = ultimate tensile bend strength obtained from the B.5 test method according to ACI 440.3R-12 (ACI 2012)
fy = steel yielding strength, εy = steel yielding strain.
138 Chapter 6: Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRP
stirrups were monitored with 6 mm electrical strain gauges mounted at mid-height of the vertical
legs of the GFRP stirrups and bend location in each orthogonal direction (see Fig. 6.2). The
concrete strains induced on the compression side were measured with five concrete strain gauges
mounted in the column vicinity. The connection deflection at the different locations along the
column centerlines in both orthogonal directions was captured with 14 string potentiometers
(pots). Figure 6.3 shows the different positions of linear potentiometers and the concrete gauges.
All the instruments were connected to a data-acquisition system (DAQ) to record the applied
loads, deflections, strains in GFRP bars and shear stirrups, and concrete strains. During testing,
the progression of cracks was marked, and the corresponding loads were recorded.
Figure 6.3 – Test setup and instrumentation
139
6.4. Test Results and Discussion
6.4.1. General Cracking Pattern and Failure Mode
The test connections displayed similar crack propagation on the tension side of the slab (bottom
surface). The connections with shear reinforcement, however, evidenced more intensive cracks
with larger punching-shear-failure surfaces compared to their counterpart without shear
reinforcement. During the test, flexural cracks appeared first on the slab tension side. The first
flexural crack began to appear at about 15% to 16% of the ultimate vertical load. These radial
flexural cracks originated from the inner slab–column interface and propagated towards the
supports. Inclined torsion cracks formed at the inner corners of the columns. These cracks started
to appear at about 25% of the ultimate load, then propagated upward the slab edge to half of the
slab depth at around 50% of the ultimate load. Thereafter, tangential cracks generated around
the column and crossed over the radial cracks at higher loads. As the load increased, the number
of such cracks and their widths in the column vicinity increased. Shear cracks initiated from the
slab tension side and propagated towards the slab compression side until failure occurred. At
failure, a major tangential crack was intercepted by the flexural cracks in approximately
perpendicular manner, forming the punching cone. Fig. 6.4 presents an overview of the cracking
pattern for all the test connections in tension and free edge sides and along the sawed sections.
The control connection G, without shear reinforcement, experienced a typical brittle punching-
shear failure without much warning. The failure mode for connection G-CS-1.75d, with stirrups
extending 1.75d, was punching-shear failure outside the shear-reinforced zone. Some
deformability was, however, achieved before failure compared to its counterpart G, without
shear reinforcement. On the other hand, the 4.25d extension of the FRP stirrups in connection
G-CS-4.25d offered sufficient resistance, larger deformations, and concrete crushing at the
column vicinity on the compression side of the slabs, which gave early warning signs before the
punching-shear failure. The final failure mode was mixed flexural/punching-shear failure inside
the shear-reinforced zone. Figure 6.4 shows the sawn sections of the connections with and
without GFRP shear stirrups. Connection G evidenced a single diagonal shear crack, while
connection G-CS-1.75d had a horizontal splitting crack over the top of the stirrups. This splitting
crack became an inclined shear crack beyond the outermost set of shear stirrups. Connection G-
CS-4.25d had several inclined shear cracks within the regions reinforced with the shear stirrups
140 Chapter 6: Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRP
as well as horizontal splitting cracks located above the stirrups. The formation of the horizontal
splitting cracks near the columns is assumed to have caused the slight gradual drops in load
capacity. Lastly, these inclined and splitting cracks created the failure surfaces.
Figure 6.4 – Final punching-shear failure surface (in bold) on slab tension side and free edge
and saw-cut section
6.4.2. Ultimate Capacity and Load–Deflection Characteristics
In general, the presence of GFRP shear stirrups inside the punching-shear zone significantly
improved slab behavior and the punching mechanism. The strength and deformation capacity
of the shear-reinforced slabs were, however, strongly influenced by the characteristics of the
shear reinforcing system (i.e., extension, amount, type, etc.). Figure 6.5 plots the applied vertical
load versus the deflection relationships at 80 mm from the column face. In general, the initial
uncracked stiffness for all connections was similar, with or without shear reinforcement. The
slabs with shear reinforcement, however, exhibited slightly higher post-cracking stiffness than
G
Pu
nch
ing
surface
Inclin
ed crack
s
Clo
sed stirru
ps
Pu
nch
ing
Su
rface In
clined
cracks
G-CS-
1.75d
G-CS-
4.25d
Clo
sed stirru
ps
Inclin
ed C
racks
Sp
litting
crack
141
their counterpart without shear reinforcement. Control connection G and connection G-CS-
1.75d, which had limited stirrups around the column, produced similar bilinear load–deflection
responses until punching failure occurred. These two connections failed at ultimate loads of 314
and 370 kN and at 21 and 28 mm, respectively. Compared to connection G, connection G-CS-
1.75d had failure load and deflection that were 18% and 34% higher, respectively. Connection
G-CS-4.25d, with shear reinforcement extending 4.25d, experienced gradual failure with
considerable post-peak deformations. The GFRP stirrups offered sufficient resistance and
confinement to control the development of large shear cracks and effectively distributed the
shearing forces around the punching-shear zone. The more significant increase in deformability
in connection G-CS-4.25d could be attributed to the flexure mechanism due to the mobilization
of the shear stirrups before punching-shear failure occurred. Connection G-CS-4.25d failed at
an ultimate load of 444 kN, with a corresponding ultimate deflection of 36 mm. The resulting
ultimate load and maximum deformation of G-CS-4.25d at failure were 1.41 and 1.8 times,
respectively, that of connection G. This confirms the effectiveness of closed stirrups in
achieving substantial deformations before slab collapse. Table 6.3 shows a summary of the test
results for all connections. These results indicate the effect of the GFRP shear stirrups in
increasing the punching-shear strength and the deformation capacity of the tested connections,
even with the limited stirrup extension around the column. Moreover, increasing the stirrup
extension around the column from 1.75d to 4.25d increased the vertical-shear force by 20%.
Figure 6.5 – Comparison between FEA and test results in terms of vertical-load deflection
G
Exp
FEA
G-CS-1.75d
Exp
FEA
G-CS-4.25d
Exp
FEA
142 Chapter 6: Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRP
Table 6.3 – Summary of the test and FEA results
Slab
Ultimate Load Mu/
Vu,
(m)
Δvu,
(mm)
ΔFE.,
(mm)
Strains at Ultimate Load (µε) Average
Stirrup Strain
(µε)
Maximum
Stirrup Strain
(µε) , uV
(kN)
VFE.,
(kN)
Mu,
(kN.m)
Concrete, (µε) Flexural
reinforcement
FRP stirrups
@ 0.25 d
Exp. FE. Exp. a FE. Exp. a FE. ┴ a // a ┴ a // a
G 314 318 98 0.31 20.55 19.72 784 820 6432 6708 ----- ----- ----- ----- ----- -----
G-CS-1.75d 370 372 115 0.31 28.08 24.2 979 930 8661 8610 2579 2589 3215 2519 3918 3402
G-CS-4.25d 444 456 133 0.30 35.82 32.5 2444 2430 13226 11845 5789 5622 5417 5193 6412 5899 a Position perpendicular (┴) or parallel (//) to the free edge
143
Figure 6.6 – Comparison between FEA and test results in terms of vertical-load reinforcement
bars, concrete, and stirrup strains perpendicular to the free edge
G-CS-1.75d G-CS-4.25d G
Exp
FEA Exp
FEA Exp
FEA
)a) Flexural reinforcement strains
G-CS-1.75d G-CS-4.25d G
Exp
FEA
Exp
FEA
Exp
FEA
(b) Concrete strains
Exp
FEA
Exp
FEA
G-CS-1.75d G-CS-4.25d
)c) Stirrup strains
144 Chapter 6: Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRP
6.4.3. Flexural Reinforcement and Concrete Strains
Figure 6.6 plots the applied vertical load versus the flexural tension reinforcement and concrete
strains for all the tested connections. The flexural-reinforcement strains were measured at 75 mm
from the column face perpendicular to the free edge, whereas the concrete strains were recorded at
the column face. Table 3 reports the maximum reinforcement and concrete strains. Connection G,
without shear reinforcement, had lower tensile strain than its counterparts with GFRP shear stirrups.
The maximum recorded strain in flexural bars was 6430 μs, which represents 35% of the ultimate
tensile strength. Moreover, the maximum concrete strains around the column vicinity were low and
below the concrete crushing strain of 3500 and 3000 μs, as per CAN/CSA S806 (2012) and ACI
440.1R (2015), respectively. Connections G-CS-1.75d and G-CS-4.25d, with shear reinforcement,
exhibited higher strains in the GFRP flexural bars and higher concrete strains values than control
connection G at ultimate. The GFRP stirrups offered sufficient resistance and confinement to
control the development of large shear cracks and effectively distributed the shearing forces in the
punching-shear zone, which mobilized the flexural reinforcement to achieve higher strains. This
observation coincides with past findings for interior GFRP-reinforced slab–column connections
with FRP stirrups (Hassan et al. 2014a). The maximum reinforcement strains were 8700 and 13200
μs, respectively, representing 47% and 71%, of the ultimate tensile strength, respectively. The
maximum recorded concrete strains were 979 and 2444 μs (< 3000 or 3500) for G-CS-1.75d and G-
CS-4.25d, respectively. No signs of concrete crushing in the compression zone for connection G-
CS-1.75d, where the mode of failure was triggered by brittle punching-shear failure occurring
outside the shear-reinforced zone. In contrast, for connection G-CS-4.25d, the achieved higher
concrete strains indicated the concrete crushing at the column vicinity on the compression side of
the slabs which evidenced the occurrence of the mixed flexure-punching shear failure.
6.4.4. Shear-Reinforcement Strains
Figure 6.6 shows the stirrup strain in the vertical portion of the FRP stirrup at 0.25d from the
column face, while Fig. 6.7 plots the applied vertical load versus the measured average strains
located between 0.25d to 1.25d from the column face in both orthogonal directions. As shown
in Figs. 6.6 and 6.7, the contribution of the GFRP stirrups to the punching-shear strength was
insignificant before cracking, however, the stirrup contribution began to appear after the
progression of shear cracks. Thereafter, the stirrups transferred most of the forces across these
145
shear cracks and controlled their further widening. In addition, the average strains at the mid-
height of the vertical portions of the FRP stirrups in both directions were 2867 and 5305 μs for
connections G-CS-1.75d and G-CS-4.25d, respectively. These values are close to the strain
limits of 4000 or 5000 μs specified in ACI 440.1R (2015) and CAN/CSA S806 (2012) for shear
design of FRP stirrups. Thus, the FRP shear reinforcement might be designed with a strain value
of 4000 or 5000 μs, as recommended in ACI 440.1R (2015) and CAN/CSA S806 (2012). Table
6.3 lists the maximum and average recorded strains in the FRP stirrups in both directions.
Figure 6.8 depicts the vertical-strain distributions in the GFRP stirrups at 95% of the ultimate
load along both orthogonal directions. The maximum measured strains were monitored up to a
distance of 0.25d to 1.25d from the column faces without any apparent signs of tensile rupture
in the vertical or bent portions of the stirrups. The FRP shear stirrups between 1.75d and 2.25d
achieved relatively high strains at 95% of the ultimate load. This implies that the FRP stirrups
were still active up to 2.25d. In addition, limiting the extension of the FRP stirrups in connection
G-CS-1.75d beyond a distance of 1.75d exhibited limited deformation capacity. Further
research, however, is needed to determine the corresponding distance for FRP stirrups.
Figure 6.7 – Average stirrup strain in vertical legs from 0.25d to 1.25d
(a) Perpendicular direction to the free edge (b) Parallel direction to the free edge
146 Chapter 6: Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRP
Figure 6.8 – Strain profile of the vertical legs of the stirrups for slabs with shear reinforcement
6.5. Finite-Element Simulations
The FEA was carried out using a finite-element software package: ANSYS (ANSYS User’s
Manual 2018). An FEA simulation was developed to investigate the punching-shear response
and strength of connections tested. The models were validated with the authors’ experimental
data presented herein, and then an extensive parametric study was conducted to investigate the
critical parameters influencing the shear capacity of such connections. The following section
describes the element types used to model the different materials; constitutive models for
concrete, steel, and FRP; meshing; and boundary conditions.
6.5.1 Material Properties
An eight-node 3-D solid element, SOLID 65, was used to model the concrete. This element is
capable of considering cracking in three orthogonal directions: crushing, plastic deformation,
and creep. To properly model the concrete, the considered model for concrete comprises linear
and multi-linear isotropic material properties in addition to the concrete model defined in
ANSYS (Wolanski 2004, Chansawat et al. 2006, Özcan et al. 2009).
The linear isotopic material properties include the elastic modulus of concrete and Poisson’s
ratio. The elastic modulus was calculated using Eq. (6.1) and Poisson’s ratio was assumed to be
0.2 whereas the uniaxial cracking stress was computed with Eq. (6.2). Figure 6.9a plots the
Exp
FEA
G-CS-4.25d
G-CS-1.75d
G-CS-1.75d
G-CS-4.25d
Exp
FEA
(a) Perpendicular direction to the free edge (b) Parallel direction to the free edge
147
multilinear isotropic stress–strain curve of the concrete with ignoring the descending branch, as
recommended in past studies (Gorji 2009; Wolanski 2004; and Büyükkaragöz 2010). The first
point on the curve represents the linear behavior of the concrete up to 30% of the ultimate
compressive strength whereas the ascending branch of the curve was obtained using the Desayi
model (Desayi and Krishnan 1964), as given by Eq. (6.3) and (6.4), up to the uniaxial crushing
stress (fc′). The ascending branch of the curve represents the stage after cracking where the
uniaxial cracking stress of the concrete element is set to zero in the direction normal to the crack
plane. The shear transfer coefficient for open cracks βt and βc for closed cracks quantifies the
ratio of shear transferred across the cracks. The shear-transfer coefficient ranged from 0.0 to
1.0, with 0.0 representing a complete loss of shear transfer and 1.0 representing no loss of shear
transfer (ANSYS, Release 19.1 2018). βt and βc have been used in past studies with different
ranges (Kachlakev et al. 2001, Wolanski 2004, Mostofinejad et al. 2006, Qi Zhang 2004). The
values of βc and βt were determined after preliminary analysis of the tested connections to
capture the load–deflection behavior at cracking and ultimate load. In this study, βt was assumed
to be within 0.25 to 0.5, while βc was assumed to be within 0.5 to 0.95. Figure 6.10 depicts the
load–deflection response of connection G-CS-4.25d with different shear-transfer coefficients.
As shown in Fig. 6.10, βt of 0.3 and βc of 0.8—indicating good agreement with the stiffness
change and the ultimate loading of connection G-S-4.25d—were adapted in this work.
𝐸𝐶 = 4500 √𝑓𝑐′ (6.1)
𝑓𝑟 = 0.6 √𝑓𝑐′ (6.2)
𝜀𝑜 =2 𝑓𝑐
′
𝐸𝑐 (6.3)
𝑓 =𝐸𝑐 𝜀
1+(𝜀 𝜀𝑜⁄ )2 (6.4)
A 3-D spar element, LINK 180, was used to the model steel and FRP reinforcement. A LINK
180 element is a uniaxial tension–compression element with two nodes and three degrees of
freedom translations in the nodal x, y, and z directions. This element is also capable of
simulating nonlinearity and plastic deformations. A LINK180 element is defined by linear and
bilinear isotropic material properties to model steel reinforcement. GFRP reinforcement,
however, is defined by linear-elastic material properties. Poisson’s ratios of 0.3 and 0.25 were
148 Chapter 6: Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRP
assumed for the steel and GFRP bars, respectively. The elastic modulus of the GFRP flexural
bars and shear stirrups were determined experimentally, as listed in Table 6.2. Figure 6.9b
provides the stress–strain relationships for the GFRP and steel bars used in this study (note that
the steel bars were only used in the columns). A discrete model concept was used to model
reinforced-concrete elements. Both the concrete and reinforcement mesh shared the same nodes
(location and numbering). As the GFRP reinforcement did not experience any bar slippage or
bond failure during the tests, a perfect bond was assumed in order to simulate the bond between
the reinforcement and concrete. The steel loading plates were modeled as an eight-node solid
element, SOLID45, with three degrees of freedom translations in the nodal x, y, and z directions
at each node. This element is capable of plasticity, creep, swelling, stress stiffening, large
deflection, and large strain. A SOLID45 element is defined by linear isotropic properties and
ignoring strain hardening. The modulus of elasticity and Poisson’s ratio used for the steel
loading plates were 200 GPa and 0.3, respectively.
Figure 6.9 – Stress–strain relationships used in the FE model
(a) concrete (b) GFRP and steel bars
149
Fig. 6.10 – Load-deflection response with different shear transfer coefficients
6.5.2. Model Geometry, Loading and Boundary Conditions
Figure 6.11 gives a complete view of the overall mesh of the concrete, reinforcement
configuration, loading plates, and boundary conditions of the FE model. Only the half model of
the tested connection was simulated, taking advantage of slab symmetry about the axis of
symmetry perpendicular to the free edge. The boundary conditions at this axis of symmetry were
set to represent the effect of continuity. To simulate the test boundary conditions, the slab was
restrained against vertical movement in the y direction along the three simply supported edges,
while the slab corners were restrained against movement in the three directions. The loads were
applied through the nodes over the top and side steel plates to simulate vertical shear (V) and
unbalanced moment (Mun). Moreover, a convergence study was carried out on the simulated
test connections with different mesh sizes in order to determine an appropriate mesh density.
The selected mesh sizes ranged from 20 to 80 mm in increments of 10 mm. Figure 6.12 shows
the results of the convergence study for G-CS-4.25d. Based on this study, a uniform mesh size
of 40 mm was chosen for the concrete and reinforcement elements of the simulated connections.
It should be mentioned that decreasing mesh size beyond 40 mm increased the computational
time without any significant change in the numerical results.
G-CS-4.25d
βt = 0.25 , βc = 0.6
βt = 0.30 , βc = 0.8
βt = 0.50 , βc = 1.0
150 Chapter 6: Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRP
Figure 6.11 – Geometry and reinforcement details of ANSYS model
Applied
Horizontal loads
Applied
Vertical load
(a) Element types and boundary conditions
(b) Applied vertical and horizontal loads
Concrete
(SOLID 65)
Loading plates
(SOLID 45)
Constraint in
z-direction Roller support
Constraint in x-
y-z direction
GFRP stirrups
(LINK 180) GFRP bars
(LINK 180)
Steel bars and stirrups
(LINK 180)
151
Fig. 6.12 – Mesh convergence study for G-CS-4.25d
6.5.3. Model Verification
The results of the finite-element analysis (FEA) were verified against the experimental results
of the tested connections to examine the validity of the FE model in describing slab behavior.
The comparison was performed with respect to the load–deflection responses; ultimate capacity;
and ultimate strains in the concrete, flexural bars, and shear stirrups; strain distributions in the
shear stirrups; and cracking propagation. Figure 6.5 depicts the experimental and predicted
vertical load–deflection curves for the tested connections. The results obtained from the
nonlinear FEA accurately describe the response of the tested slabs and the reduction in stiffness
after cracking. The FEA of the slabs predicted a punching-shear capacity almost 1% higher than
the test results, but the differences are not significant. As for the deflection values at ultimate
load, the predicted values (ΔFE.) were mostly safer than those obtained experimentally (Δexp.).
Table 6.3 presents the numerical and experimental deflections at failure. The average numerical-
to-experimental deflection at ultimate load was 91% with a standard deviation of 5%. This
indicates a good prediction by the FEA. Figure 6.13 gives the deformed shapes at ultimate load
for all slabs produced by FEA. Figure 6.6 plots the applied vertical load versus the maximum
recorded strains in the concrete, flexural bars, and FRP stirrups located at 0.25d from the column
face. As the figure shows, the analytically predicted and experimentally measured strains are in
good agreement. The average numerical-to-experimental strains at ultimate load in the concrete,
reinforcement, and stirrups were 99%, 98%, and 99% with standard deviations of 5%, 7%, and
2%, respectively. Figure 6.8 compares the measured and predicted vertical strain distributions
152 Chapter 6: Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRP
in the GFRP stirrups at 95% of the ultimate load along both orthogonal directions. The FEA
properly reproduces the experimentally measured stains, as shown in Fig. 6.8. The average
numerical-to-experimental vertical strains at 95% of the ultimate load in the FRP stirrups was
98%, with a standard deviation of 6%. Furthermore, cracking propagation in both the tests and
FEA started on the tension side of the slabs. The cracking started at a vertical load of
approximately 49 kN to 59 kN. Cracking initiated from the inner corners of the columns and
developed toward the slab edges. Cracks on the compressive side of the slabs also developed at
approximately 75% of the ultimate load. Cracking propagation yielded by the finite-element
simulations was in good agreement with the experimentally observed cracks. Figure 6.14 shows
the typical crack progression on the tension side of connection G-CS-1.75d at different loading
stages, as determined by the FE modeling. In short, the model was able to predict, with
reasonable accuracy, the load–deflection behavior; experimentally monitored strains in the
flexural bars, concrete, and stirrups; strain distributions in the shear stirrups; and the cracking
pattern.
6.6. Parametric Study
The calibrated FEA model presented herein was used to develop an extended parametric study,
pertaining, in particular, to GFRP edge slabs with FRP stirrups. The influence of stirrup
extension, diameter, and stirrup-to-stirrup spacing in the punching-shear zone were investigated.
6.6.1. Effect of Stirrup Extension from the Column Face
The effectiveness of shear reinforcement to increase the punching-shear capacity of a slab–
column connection depends on the extension of the shear reinforcement around the column.
Figure 6.15a depicts the vertical load–deflection relationships with different stirrup extensions,
ranging from 1.75d to 4.25d in increments of 0.5d from the column face. As expected, the slab
with the lowest stirrup extension around the column, 1.75d, experienced the lowest stiffness and
punching capacity. Increasing the GFRP-stirrup extension from 1.75d to 4.25d significantly
improved the punching-shear and deformation capacities, which is in good agreement with the
experimental results. The GFRP stirrups provided sufficient resistance and confinement, which,
in turn, controlled the progression of shear cracks and effectively distributed the shearing forces
in the punching-shear zone. The stirrup extension, however, had less impact on the post-
153
cracking stiffness. According to the FEA predictions of the slabs, the vertical shear force
increased significantly (18%) by increasing the stirrup extension from 1.75d to 4.25d. This is
almost 2% lower than the experimental results of connections G-CS-1.75d and G-CS-
4.25d.increasing the stirrup extension from 1.75d to 4.25d.
Figure 6.13 – Deformed shapes of simulated connections
G
G-CS-4.25d
G-CS-1.75d
154 Chapter 6: Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRP
Figure 6.14 – Cracking progression at different loading levels for connection G-CS-1.75d
6.6.2. Effect of Stirrup Diameter
The numerical modeling of G-CS-1.75d was considered in order to address the effect of using
different stirrup diameters (8, 10, and 12 mm). Figure 6.15 b depicts the effect of stirrup diameter
on ultimate capacity. Increasing stirrup diameter has a direct contribution to the ultimate
capacity, whereas the shear-reinforcement area at the critical section of the punching shear is
increased. Increasing the stirrup diameter from 8 mm to 12 mm increased the punching capacity
and deflection by approximately 23% and 14%, respectively. Note that the numerical results are
a) 25% Vu, FEM b) 50% Vu, FEM
c) 75% Vu, FEM d) 100% Vu, FEM
155
limited to stirrups with 12 mm diameter because the stirrup diameter is restricted by the slab’s
effective depth. From the practical point of view, the ratio between the bent radius and stirrup
diameter should not less than 4 (ACI 440.1R 2015). Therefore, more experimental testing is
needed to accurately investigate the effect of stirrup diameter with greater slab thicknesses.
6.6.3. Effect of Spacing Between Stirrups
The spacing between stirrups is one of the most significant parameters affecting the punching
shear strength, slab deformation, failure mechanism, and development of the internal diagonal
shear cracks. After the development of shear cracks, the shear stirrups transferred most of the
forces across the developed shear cracks and delayed further widening, particularly when the
stirrup spacing was reduced. This, in turn, increased the punching-shear and deformation
capacities of the tested connections. Figure 6.15 c compares the numerical results at different
stirrup spacings between 0.25d (40 mm) and 0.75d (120 mm). As seen in Fig. 6.13 c, the post-
cracking stiffness, punching strength, and deformation capacity decreased when the spacing
between stirrups was increased from 40 mm to 120 mm. According to the FEA results, the
predicated ultimate strength and deformation capacity decreased by 18% and 13%, respectively.
Based on the numerical results, the spacing between FRP stirrups should not exceed 0.5d, as per
CAN/CSA A23.3 (2014) for steel-reinforced slabs. Further experimental testing on such
connections reinforced with FRP is, however, needed.
156 Chapter 6: Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRP
Figure 6.15 – Parametric study vertical load–deflection results
6.7. Proposed Approach
So far, CAN/CSA S806 (2012) and ACI 440.1R (2015) lack provisions for estimating the
ultimate capacity of two-way FRPRC slabs with FRP shear reinforcement, due to the distinct
lack of experimental work. This section proposed a simple design approach to predict the
punching-shear capacity of FRP-RC edge slab column connections reinforced with FRP shear
stirrups. The CAN/CSA S806 concrete shear-strength equation for slabs without shear
reinforcement was adapted by introducing a new parameter β to consider the contribution of
FRP shear stirrups, based on the finite-element parametric study. The approach also modified
(a) Effect of GFRP-stirrup extension (b) Effect of GFRP-stirrup diameter
(c) Effect of GFRP stirrup spacing
157
the equation for the stirrup-contribution equation in CAN/CSA A23.3 to consider the difference
between the mechanical characteristics of FRP and steel reinforcement. The nominal punching-
shear capacity, Vf, of two-way slabs due to moment transfer by eccentricity of shear is calculated
with Eq. (6.5) according to ACI 318 (2014) and CAN/CSA A23.3 (2014).
𝑉𝑓 = 𝑣𝑢/ (1
𝑏𝑜; 0.5𝑑 𝑑+𝛾𝑣 𝑐
𝐽𝑐𝑒) (6.5)
where vu = ultimate shear stress at 0.5d from column face; bo;0.5d = critical shear perimeter at
0.5d from the column face; γv = fraction of unbalanced moment transferred by shear eccentricity;
d = effective slab depth; c = distance from the centroid of the critical shear section to the face
of shear critical section; e = eccentricity of the shear force from the centroid of the critical shear
section; and Jc = polar moment of inertia of critical shear section.
The factored shear–stress resistance, computed as vc+vf, where vc and vf are the concrete and
shear-reinforcement contributions to the shear strength inside the punching zone, respectively.
Equation (6.6) is proposed to calculate the FRP-stirrup contribution (vf). This equation is a
modified version of the equation for steel stirrups in CAN/CSA A23.3 (2014), replacing fy
(yielding strength) with a specific stress (ffv) at a limiting strain value (εfv) of 4000 με, as per
ACI 440.1R (2015). This is close to the average strain of the FRP stirrups in both orthogonal
directions based on the numerical (3920 µε) and experimental results (4086 µε). In addition, the
average strain of the FRP stirrups in both orthogonal directions was 3718 µε for the simulated
GFRP-reinforced edge slab-column connections in the parametric study as listed in Table 6.4.
𝑣𝑓 = 𝐴𝑓𝑣 𝑓𝑓𝑣
𝑏𝑜 𝑠𝑓𝑣 (6.6 a)
𝑓𝑓𝑣 = 0.004 𝐸𝑓𝑣 (6.6 b)
where Afv = cross-sectional area of the FRP shear reinforcement at a perimeter of 0.5d from the
column face; db = stirrup diameter; rb = bend radius of stirrup; ffv = tensile strength in the straight
portion of the FRP stirrups; bo,0.5d = perimeter of shear critical section at a distance of 0.5d from
the column face; and sfv = stirrup spacing measured perpendicular to bo;0.5d.
The concrete shear strength inside the shear reinforced zone was quantified from the relation vc
inside = vFE -vf, where vFE is the ultimate shear stress from FE results and vf is the FRP-stirrup
158 Chapter 6: Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRP
contribution computed from Eq. 6.6 and listed in Table 6.4. vc inside was expressed as a ratio of
the CAN/CSA S806 (2012) concrete shear-strength equation for two-way slabs without shear
reinforcement (vc CSA), as shown in Eq. (6.7). vc CSA was modified with a multiplier factor β to
consider a reduction in concrete strength due to the contribution of FRP shear stirrups, as shown
in Eq. (6.8). β was calculated based on the FE parametric study. A regression analysis was
performed to quantify the best fit for vc inside . This factor was found to be 0.64 (on average) using
a stirrup strain of 4000 με (as per ACI440.1R 2015). It is worth mentioning that, a close value
was achieved for β using the FE stirrup-strain results. The final form of vc inside is presented in
Eq. (6.9).
𝑣𝑐 𝐶𝑆𝐴 = 0.056 𝜆 ∅𝑐 (𝐸𝑓 𝜌𝑓 𝑓𝑐′ )
1
3 (6.7)
𝑣𝑐 𝑖𝑛𝑠𝑖𝑑𝑒 = β × 0.056 𝜆 ∅𝑐 (𝐸𝑓 𝜌𝑓 𝑓𝑐′ )
1
3 (6.8)
𝑣𝑐 𝑖𝑛𝑠𝑖𝑑𝑒 = 0.036 𝜆 ∅𝑐 (𝐸𝑓 𝜌𝑓 𝑓𝑐′ )
1
3 (6.9)
where λ = concrete density factor (1 for normal weight); ϕc = concrete resistance factor (0.65);
Ef = elastic modulus of the FRP bars; and ρf = FRP-reinforcement ratio.
As shown in Table 6.5, the proposed approach gave reasonable predications with respect to the
experimental results as well as against the results reported in the literature for connections
reinforced with different types of FRP shear reinforcement such as corrugated bars, shear studs,
and grids (El-Gendy and El-Salakawy 2015; Mostafa and El-Salakawy 2018; Zaghloul 2007): an
average Vtest/Vpred of 1.08 ± 0.22 and a corresponding COV of 20.40%. Further research,
however, is required to assess the accuracy of the proposed approach that takes into
consideration a large number of different variables influencing the behavior and strength of such
FRP-reinforced slab–column connections.
158 Chapter 6: Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRP
Table 6.4 – Results of finite element parametric study
Connection Parameter
Ultimate Load Average Stirrup
Strains (µε)
Using Average Stirrup Strains Using ACI 440.1R Strain Limit (4000 µε)
VFE.,
(kN)
ΔFE.,
(mm)
vFE
(MPa)
vf
(Eq.6)
(MPa)
vc inside = vFE -vf
(MPa) vc inside /vc CSA
vf
(MPa)
vc inside = vFE -vf
(MPa) vc inside /vc CSA
┴ a // a
G-CS-1.75d Stirrup
extension
372 24.2 2.83 3390 3174 1.31 1.52 0.77 1.60 1.24 0.62
G-CS-2.25d 387 25 2.95 3743 3402 1.43 1.52 0.76 1.60 1.35 0.68
G-CS-2.75d 397 26.5 3.02 3918 3687 1.52 1.51 0.76 1.60 1.43 0.72
G-CS-3.25d 411 28 3.13 4124 3965 1.61 1.52 0.76 1.60 1.53 0.77
G-CS-3.75d 430 28.92 3.27 4529 4300 1.76 1.51 0.76 1.60 1.68 0.84
G-CS-4.25d 439 31 3.34 4857 4756 1.92 1.42 0.72 1.60 1.75 0.88
G-CS-1.75d-8 Stirrup
diameter
332 23.13 2.53 3125 2832 0.84 1.69 0.85 1.12 1.40 0.71
G-CS-1.75d-12 407 26.4 3.10 3809 3578 2.35 0.75 0.38 2.54 0.56 0.28
G-CS-1.75d-40 Stirrups
spacing
420 27 3.20 3827 3583 2.36 0.83 0.42 2.55 0.64 0.32
G-CS-1.75d-60 400 25.6 3.05 3645 3412 1.88 1.17 0.59 2.13 0.92 0.46
G-CS-1.75d-120 344 23.5 2.62 3265 2875 0.82 1.80 0.91 1.06 1.56 0.78
Average 3839 3597 0.70 0.64 a Position perpendicular (┴) or parallel (//) to the free edge; vc CSA = concrete contribution determined from CAN/CSA S806 (2012) (Eq.7); vf = ultimate punching-
stress provided by the FRP shear stirrups (Eq. 6)
159
Table 6.5 –Tested-to-predicted punching shear capacities using the simplified proposed equation
Reference Slab C1 x C2,
(mm x mm)
t,
(mm)
d,
(mm) t,
(%)
RFT.
Type
Shear RFT
Type M/V (m)
Vu test,
(kN)
Proposed Simplified Equation
Vin, pred, kN vin, pred, a
(MPa) Vu/Vpred
This study G-CS-1.75d 300 x 300
200 160
1.55 SG SG stirrups 0.31 370 371 2.87 1.00
G-CS-4.25d 300 x 300 1.55 SG SG stirrups 0.30 444 381 2.90 1.16
Mostafa et al.
(2018)
N-0.9-C8 300 x 300 0.85 SG SG C. bars 0.40 286 204 1.82 1.40
N-0.9-C6 300 x 300 0.85 SG SG C. bars 0.40 253 183 1.64 1.38
N-0.9-S8 300 x 300 0.85 SG SG studs 0.40 294 324 2.90 0.91
N-0.9-S6 300 x 300 0.85 SG SG studs 0.40 298 272 2.43 1.09
El-Gendy et al. (2015) RD-75-M 300 x 300 0.85 GRD GRD studs 0.40 256 236 2.11 1.09
RD-50M 300 x 300 0.85 GRD GRD studs 0.40 273 295 2.64 0.92
Zaghloul (2007) ZJEFCS 250 x 250 150 120 0.85 NEF NEF studs 0.42 230 314 5.43 0.73
Average c 1.08
SD c 0.22
COV% c 20.40
C1 = shorter side of the column; C2 = longer side of the column; t is the average flexural tensile-reinforcement ratio; SG = sand-coated glass-fiber bars; GRD =
ribbed glass-fiber bars; NEF= NEFMAC 2-D carbon-fiber grids, C. bars =corrugated bars.
160 Chapter 6: Effect of GFRP Shear Stirrups on the Strength of Two-Way GFRP
6.8. Summary and Conclusions
This paper reported the test results of full-scale RC edge slab–column connections reinforced
with GFRP bars and shear stirrups. Finite-element models were also created in this study. The
simulation was verified against the experimental results presented herein and used to develop
an extended parametric study to investigate the behavior and critical parameters influencing the
shear strength of GFRP edge connections reinforced with shear stirrups. Based on the work
presented in this paper, the following conclusions can be drawn:
• Using closed shear stirrups improved the punching behavior of GFRP-reinforced-concrete
edge-slab–column connections. The crack widths were effectively reduced, and the cracks
were more widely distributed compared to the connection without shear reinforcement,
which failed in a brittle punching-shear mode.
• The connections reinforced with GFRP shear stirrups achieved higher strains in the flexural-
reinforcement bars than their counterpart with no shear reinforcement. The GFRP stirrups
offered sufficient resistance and confinement to control the development of large shear
cracks and effectively distributed the shearing forces in the punching-shear zone, which
mobilized the flexural bars to achieve higher strains.
• The FRP shear stirrups between 1.75d and 2.25d achieved relatively high strains at 95% of
ultimate load, respectively, which implies that the FRP stirrups were still active up to 2.25d.
Further investigation, however, is needed to determine the minimum extension limit for FRP
stirrups.
• The FEA adequately predicted the experimental response of the tested GFRP-reinforced
edge-slab–column connections. The numerical results were in good agreement compared to
the experimental ones. The FE model can be an effective tool for providing insight into
behavior and the various aspects affecting punching shear in edge connections.
• The proposed design approach gave good yet conservative predications for the punching-
shear strength of GFRP-RC edge connections with different types of FRP shear
reinforcement as stirrups, studs, and corrugated bars. The proposed approach showed an
average Vtest/Vpred of 1.08 ± 0.22 with a COV of 20.40%. This approach signals an
innovation for using FRP shear stirrups in FRP-RC edge-slab–column connections. More
investigations are, however, needed to refine this proposed approach.
161
6.9. Acknowledgements
The authors wish to express their sincere gratitude to the Canada Research Chair in Advanced
Composite Materials for Civil Structures, the Natural Sciences and Engineering Research
Council of Canada (NSERC), the Fonds de recherché du Québec en Nature et technologies
(FRQ-NT) and technical staff of the structural and materials laboratory in the Department of
Civil Engineering at the University of Sherbrooke.
162
CHAPTER 7
CONCLUSIONS AND RECOMMENDATIONS
7.1. Summary
The main objective of the current research was to examine the punching-shear strength and
behavior of reinforced concrete GFRP-RC edge slab-column connections with and without
GFRP stirrups shear reinforcement. Nine full-scale connections—one reinforced with steel bars,
five reinforced with GFRP bars, and three reinforced with GFRP bars and stirrups as shear
reinforcement, were presented. The test variables were chosen to examine the effect of GFRP
stirrups type and extension, flexural reinforcement ratio and type, concrete strength, and
moment-to-shear ratios. Strength, deformation, energy absorption and failure mode of the tested
connections were investigated. Evaluation of the ultimate punching shear capacity using current
FRP codes was introduced. This was followed by a finite element parametric study using
ANSYS software to investigate the key parameters influencing the shear capacity of such
connections with FRP stirrups. Finally, a simplified design approach for edge connections with
FRP stirrups was also proposed based on the finite element parametric study. The proposed
approach was evaluated against the experimental results for the tested connections and other
specimens in the literature. based on the conducted experimental and analytical investigations,
the following concluding remarks can be drawn as follows.
7.2. Conclusions
7.2.1. GFRP–RC Edge Slab-column Connections with GFRP Stirrups
Shear Reinforcement
• Using either closed or spiral stirrups as shear reinforcement improved the punching behavior
of FRPRC edge slab–column connections. The cracks were more widely distributed
compared to the specimen without shear reinforcement, which failed in a brittle punching-
shear mode.
163
• The specimens with FRP shear reinforcement extended 4.25d demonstrated a substantial
increase in shear-strength increase over 38%, enhancement of deformation capacity of over
104%, and deformability and energy absorption of over 185%, and 194% (on average) were
observed. This increase might be of interest because it gives significant warning before
punching-shear failure occurs. As a result, these connections fail in mixed flexure–
punching-shear failure.
• The FRP stirrups offered sufficient resistance and confinement to control the development
of large shear cracks and effectively distributed the shearing forces around the punching-
shear zone so that failure occurred inside or outside the shear-reinforced zone.
• In comparison to closed stirrups, spiral stirrups provided better performance as well as fast
and easy installation during construction of the tested specimens for the same amounts of
flexural and shear reinforcement. Specimen G-SS-4.25d, with spiral stirrups, showed an
increase in the punching-shear strength, deformation capacity, and energy absorption of over
9%, 33%, and 36% compared to G-CS-4.25d, respectively. Both systems, however, could
be used to effectively reduce the brittleness of the tested specimens.
• The results indicate that the shear-stress resistance of the concrete contribution decreased
outside the shear-reinforced zone. For instance, specimen G-CS-1.75d failed outside the
shear-reinforced zone under an ultimate shear-stress resistance of 1.21 MPa (0.18 ksi),
which is 52% lower than the normalized shear-stress resistance of 2.56 MPa (0.37 ksi) for
specimen G. Thus, it is reasonable to assume the concrete contribution to shear resistance
outside the shear-reinforced zone be reduced by 50% as recommended in ACI 318 (2014)
and CSA A23.3 (2014). Further experimental tests are needed, however, to examine the
effect of FRP shear reinforcement with different extensions around the column to quantify
this effect on the concrete contribution to the shear resistance.
• FRP shear stirrups between 1.75d and 2.25d achieved relatively high strains of 4129 and
3748 µs (on average in both directions) at 95% of ultimate load, which implies that the FRP
stirrups were still active up to 2.25d, respectively. In addition, limiting the extension of the
FRP stirrups beyond 1.75d showed only limited deformation capacity and brittle punching
failure occurred. Therefore, more experimental work is needed to determine a minimum
extension limit of FRP stirrups for FRP-reinforced slab–column connections to overcome
brittle punching failure.
164 Chapter 7: Conclusions and Recommendations
• On the basis of the test results, FRP shear reinforcement can be designed with a strain value
of 4000 or 5000 microstrains, as recommended in ACI 440.1R (2015) or CSA S806 (2012),
respectively.
• The simplified approach proposed to predict the ultimate shear capacity of FRP-reinforced
edge slab–column connections with FRP shear reinforcement as an extension to those in
CSA S806 (2012) gave better predications with respect to the experimental test results as
well as the available results in the literature.
• The proposed ACI 440.1R (2015) simplified approach was consistently very conservative
for test specimens with FRP shear stirrups reported in this study and other data available in
the literature. The reason for this is the high level of conservatism of the concrete-
contribution (vc) in ACI 440.1R (2015) (Eq. 6).
• The proposed design provisions provide a step forward for engineers in designing two-way
FRPRC slabs with FRP stirrups. Nevertheless, more experimental results under eccentric
punching shear for interior and edge slab–column connections are urgently required.
• The FEA adequately predicted the experimental response of the tested GFRP-reinforced
edge-slab–column connections. The numerical results were in good agreement compared to
the experimental ones. The FE model can be an effective tool for providing insight into
behavior and the various aspects affecting punching shear in edge connections.
• The proposed design approach based on the results on the FEA analysis gave good yet
conservative predications for the punching-shear strength of GFRP-RC edge connections
with different types of FRP shear reinforcement as stirrups, studs, and corrugated bars. The
proposed approach showed an average Vtest/Vpred of 1.08 ± 0.22 with a COV of 20.40%. This
approach signals an innovation for using FRP shear stirrups in FRP-RC edge-slab–column
connections. More investigations are, however, needed to refine this proposed approach.
7.2.2. GFRP–RC Edge Slab-Column Connections without Shear
Reinforcement
• The tested connections without shear reinforcement experienced punching-shear failure as
the final mode without any signs of concrete crushing. This failure was characterized by an
165
immediate drop in the ultimate load, accompanied by the appearance of a clear crack
defining the failure surface.
• Using HSC significantly enhanced the punching-shear capacity, deflection, and initial
stiffness of the GFRP-reinforced connections. The punching-shear capacity, deflection, and
initial stiffness of the HSC connections were 18.5%, 15.5%, and 29% (on average) higher
than that of the GFRP-reinforced connections constructed with NSC, respectively. The post-
cracking stiffness, however, was similar to the NSC GFRP-reinforced connections.
• Increasing the M/V ratio from 0.3 m to 0.6 m for the NSC and HSC connections resulted in
slightly steeper shear cracks. The inclined cracks at the free edge ran in opposite direction
to the punching-shear force as a result of the reversed shear stresses caused by highly
unbalanced moment.
• Increasing the M/V ratio transferred between the slabs and columns produced significant
shear stresses that increased the likelihood of brittle failure and resulted in a reduction in the
vertical-load capacity by approximately 31% and 30% for the NSC and HSC connections,
respectively.
• The JSCE-97 (JSCE 1997) and CSA S806-12 (CSA 2012) reasonably predicted the
punching capacities of the tested connections with average of Vu test /VJSCE = 1.28 ± 0.13 and
Vu test /VCSA = 1.27 ± 0.04, respectively. The ACI 440.1R-15 (ACI 2015) equation, however,
underestimated, giving average of Vu test /VACI = 2.13 ± 0.09. In contrast, the Hassan et al.
equation (2017) overestimated the capacity of the tested connections with an average of Vu
test /VHassan = 0.88 ± 0.06.
• Using the actual concrete strengths of 85 and 86 MPa for the HSC connections (G-H-0.3
and G-H-0.6) in the CSA S806-12 (CSA 2012) equation better estimated the ultimate
capacity (Vu test /VCSA = 1.19 ± 0.08) than using the 60 MPa concrete-strength limit as per
CSA S806-12 (CSA 2012). Further research, however, is needed with a wide range of
concrete strengths.
166 Chapter 7: Conclusions and Recommendations
7.3. Recommendations for Future Work
Results of the current study represent a promising step toward implementing GFRP bars and
shear stirrups shear reinforcement in edge slab column connections. Based on the findings of
the current study, additional researches are recommended to cover the following points:
1. Elaborating more experimental works is highly needed to generate data with emphasis on
the following points;
• Different shapes of shear reinforcement including, different layout and arrangement in
FRP edge connections with high flexural reinforcement ratios;
• Different anchorage types in flexural bars normal to the free edge;
• Effect of column aspect ratio and shear perimeter-to- slab depth ratio;
• Effect of openings in the column vicinity;
• Effect of different slab thicknesses;
• Edge connections with different column sizes;
• Existence of marginal beam at the free edge of the connection; and
• Effect of different sizes of drop panels.
2. Development an alternative design equation for the current punching shear equations in ACI
440.1R-15 and CSA S806-12 design codes including the most affecting paraments.
3. Development of mechanical model that can reasonably predict the punching shear capacity
of FRP edge connections with shear reinforcement based on the interaction between shear
and unbalanced moment.
4. Study the effect of reversed cyclic unbalanced moment on the behavior edge slab column
connections reinforced with and without FRP shear reinforcement.
5. One further step is to study the punching shear strength and performance of GFRP corner
slab-column connections.
7.4. Résumé
L’objectif principal du présent projet de recherche était d’examiner la résistance au
poinçonnement et le comportement des jonctions dalle-poteau en béton armé de PRFV avec et
sans armatures de cisaillement constituées d’étriers en PRFV. Neuf (9) jonctions pleine grandeur
167
(une jonction avec des barres d’armature en acier à des fins de comparaison, cinq jonctions avec
uniquement des barres d’armature en flexion en PRFV et trois jonctions avec des barres et des
étriers en PRFV comme armatures de cisaillement) ont été étudiées. Les paramètres d’essais ont
été choisis pour examiner l’effet du type d’étrier en PRFV et leur prolongement, l’effet du type
et du taux d’armature en flexion, l’effet de la résistance en compression du béton, et l’effet des
rapports moment/cisaillement. La résistance, la déformation, l'absorption d'énergie et les modes
de rupture des jonctions testées ont été étudiés. L'évaluation de la résistance ultime de
poinçonnement à l’aide des codes de conception actuels sur les PRF a été présentée. Ensuite,
une étude paramétrique par éléments finis à l’aide du logiciel ANSYS a été réalisée pour étudier
les principaux paramètres influençant la résistance au cisaillement de telles jonctions. Enfin,
deux méthodes simplifiées de calcul pour les jonctions de rive sans et avec étriers en PRF ont
également été proposées sur la base de l'étude paramétrique par éléments finis. Les méthodes
proposées ont été évaluées à l’aide des résultats expérimentaux obtenus des essais sur les
jonctions et d’autres spécimens dans la littérature. Sur la base des études expérimentales et
analytiques menées, les conclusions finales suivantes peuvent être tirées ci-après.
7.5. Conclusions
7.5.1. Jonctions PRV–RC Bord Dalle-Colonne avec Étriers PRV Renfort
de Cisaillement
• L’utilisation d’étriers fermés ou à spirale comme renfort de cisaillement a amélioré le
comportement de poinçonnage des raccords de la dalle et de la colonne du bord du FRPRC.
Les fissures étaient plus largement réparties que l’éprouvette sans renfort de cisaillement,
qui s’est rompue en mode de cisaillement fragile.
• Les éprouvettes avec renfort en cisaillement FRP prolongé 4.25d ont montré une
augmentation substantielle de la résistance au cisaillement de plus de 38%, une
augmentation de la capacité de déformation de plus de 104%, et une déformabilité et une
absorption d’énergie de plus de 185%, et 194% (en moyenne) ont été observés. Cette
augmentation pourrait être intéressante parce qu’elle donne un avertissement important
168 Chapter 7: Conclusions and Recommendations
avant qu’une rupture de poinçonnage-cisaillement ne se produise. Par conséquent, ces
raccords se rompent en cas de rupture mixte flexion-poinçonnage-cisaillement.
• Les étriers FRP offraient une résistance et un confinement suffisants pour contrôler le
développement de grandes fissures de cisaillement et répartissaient efficacement les forces
de cisaillement autour de la zone de cisaillement de façon à ce que la rupture se produise à
l’intérieur ou à l’extérieur de la zone de cisaillementzone renforcée.
• Par rapport aux étriers fermés, les étriers hélicoïdaux ont fourni de meilleures performances
ainsi qu’une installation rapide et facile pendant la construction des éprouvettes testées pour
les mêmes quantités de renfort de flexion et de cisaillement. L’éprouvette G-SS-4.25d, avec
étriers hélicoïdaux, a montré une augmentation de la résistance au cisaillement, de la
capacité de déformation et de l’absorption d’énergie de plus de 9 %, 33 % et 36 % par rapport
à G-CS-4.25d, respectivement. Cependant, les deux systèmes pourraient être utilisés pour
réduire efficacement la fragilité des éprouvettes testées.
• Les résultats indiquent que la résistance au cisaillement de l’apport de béton a diminué en
dehors de la zone de cisaillement. Par exemple, l’éprouvette G-CS-1.75d s’est rompue à
l’extérieur de la zone renforcée de cisaillement sous une résistance ultime à la contrainte de
cisaillement de 1.21 MPa (0.18 ksi), ce qui est inférieur de 52 % à la résistance normalisée
à la contrainte de cisaillement de 2.56 MPa (0.37 ksi) pour l’éprouvette G. Ainsi, il est
raisonnable de supposer que la contribution du béton à la résistance au cisaillement à
l’extérieur de la zone renforcée par cisaillement soit réduite de 50 %, comme le
recommandent l’ACI 318 (2014) et la norme CSA A23.3 (2014). D’autres essais
expérimentaux sont cependant nécessaires pour examiner l’effet du renforcement en
cisaillement FRP avec différentes extensions autour de la colonne afin de quantifier cet effet
sur la contribution du béton à la résistance au cisaillement.
• Les étriers de cisaillement FRP entre 1.75d et 2.25d ont obtenu des déformations
relativement élevées de 4129 et 3748 µs (en moyenne dans les deux sens) à 95% de la charge
ultime, ce qui signifie que les étriers FRP étaient encore actifs jusqu’à 2.25d, respectivement.
De plus, le fait de limiter le prolongement des étriers en PRF au-delà de 1.75d n’a montré
qu’une capacité de déformation limitée et une rupture de poinçonnage fragile s’est produite.
Par conséquent, des travaux plus expérimentaux sont nécessaires pour déterminer une limite
169
d’extension minimale des étriers en PRF pour les raccordements PRF renforcés de la dalle
et de la colonne afin de surmonter la rupture de poinçonnage fragile.
• Sur la base des résultats des essais, le renforcement en cisaillement FRP peut être conçu
avec une valeur de déformation de 4000 ou 5000 microstrains, comme le recommande l’ACI
440.1R (2015) ou la norme CSA S806 (2012), respectivement.
• L’approche simplifiée proposée pour prévoir la capacité de cisaillement ultime des raccords
de dalle-colonne renforcés en PRF avec renfort de cisaillement en PRF comme
prolongement de ceux de la norme CSA S806 (2012) a donné de meilleures prédications en
ce qui concerne les résultats des tests expérimentaux ainsi que les résultats disponibles dans
la littérature.
• L’approche simplifiée proposée dans l’ACI 440.1R (2015) était toujours très prudente pour
les spécimens d’essai avec étriers de cisaillement en PRF signalés dans cette étude et
d’autres données disponibles dans la littérature. La raison en est le haut niveau de
conservatisme de la contribution concrète (vc) dans l’ACI 440.1R (2015) (Eq. 6).
• Les dispositions de conception proposées représentent un pas en avant pour les ingénieurs
dans la conception de plaques FRPRC bidirectionnelles avec étriers FRP. Néanmoins, des
résultats plus expérimentaux sous cisaillement excentrique de poinçonnage pour les
raccordements intérieurs et de bord dalle-colonne sont urgents.
• La FEA a adéquatement prédit la réponse expérimentale des raccords GFRP-dalle-bord-
colonne renforcés testés. Les résultats numériques concordent bien avec les résultats
expérimentaux. Le modèle FE peut être un outil efficace pour fournir des informations sur
le comportement et les différents aspects affectant le cisaillement de poinçonnage dans les
raccords de bord.
• L’approche de conception proposée basée sur les résultats de l’analyse de la FEA a donné
de bonnes bases, mais prudentes, pour la résistance au poinçonnage-cisaillement des
raccords de bord de la GFRP-RC avec différents types de renfort de cisaillement en FRP
comme étriers, goujons et barres ondulées. L’approche proposée montrait un Vtest/Vpred
moyen de 1,08±0.22 avec un COV de 20.40 %. Cette approche signale une innovation pour
l’utilisation des étriers de cisaillement FRP dans les raccordements FRP-RC bord-dalle-
colonne. D’autres enquêtes sont toutefois nécessaires pour peaufiner cette approche
proposée.
170 Chapter 7: Conclusions and Recommendations
7.5.2. Jonctions PRV–RC Bord Dalle-Colonne sans Armatures de
Cisaillement
• Les raccords testés sans renfort de cisaillement ont subi une rupture de cisaillement comme
mode final sans aucun signe de concassage du béton. Cette rupture a été caractérisée par
une chute immédiate de la charge ultime, accompagnée de l’apparence d’une fissure claire
définissant la surface de rupture.
• L’utilisation du HSC a considérablement amélioré la capacité de poinçonnage-cisaillement,
la déflexion et la rigidité initiale des raccords renforcés par la PRV. La capacité de
poinçonnage-cisaillement, la déflexion et la rigidité initiale des raccords HSC étaient de
18.5 %, 15.5 % et 29 % (en moyenne) supérieures à celles des raccords renforcés PRV
construits avec du NSC, respectivement. La rigidité postérieure à la fissuration était toutefois
semblable aux raccords renforcés NSC GFRP.
• L’augmentation du rapport M/V de 0.3 m à 0.6 m pour les raccords NSC et HSC a entraîné
des fissures de cisaillement légèrement plus prononcées. Les fissures inclinées au bord libre
allaient dans une direction opposée à la force de poinçonnage-cisaillement en raison des
contraintes de cisaillement inversées causées par un moment très déséquilibré.
• Le JSCE-97 (JSCE 1997) et le CSA S806-12 (CSA 2012) ont raisonnablement prédit les
capacités de poinçonnage des raccords testés avec une moyenne de Vu test /VJSCE = 1.28±0.13
et Vu test /VCSA = 1.27±0.04, respectivement. L’équation de l’ACI 440.1R-15 (IPEC 2015) a
toutefois été sous-estimée, ce qui donne une moyenne de l’essai de l’ACI Vu test /VACI =
2.13±0.09. En revanche, l’équation de Hassan et al. (2017) a surestimé la capacité des
connexions testées avec une moyenne de Vu test /VHassan = 0.88±0.06.
• En utilisant la résistance réelle du béton de 85 et 86 MPa pour les raccords HSC (G-H-0.3
et G-H-0.6) dans l’équation de la norme CSA S806-12 (CSA 2012), on estime mieux la
capacité ultime (Vu test /VCSA = 1.19±0.08) qu’en utilisant le béton de 60 MPa-limite de
résistance conformément à la norme CSA S806-12 (CSA 2012). Des recherches plus
poussées sont toutefois nécessaires avec un large éventail de points forts concrets.
171
7.6. Recommandations pour des Travaux Futurs
Les résultats de la présente étude représentent une étape prometteuse dans l’application de barres
d’armature et des étriers de cisaillement en PRFV dans les jonctions de dalle-poteau de rive. Sur
la base des conclusions de l’étude actuelle, il est recommandé d’effectuer des recherches
supplémentaires pour couvrir les points suivants :
1. Il est indispensable de développer davantage de travaux expérimentaux pour générer des
données tout en mettant l’accent sur les points suivants :
• Différentes formes d’armatures de cisaillement, y compris différentes dispositions et
agencements dans les jonctions de rive en PRF avec des taux d’armature en flexion
élevés ;
• Différents types d'ancrages pour les armatures de flexion perpendiculaires au côté libre ;
• Effet des sections du poteau et du rapport profondeur du périmètre de
cisaillement/épaisseur de la dalle ;
• Effet des ouvertures au voisinage du poteau ;
• Effet de différentes épaisseurs de dalle ;
• Jonctions de rive avec différentes dimensions de poteau ; et
• Présence de poutre périphérique sur le bord libre de la jonction.
• Effet de différentes dimensions de panneaux de retombée.
2. Élaborer une équation alternative à l’équation de calcul du poinçonnement des guides et
normes de conception de l’ACI 440.1R-15 et de la CSA S806-12, en tenant compte des
paramètres les plus importants.
3. Développement d'un modèle mécanique permettant de prédire de manière raisonnable la
résistance au cisaillement des jonctions de rive en PRF en se basant sur l'interaction entre le
cisaillement et le moment non équilibré.
4. Étudier l’effet du moment cyclique inversé non équilibré sur le comportement des jonctions
dalle-poteau de rive avec et sans armatures de cisaillement en PRF.
5. Une autre étape consiste à étudier la résistance au cisaillement et les performances des
jonctions dalle-poteau de coin en béton armé de PRFV
172
BIBLIOGRAPHY
AASHTO (American Association of State Highway and Transportation Officials). (2009).
“AASHTO LRFD bridge design guide specifications for GFRP–reinforced concrete bridge
decks and traffic railings.” Washington, D.C.
ACI (American Concrete Institute). (2012). “Guide Test Methods for Fiber-Reinforced
Polymers (FRPs) for Reinforcing or Strengthening Concrete Structures.” ACI 440.3R-12,
Farmington Hills, MI.
ACI (American Concrete Institute). (2014). “Building code requirements for structural concrete
and commentary.” ACI 318-14, Farmington Hills, MI.
ACI (American Concrete Institute). (2015). “Guide for the design and construction of structural
concrete reinforced with fiber-reinforced polymer bars.” ACI 440.1R-15, Farmington Hills,
MI.
ACI-ASCE Committee 445 on Shear Torsion. (1998). “Recent approaches to shear design of
Ahmed, E. A., Settecasi, F., and Benmokrane, B., (2014). “Construction and testing of steel-
GFRP hybrid-reinforced-concrete bridge-deck slabs of the Ste-Catherine overpass bridges.”
J. Bridge Eng., 10.1061/(ASCE) BE.1943-5592.0000581, 04014011.
Ahmed, E.; Benmokrane, B.; and Sansfaçon, M. (2017). “Case Study: Design, Construction,
and Performance of the La Chancelière Parking Garage’s Concrete Flat Slabs Reinforced
with GFRP Bars,” J. Comp. Constr., 21(1), 10.1061/(ASCE)CC.1943-5614.0000656.
Arafa, A., (2017). “Assessment of strength, stiffness, and deformation capacity of concrete
squat walls reinforced with GFRP bars.” Ph.D. Thesis, Sherbrooke Univ., Canada.
ASTM. (2011). “Standard test method for tensile properties of fiber reinforced polymer matrix
composite bars.” ASTM D7205/D7205M, West Conshohocken, PA.
173
Bedard, C. (1992). “Composite reinforcing bars: assessing their use in construction.” Conc.
Inter., 14(1), 55-59.
Benmokrane, B., Ahmed, E., Dulude, C., and Boucher, E. (2012). “Design, construction, and
monitoring of the first worldwide two-way flat slab parking garage reinforced with GFRP
bars.” Proc., 6th Int. Conf. on FRP Comp. Civ. Eng., Università di Roma.
Benmokrane, B., El-Salakawy, E., El-Gamal, S., and Goulet, S, (2007). “Construction and
testing of an innovative concrete bridge deck totally reinforced with glass FRP bars: Val-
Alain Bridge on Highway 20 East.” J. Bridge Eng., 10.1061/(ASCE)1084-
0702(2007)12:5(632), 632–645.
Broms, C.E., (1990). “Punching of Flat Plates - A Question of Concrete Properties in Biaxial
Compression and Size Effect.” ACI Str. J., 87, 292-304
Büyükkaragöz, A. (2010). “Finite element analysis of the beam strengthened with prefabricated
reinforced concrete plate.” Scientific Research and Essays, 5(6), 533–544.
Chaallal, O., and Benmokrane, B. (1993). “Physical and Mechanical Performance of an
Innovative Glass-Fiber-Reinforced Plastic Rod.” Can. J. Civ. Eng., 20(2), 254-268.
Chansawat, K., Yim, S., Miller, TH. (2011) “Nonlinear finite element analysis of a FRP
strengthened reinforced concrete bridge.” J Bridge Eng., 11(1), 21–32.
CSA (Canadian Standard Association). (2014). “Design of concrete structures.” CAN/CSA-
A23.3-14, Rexdale, Ontario, Canada.
CSA (Canadian Standards Association). (2012). “Design and construction of building structures
with fiber reinforced polymers,” CAN/CSA S806-12, Rexdale, Ontario, Canada.
CSA (Canadian Standards Association). (2014). “Canadian highway bridge design code.”
CAN/CSA S6-14, Rexdale, Ontario, Canada.
174 Bibliography
CSA (Canadian Standards Association). (2015). “Specification for fiber reinforced polymers,”
CAN/CSA S807-15, Rexdale, Ontario, Canada.
Dam, Thai X., Wight, James K., and Parra-Montesinos, Gustavo J., (2017). “Behavior of
Monotonically Loaded Slab-Column Connections Reinforced with Shear Studs.” ACI
Str. J., 114(1), 221-232.
De Luca, A., Matta, F., and Nanni, A. (2009). “Behavior of full-scale concrete columns
internally reinforced with glass FRP bars under pure axial load.” COMP. & POLY. 2009,
Amer. Comp. Manuf. Asso., Tampa, FL USA, 1-10.
Deiveegan, A., and Kumaran, G. (2009). “Reliability analysis of concrete columns reinforced
internally with glass fiber reinforced polymer reinforcement.” ICFAI Univ. J. Struct.
Eng., 2(2), 49–59.
Desayi, P., Krishnan, S. (1964) “Equation for stress–strain curve of the concrete.” ACI str. J.
61(3), 345–50.
Design Manual No.3, (2007). “Reinforcing concrete structures with fiber reinforced
polymers.” Int. Sen. Innov. Str. Canada, Winnipeg, MB, Canada.
Dulude, C., Hassan, M., Ahmed, E., and Benmokrane, B. (2013). “Punching shear behavior of
flat slabs reinforced with glass fiber-reinforced polymer bars.” ACI Struct. J., 110(5), 723–
734.
Elgabbas, F., Ahmed, E. and Benmokrane, B., (2016). “Experimental Testing of Concrete
Bridge Deck Slabs Reinforced with Basalt-FRP Reinforcing Bars under Concentrated
Loads.” J. Brid. Eng., 10.1061/(ASCE)BE.1943-5592.0000892.
Elgabry, A. and Ghali, A., (1996). “ Transfer of moments between columns and slabs.” ACI Str.
J. 93, 56 61.
Elgabry, A.,(1991)."Shear and Moment Transfer of Concrete Flat Plates” Ph.D. Thesis, Univ.
of Calgary.
175
Elgabry, Adel A. and Ghali, Amin, (1987). “Design of stud-shear reinforcement for slabs.” ACI
Str.J.,87(3), 350-361
El-Gendy, M., and El-Salakawy, E. (2016). “Effect of shear studs and high moments on
punching behavior of GFRP-RC slab-column edge connections.” J. Compos. Constr.,
10.1061/(ASCE)CC.1943-5614.0000668, 04016007.
El-Gendy, M., and El-Salakawy, E., (2018). “Punching Shear Behavior of GFRP-RC Slab-
Column Edge Connections.” ACI SP, SP-322, 5.1-5.20.
El-Ghandour, A. W., Pilakoutas, K., and Waldron, P. (2003). “Punching shear behavior of fiber
reinforced polymers reinforced concrete flat slabs: Experimental study.” J. Compos. Constr.,
10.1061/(ASCE)1090-0268(2003)7:3(258).
El-Mogy, M., El-Ragaby, A., and El-Salakawy, E. (2010). “Experimental testing and finite
element modeling on continuous concrete beams reinforced with fiber reinforced polymer
bars and stirrups.” Can. J. Civ. Eng., 40 (11), 1091–1102.
El-Salakawy, E., Polak, M., and Soliman, M. (1998). “Slab-column edge connections subjected
to high moments.” Can. J. Civ. Eng., 25(3), 526–538.
El-Salakawy, E., Polak, M., and Soliman, M. (2000). “Reinforced concrete slab-column edge
connections with shear studs.” Can. J. Civ. Eng., 27(2), 338–348.
El-Salakawy, E.F., Polak, M.A., and Soliman, M.H. (1998). “Slab-column edge connections
subjected to high moments.” Can. J. of Civ. Eng., 25(3), 526–538.
El-Salakawy, E.F., Polak, M.A., and Soliman, M.H. (2000). “ Reinforced concrete slab –
column edge connections with shear studs.” Can. J. Civ. Eng., 27(2),338–348.
Gardner, N.J., (1990). “Relationship of the punching shear capacity of reinforced concrete slabs
with concrete strength.” ACI Str. J.,87,66-71.
176 Bibliography
Gorji, M.S. (2009). “Analysis of FRP strengthened reinforced concrete beams using energy
variation method.” World App. Sci. J. 6 (1), 105–111.
Gouda, A., and El-Salakawy, E. (2015). “Punching shear strength of GFRPRC interior slab-
column connections subjected to moment transfer.” J. Compos. Constr.,
10.1061/(ASCE)CC.1943-5614.0000597, 04015037.
Gouda, A., and El-Salakawy, E. (2016). “Behavior of GFRP-RC interior slab-column
connections with shear studs and high-moment transfer,” J. Compos. Constr.,
10.1061/(ASCE)CC.1943-5614.0000663.
Hassan, M., Ahmed, E. A., and Benmokrane, B. (2013a). “Punching-shear strength of GFRP-
reinforced concrete flat slabs,” Can. J. of Civ. Eng., 40(10), 951-960.
Hassan, M., Ahmed, E. and Benmokrane, B, (2014 a), “Punching shear behavior of two-way
slabs reinforced with FRP shear reinforcement.” J. Compos. Constr.,
10.1061/(ASCE)CC.1943-5614.0000493.10.1061/(ASCE).
Hassan, M., Ahmed, E., and Benmokrane, B. (2013 b). “Punching-shear strength of normal and
high-strength two-way concrete slabs reinforced with GFRP bars.” J. Compos. Constr.,
10.1061/(ASCE)CC.1943-5614.0000424, 04013003.
Hassan, M.; Ahmed, E.; and Benmokrane, B, (2014 b), “Punching-shear design equation for
two-way concrete slabs reinforced with FRP bars and stirrups.” Constr. and Build. Mat., 66,
pp. 522-532.
Hassan, M.; Fam, A., Benmokrane, B., and Ferrier, E. (2017). “Effect of column size and
reinforcement ratio on shear strength of glass fiber-reinforced polymer reinforced concrete
two-way slabs.” ACI Struct. J., 114(4), 937-950.
177
Hussein, A. H., and El-Salakawy, E. (2018). “Punching Shear Behavior of Glass Fiber-
Reinforced Polymer-Reinforced Concrete Slab-Column Interior Connections.” ACI Struct.
J., 115(4),1075-1088.
Issa, M. S., Metwally, I. M., and Elzeiny, S. M. (2011). “Structural performance of eccentrically
loaded GFRP reinforced concrete columns.” Int. J. Civ. Struct. Eng., 2(1), 395–404.
Jaeger, L. G., Mufti, A., and Tadros, G. (1997). “The concept of the overall performance factor
in rectangular- section reinforced concrete beams.” Proce., the Third Int. Symp.
Nonmetallic (FRP) Reinf. for Conc. Str. (FRPRCS-3), Japan Con. Inst., Sapporo, Japan,
2, 551-558.
JSCE (Japan Society of Civil Engineers). (1997). “Recommendation for design and construction
of concrete structures using continuous fiber reinforcing materials.” Concrete engineering,
A. Machida, ed., Tokyo.
Kachlakev, D., Miller, T., Yim, S., Chansawat, K., and Potisuk, T. (2001).“Finite Element
Modeling of Reinforced Concrete Structures strengthened with FRP Laminates.” Final
Report SPR-316, Oregon Dept. of Trans., Salem, Oregon.
Kinnunen S., Nylander H., (1960). “Punching of Concrete Slabs without Shear Reinforcement.”
Royal Institute of Technology Stockholm, Sweden.
Lee, J.H., Yoon, Y.S., and Mitchell, D. (2009). “Improving Punching Shear Behavior of Glass
Fiber-Reinforced Polymer Reinforced Slabs.” ACI Structural Journal, 106 (4), 427– 434.
Lips, S.; Ruiz, M.; and Muttoni A. (2012). “Experimental Investigation on Punching Strength
and Deformation Capacity of Shear-Reinforced Slabs.” ACI Structural Journal, 109 (6), 889-
900.
Marzouk, H., Emam, M., and Hilal, S, (1996). “Effect of High-Strength Concrete Columns on
the Behavior of Slab-Column Connections.” ACI Struct. J., 93(5), 545–555.
178 Bibliography
Marzouk, H., Imam, M., and Hilal, M. (1998). “Effect of High-Strength Concrete Slab on the
Behavior of Slab-Column Connections.” ACI Struct. J., 95(3), 227-236.
Megally, S., and Ghali, A. (2000) “Seismic behavior of slab-column connections.” Can. J. Civ.
Eng., 27(1), 84-100.
Mokhtar, A., Ghali, A., and Dilger, W., (1985). “Stud shear reinforcement for flat concrete
plates.” ACI J. Pro. 82(5),676-683.
Morphy, R., Shehata, E., and Rizkalla, S. (1997). “Bent Effect on Strength of CFRP Stirrups.”
Proce., the Third International Symposium on Nonmetallic (FRP) Reinforcement for
Concrete Structures (FRPRCS-3).” Sapporo, Japan, 2, 19-26.
Mortin, D., and Ghali, A., (1991). “Connection of flat plates to edge columns” ACI Str. J., 88(2).
Mostafa, A., and El-Salakawy, E. (2018). “Behavior of GFRP-RC Slab–Column Edge
Connections with High-Strength Concrete and Shear Reinforcement.” J. of Compos. Constr.,
10.1061/(ASCE)CC.1943-5614.0000831.
Mostofinejad, D., and Talaeitaba, S.B. (2006). “Finite element modeling of RC connections
strengthened with FRP laminates.” Ira. J. Sci. Tec., 30, 21–30.
Nanni, A. (1993). “Flexural behavior and design of reinforced concrete using FRP rods.” J. Str.
Eng., 119 (11), 3344 – 3359.
National Research Council of Canada. (2015). “National building code of Canada.” NBCC 2015,
Ottawa.
Nguyen-Minh, L., and Rovnak, M. (2013). “Punching-shear resistance of interior GFRP
reinforced slab-column connection.” J. Compos. Constr., 10.1061/(ASCE)CC.1943-
5614.0000324, 2–13.
Ospina, C. E., Alexander, S. D. B. and Cheng, J. J. R. (2003). “Punching of Two-Way Concrete
Slabs with Fiber- Reinforced Polymer Reinforcing Bars or Grids.” ACI Struct. J., 100 (5),
589-598.
179
Özcan DM, Bayraktar A, Sahin A, Haktanir T, Türker T. (2009). “Experimental and finite
element analysis on the steel fiber-reinforced concrete (SFRC) beams ultimate behavior.”
Const. Build. Mat. , 23 (2), 1064 –1077.
Ozden, S., Ersoy, U., and Ozturan, T., (2006). “Punching Shear tests of normal- and high-
strength concrete flat plates,” Can. J. Civ. Eng., 33(11), 1389-1400.
Park, R., and Gamble, W. (1980). “Reinforced concrete slabs.” Wiley, New York.
Perera, U. (2005). “Seismic Performance of Concrete Beam-Slab-Column Systems Constructed
with a Re-Useable Sheet Metal Formwork System.” M.Sc. Thesis, Univ. of Melbourne,
Victoria, Australia.
Phillips, L.N. (1989). “Design with Advanced Composite Materials.” Springer- Verlag.
Pultrall, (2016). “Technical Data Sheet.” www.pultrall.com.
Razaqpur, A. G., Isgor, O. B., Cheung, M. S., and Wiseman, A. (2001). “Background to shear
design provisions of the proposed Canadian standard for FRP reinforced concrete
structures.” Proc., Int. Conf. Comp. Const., Porto, Portugal, 403 – 408.
Razaqpur, A. G., Isgor, O. B., Greenaway, S., and Selley, A. (2004). “Concrete contribution to
the shear resistance of FRP reinforced concrete members.” J. Comp. Const., ASCE,
8(5), 452-460.
Reilly, J. L., Cook W., Bastien J., and Mitchell D., (2014). “Effects of delamination on the
performance of two-way reinforced concrete slabs.” J. of Compos. Constr.,
10.1061/(ASCE)CF.1943-5509.0000457.
Rosenthal, I., (1959). “Experimental investigation of flat plate floors.” ACI J. pro., 56, 153-166.
Salama, A., (2016) “punching shear behaviour of concrete edge slab–column connection
reinforced with glass fiber reinforced polymer (GFRP) bars” Définition du Projet de
Recherche au Doctorat, Sherbrooke university, QC, Canada.
180 Bibliography
Seible, F., Ghali, A., and Dilger, W., (1980). “Preassembled shear reinforcing units for flat
plates.” ACI J. Pro.,77(l), 28-35.
Shehata, E., Morphy, R. and Rizkalla, S. (2000). “Fiber Reinforced Polymer shear
reinforcement for concrete members: behavior and design guidelines.” Can. J. Civ. Eng.,
27, 859-872.
Shehata, I.AE.M. and Regan, P.E., (1989). “Punching in R.C. Slabs.” ASCE J. Str. Eng., 115
(7), 1726-1740
Sherif, A.G., (1996). “Behaviour of reinforced concrete flat slabs.” Ph.D. Thesis, ,
Univ. of Calgary, Alta.
Stamenkovic, A., and Chapman, J.C. (1972). “Local strength of flat slabs at column heads.”
Report 39, Constr. Indust. Res. and Info. Asso., London, U.K., 205–232.
structural concrete.” J. Str. Eng., 124 (12), 1375–1417.
Tavassoli, A., Liu, J., and Sheikh, S. (2015). “Glass fiber-reinforced polymer-reinforced circular
columns under simulated seismic loads” ACI Str. J., 112(10), 103–114.
Wolanski, A.J. (2004). “Flexural behavior of reinforced and prestressed concrete beams using
finite element analysis.” M.Sc. Thesis, Marquette University, Milwaukee, Wisconsin.
Wu, W. P. (1990). “Thermomechanical Properties of Fiber Reinforced Plastic (FRP) Bars.”
Ph.D. Thesis, West Virginia University, Morgantown, W.Va., 292 pp.
Zaghlool, E.R.F. (1971). “Strength and behavior of corner and edge column–slab connections
in reinforced concrete flat plates.” Ph.D. thesis, Department of Civil Engineering, The
University of Calgary, Calgary, Alta.
Zaghlool, E.R.F., de Paiva H.A.R., (1973-a). “Strength analysis of comer column-slab
connection” J. Str. Div., ASCE, 99(ST1), Proc., 53-70.
Zaghlool, E.R.F., de Paiva H.A.R., (1973-b). “ Tests of flat plate comer column- slab
connection” J. Str Div., ASCE Pro., 99(ST3), 551-572.
181
Zaghloul, A. (2002). “Behaviour and Strength of CFRP-Reinforced Flat Plate Interior Column
Connections Subjected to Shear and Unbalanced Moments.” M.Sc. Thesis, Carleton Univ.,
Ottawa, ON, Canada.
Zaghloul, A. E., Razaqpur, A. G., and Zaghloul, E.R. (2004). “Refined Prediction of Punching
Shear Strength of Slab-Column Connections: Applications to Slab Reinforced with Steel or
FRP.” 4th Inter. Conf. on Adv. Compos. Mat. in Brid. and Struct., Calagary, Alberta, 20-23.
Zaghloul, A., (2007). “Punching shear strength of interior and edge column-slab connections in
CFRP reinforced flat plate structures transferring shear and moment.” Ph.D. Thesis, Carleton
univ., Ottawa, ON, Canada.
Zhang, Q. (2004). “Finite element application to slab-column connections reinforced with glass
fiber-reinforced polymers.” M.Sc. thesis, Memorial Univ., Newfoundland, St. John's,
Canada.
Zhang, Q., Marzouk, H., and Hussein, A., (2005). “A Preliminary Study of High Strength
Concrete Two-Way Slabs Reinforced with GFRP Bars.” Proceedings, 33rd CSCE Ann.
Conf., Can. Soc. Civ. Eng., Toronto, ON, Canada.
182
APPENDIX
1.1. Introduction
This chapter represents the calculations of flexure design and punching shear capacity
predictions of the test connections that were reported and discussed in chapter 4 and 5. The
flexural design of the connections for flexure is completed in accordance with the Canadian
codes CSA A23.3-14 and CSA S806-12. However, the punching-shear capacity of the
connections with and without shear reinforcement were predicted using new proposed equations
and available equations in FRP codes and guides, CSA S806-12, ACI 440.1R-15 and JSCE-97,
respectively.
1.2. Analysis of Prototype Structure
The prototype structure is a parking garage flat-plate structure with 5 × 5 m2 square panels as
shown in Fig A.1. The edge slab-column connection is bounded by the lines of contra flexure
in the prototype floor, and monolithic with a column at the middle of the free edge. The parking
garage flat plate structure is analysed using Equivalent Frame Method in CSA A23.3-14. In the
equivalent frame method, the 3D flat-plate structure is idealized into 2D frames along column
centre lines in both longitudinal and transverse directions, X and Y frames as shown in Figure
A.1. Each equivalent frame shall consist of a row of columns and slab-beam strips bounded
laterally by the panel centreline on each side of the centreline of columns. for analysis of each
equivalent frame, a separate analysis can be carried for each floor with the fixed far ends of
columns under gravity loading. The selected X and Y frames were analysed to determine their
straining actions, bending moment and shear. Consequently, the applied M/V ratio and amount
of flexural reinforcement can be estimated for the selected connection. The selected connection
is located at the interstation between the centrelines A and 3.
1.2.1. Concrete Dimensions and Loads
• Concrete Dimensions
- Slab Thickness (ts) = 200 mm
- Column Dimensions (c1 × c2) =300 × 300 mm
183
• Service and Ultimate Loads
The loads were specified according to the National Building Code of Canada (NBCC 2015)
2. c sw γ t Partations 24 0.2 1.0 5.8 KN /mD L = + = + = ,
2. W 2.4 KN / mL L =
2. .w w w 5.8 2.4 8.2 KN / ms D L L L= + = + =
2.
2. .
1.4 w 1.4 5.8 8.12 / mw max
1.25W 1.5W 1.25 5.8 1.5 2.4 10.85 / m
D Lf
D L L L
kN
kN
= ==
+ = + =
1.2.2. Analysis of the Equivalent 2D Frame in X-direction
• Slab-Beam Stiffness and Fixed End Moment
For span A3−B3 at end A
- C1
𝑙1=
300
5000= 0.06,
C2
𝑙2=
300
5000= 0.06 → 𝑘 = 4.067, 𝐶𝑂𝐹 = 0.505 (Table A. 1)
- 𝐼𝑠 =𝑙2 𝑡𝑠
3
12=
5000×2003
12= 3333 × 106 mm4
- 𝐾𝐴3−𝐵3 =𝑘 𝐸𝑐𝐼𝑠
𝑙1=
4.067 ×3333×106×𝐸𝑐
5000= 2711062 𝐸𝑐
(𝑀𝐹.𝐸.𝑀)𝑓 = 0.084 wf l2 l12 = 0.084 × 10.85 × 5 × 52 = 113.93 kN.m
Note: The remaining spans will have the same values because they have the same geometry as
well as the fixed end moment is constant of each span.
• Equivalent Column Stiffness (Kec)
The equivalent column stiffness (Kec) represents the combined stiffens of the column (Kc) and
attached torsional members (Kt), where the column is assumed to be attached to the slab by the
transverse torsional members.
1
𝐾𝑒𝑐=
1
Σ𝐾𝑐+1
𝐾𝑡
184 Appendix
Figure A.1 – Plan of flat plate prototype
For column A3, the equivalent column stiffness was calculated as follows
Torsional member stiffness (Kt)
The factor (C) in the torsional member stiffness equation defines the cross section of the
torsional members. The attached torsional members at the exterior column is a portion of the
slab having width equal to column width y and depth equals slab thickness x (refer to Fig A.2a).
20
0
5
4
3
2
1
A B C D E
A B C D E
5
4
3
2
1
Y-Frame
X-Frame
5m 5m 5m 5m
5m
5
m
5m
5
m
2.5
m
1.35 m
Design specimen
2.65 m
5 m
185
The Torsional member stiffness (Kt) was multiplied by 2 because two similar torsional members
meet at column A3. The values of Kt for all other columns will be the same as column A3
because of similar column dimensions.
C = Σ (1 − 0.63 x
y) x3 y
3= (1 − 0.63
200
300) 2003 × 300
3= 464 × 106 mm4
𝑘𝑡 = Σ 9 𝐸𝑐 C
𝑙2 (1−𝑐2𝑙2)3 = 2 ×
9 ×E𝑐 × 464 × 106
5000(1− 300
5000)3 = 2011115 𝐸𝑐
Column stiffness (Kc)
The column stiffness (Kc) was multiplied by 2 for interior story with similar columns above and
below
𝑙𝑐
𝑙𝑢=
3200
3000= 1.07,
ta
tb= 1 → 𝑘𝐴𝐵 = 4.748, CAB = 0.55 (Table A. 2)
Σ𝐾𝑐 =𝑘 𝐸𝑐 𝐼𝐶
𝑙𝑐= 2 ×
4.748× 𝐸𝑐×(3004
12)
3200= 2003063 𝐸𝑐
Table A.1 – Moment-Distribution Factors for flat plates (Wight and MacGregor 2011)
Carryover factor = COF
c2 / l2
c1 / l1 0.00 0.05 0.10 0.15 0.20 0.25
0.00 M 0.083 0.083 0.083 0.083 0.083 0.083
k 4.000 4.000 4.000 4.000 4.000 4.000
COF 0.500 0.500 0.500 0.500 0.500 0.500
0.05 M 0.083 0.084 0.084 0.084 0.085 0.085
k 4.000 4.047 4.093 4.138 4.181 4.222
COF 0.500 0.503 0.507 0.510 0.513 0.516
0.10 M 0.083 0.084 0.085 0.085 0.086 0.087
k 4.000 4.091 4.182 4.272 4.362 4.449
COF 0.500 0.506 0.513 0.519 0.524 0.530
0.15 M 0.083 0.084 0.085 0.086 0.087 0.088
k 4.000 4.132 4.267 4.403 4.541 4.680
COF 0.500 0.509 0.517 0.526 0.534 0.543
0.20 M 0.083 0.085 0.086 0.087 0.088 0.089
k 4.000 4.170 4.346 4.529 4.717 4.910
COF 0.500 0.511 0.522 0.532 0.543 0.554
0.25 M 0.083 0.085 0.086 0.087 0.089 0.090
k 4.000 4.204 4.420 4.648 4.887 5.138
COF 0.500 0.512 0.525 0.538 0.550 0.563
186 Appendix
Equivalent column stiffness (Kc)
All columns have same dimensions and geometry, hence the Kec value for all columns will be
the same.
1
𝐾𝑒𝑐=
1
Σ𝐾𝑐+
1
𝐾𝑡=
1
2003062 Ec+
1
2011115 Ec→ 𝐾𝑒𝑐 = 1003540 𝐸𝑐
• Moment-Distribution Coefficients for Slabs and Columns
The stiffness, carry over, and distribution factors for slabs and columns are shown in Figure
A.2b.
𝐷𝐹 𝐴3−𝐵3 =𝐾𝑠𝑏𝐴3−𝐵3
𝐾𝑠𝑏𝐴3−𝐵3+𝐾𝑒𝑐𝐴3=
2711062 𝐸𝑐
2711062 𝐸𝑐 +1003540 EC= 0.73
𝐷𝐹𝐾𝑒𝑐 𝐶𝑜𝑙𝑢𝑚𝑛 𝐴3=
𝐾𝑒𝑐𝐴3
𝐾𝑠𝑏𝐴3−𝐵3+𝐾𝑒𝑐𝐴3=
1003540 𝐸𝑐
2711062 𝐸𝑐 +1003540 EC= 0.27
𝐷𝐹 𝐵3−𝐴3 =𝐾𝑠𝑏𝐵3−𝐴3
𝐾𝑠𝑏𝐵3−𝐴3+𝐾𝑠𝑏𝐵3−𝐶3+𝐾𝑒𝑐𝐵3=
2711062 𝐸𝑐
𝐸𝑐(2711062 +2711062+1003540)= 0.422
𝐷𝐹𝐾𝑒𝑐 𝐶𝑜𝑙𝑢𝑚𝑛 𝐵3= 1 − 2(0.422) = 0.156
187
Table A.2 – Stiffness and carryover factors for columns (Wight and MacGregor 2011)
lc/lu
ta>tb 1.05 1.10 1.15 1.20 1.25 1.30 1.35 1.40 1.45
0.00 kAB 4.20 4.40 4.60 4.80 5.00 5.20 5.40 5.60 5.80
CAB 0.57 0.65 0.73 0.80 0.87 0.95 1.03 1.10 1.17
0.2 kAB 4.31 4.62 4.95 5.30 5.65 6.02 6.40 6.79 7.20
CAB 0.56 0.62 0.68 0.74 0.80 0.85 0.91 0.96 1.01
0.4 kAB 4.38 4.79 5.22 5.67 6.15 6.65 7.18 7.74 8.32
CAB 0.55 0.60 0.65 0.70 0.74 0.79 0.83 0.87 0.91
0.6 kAB 4.44 4.91 5.42 5.96 6.54 7.15 7.81 8.50 9.23
CAB 0.55 0.59 0.63 0.67 0.70 0.74 0.77 0.80 0.83
0.8 kAB 4.49 5.01 5.58 6.19 6.85 7.56 8.31 9.12 9.98
CAB 0.54 0.58 0.61 0.64 0.67 0.70 0.72 0.75 0.77
1.0 kAB 4.52 5.09 5.71 6.38 7.11 7.89 8.73 9.63 10.60
CAB 0.54 0.57 0.60 0.62 0.65 0.67 0.69 0.71 0.73
1.2 kAB 4.55 5.16 5.82 6.54 7.32 8.17 9.08 10.07 11.12
CAB 0.53 0.56 0.59 0.61 0.63 0.65 0.66 0.68 0.69
Figure A.2 – (a) Column A3 with attached torsional member; and (b) Stiffness, carry over, and
distribution factors
(a) (b)
188 Appendix
Figure A.3 – Moment and shear diagrams from equivalent frame analysis along line 3
• Moment Distribution Analysis
The moment distribution method is a convenient hand calculation method for analyzing partial
frames in the Equivalent Frame Method. The moment-distribution analysis is carried out in
Table A.3. The moment and shear force diagrams are plotted as shown in Figure A.3.
Table A.3– Moment distribution analysis in the X- frame
Joint A B C
Member Col. Slab Slab Col. slab Slab
C.O. F 0.505 0.505
D.F 0.27 0.73 0.422 0.156 0.422 0.422
FEM 0 113.93 -
113.93
0 113.93 -
113.93 BM -30.76 -83.17 0 0 0 0
COM 0. - 42 0 0 0
BM 0 17.72 6.56 17.72 0
COM 8.95 0 0 8.95
BM - 2.42 - 6.53 0
COM 0 - 3.29
BM 0 1.39 0.51 1.39 0
COM 0.70 0 0 0.70
BM - 0.19 - 0.51 0
Mfinal - 33.37 33.37 -
140.11
7.07 133.04 -
104.28
189
• Distribution of Frame Moments
Once the negative and positive moments have been determined for each equivalent frame, these
are distributed to column and middle strips in the same way as in the direct-design method. The
moment distribution for column and field strips in the longitudinal direction are listed in Table
A.4.
Table A.4 – Distribution of frame moments
• Moment-to-Shear Ratio at Column Centroid (M/V)
𝑀/𝑉 = 33.37/114.28 = 0.292 → 𝑡𝑎𝑘𝑒 𝑀/𝑉 = 0.3
1.2.3 Analysis of the Equivalent 2D frame in the Y-direction
• Slab-beam Stiffness and Fixed end moment
For span 5A−4A at end 5
- C1
𝑙1=
300
5000= 0.06,
C2
𝑙2=
300
2650= 0.11 → 𝑘 = 4.122, 𝐶𝑂𝐹 = 0.509 (Table A. 1)
- 𝐼𝑠 =𝑙2 𝑡𝑠
3
12=
2650×2003
12= 1767 × 106
- 𝐾𝐴3−𝐵3 =𝑘 𝐸𝑐𝐼𝑠
𝑙1=
4.122 ×1767×106×𝐸𝑐
5000= 1456715 𝐸𝑐
(𝑀𝐹.𝐸.𝑀)𝑓 = 0.0842 wf l2 l12 = 0.0842 × 10.85 × 2.65 × 52 = 60.52 kN.m
• Equivalent column stiffness (Kec)
For column 5A, the equivalent column stiffness was calculated as follows
Torsional member stiffness (Kt)
Joint A B C
Moment 33.37 82.79 140.11 133.04 50.87 104.28
Moment in column strip
Percentage (%) 100 60 70-90 70-90 55-65 70-90
Moment (kN.m) 33.37 49.67 98 -126 93.13-
119.74
27.98 -
33.07
73 –
93.87
Moments in field strip 2 half middle strips
Percentage (%) 0 40 30-10 30-10 45-35 30-10
Moment (kN.m) 0 33.12 42.11 -
14.11
39.91 -
13.30
22.89 –
17.80
31.31 -
10.43
190 Appendix
There is only one torsional member meet at column 5A. The value of Kt for all other columns
will be the same as column 5A because of similar column dimensions.
C = Σ (1 − 0.63 x
y) x3 y
3= (1 − 0.63
200
300) 2003 × 300
3= 464 × 106 mm4
𝑘𝑡 = Σ 9 𝐸𝑐 C
𝑙2 (1−𝑐2𝑙2)3 =
9 ×E𝑐 × 464 × 106
2650 (1− 300
2650)3 = 2259689 𝐸𝑐
Column stiffness (Kc)
𝑙𝑐
𝑙𝑢=
3200
3000= 1.07,
ta
tb= 1 → 𝑘𝐴𝐵 = 4.748, CAB = 0.55 (Table A. 2)
Σ𝐾𝑐 =𝑘 𝐸𝑐 𝐼𝐶
𝑙𝑐= 2 ×
4.748× 𝐸𝑐×(3004
12)
3200= 2003063 𝐸𝑐
Equivalent column stiffness (Kc)
1
𝐾𝑒𝑐=
1
Σ𝐾𝑐+
1
𝐾𝑡=
1
2003062 Ec+
1
2259689 Ec→ 𝐾𝑒𝑐 = 1061825 𝐸𝑐
• The Moment-Distribution Coefficients for Slabs and Columns
The Stiffness, carry over, and distribution factors for slabs and columns are shown in Figure
A.4.
𝐷𝐹 5𝐴−4𝐴 =𝐾𝑠𝑏𝐴3−𝐵3
𝐾𝑠𝑏𝐴3−𝐵3+𝐾𝑒𝑐𝐴3=
1456715 𝐸𝑐
1456715 𝐸𝑐 +1061825 EC= 0.58
𝐷𝐹𝐾𝑒𝑐 𝐶𝑜𝑙𝑢𝑚𝑛 5𝐴=
𝐾𝑒𝑐𝐴3
𝐾𝑠𝑏𝐴3−𝐵3+𝐾𝑒𝑐𝐴3=
1061825 𝐸𝑐
1456715 𝐸𝑐 +1061825 EC= 0.42
𝐷𝐹 4𝐴−5𝐴 =𝐾𝑠𝑏𝐵3−𝐴3
𝐾𝑠𝑏𝐵3−𝐴3+𝐾𝑠𝑏𝐵3−𝐶3+𝐾𝑒𝑐𝐵3=
1456715 𝐸𝑐
𝐸𝑐(1456715 +1456715+1061825)= 0.37
𝐷𝐹𝐾𝑒𝑐 𝐶𝑜𝑙𝑢𝑚𝑛 4𝐴= 1 − 2(0.37) = 0.26
191
Table A.5 – Moment distribution analysis in the Y- frame
• Moment Distribution Analysis
The moment-distribution analysis is carried out in Table A.5. The moment and shear force
diagrams are plotted as shown in Figure A.5.
Figure A.4 – Stiffness, carry over, and distribution factors
Joint 5 4 3
Member Col. Slab Slab Col. slab Slab
C.O. F 0.509 0.509
D.F 0.42 0.58 0.37 0.26 0.37 0.37
F.E.M. 0 60.52 - 60.52 0 60.52 - 60.52
B.M. -25.42 - 35.1 0 0 0 0
C.O.M 0 - 17.87 0 0 0
B.M 0 6.61 4.65 6.61 0
C.O.M 3.36 0 0 3.36
B.M - 1.41 - 1.95 0
C.O.M 0 - 0.99
B.M 0 0.37 0.25 0.37 0
C.O.M 0.19 0 0 0.19
B.M - 0.08 - 0.11 0
Mfinal - 26.91 26.91 -72.4 4.9 67.5 -56.97
192 Appendix
Figure A.5 – Moment and shear diagrams from equivalent frame analysis along line A
• Distribution of Frame Moments
The moment distribution for column and field strips in the longitudinal direction are listed in
Table A.6.
Table A.6 – Distribution of frame moments
1.3. Flexural Design of Test Specimen
1.3.1 Material Properties
• Concrete Properties
- fcˊ= 35 MPa 𝜆 = 1 𝜙𝑐= 1 Ec = 4500√𝑓𝑐′ = 26622 MPa
- 𝛼1 = 0.85 − 0.0015 𝑓𝑐′ = 0.798 𝛽1 = 0.97 − 0.0025 𝑓𝑐
′ = 0.883
Joint 5 4 3
Moment 26.91 40.20 72.4 67.5 27.62 56.97
Moment in column strip
Percentage (%) 100 60 70-90 70-90 55-65 70-90
Moment (kN.m) 26.91 24.12 50.68-
65.16
47.25
-60.75
15.19
-17.95
39.88-
51.27
Moments in field strip (half middle strip)
Percentage (%) 0 40 30-10 30-10 45-35 30-10
Moment (kN.m) 0 16.08 21.72
-7.24
20.25
-6.75
12.43
-9.67
17.1-
5.7
193
• Reinforcement Properties
- GFRP Bent Bars N0.20 (Af = 285 mm2; ƒƒrpu =1210 MPa; Efrp = 53 GPa; εƒrpu = 0.0228)
- GFRP Straight Bars No.20 (Af = 285 mm2; ƒƒrpu =1334 MPa; Efrp = 64.9 GPa; εƒrpu=
0.0206)
- GFRP Straight Bars No.15 (Af = 199 mm2; ƒƒrpu =1323 MPa; Efrp = 64.8 GPa; εƒrpu=
0.0204)
1.3.2 Test connections without shear reinforcement
Reinforcement perpendicular to the Free Edge
According to clause 13.10.3 in CSA A23.3-14, The width of the column strip equals 2500mm,
while the total factored negative moment transferred to the exterior columns is resisted by the
reinforcement placed in the band width (bb). The bottom reinforcement placed in the connection
refers to negative moment reinforcing bars. The reinforcement in the band width (bb) was
calculated as follows
Mr =33.37 kN.m (Table A.2)
bb = c + 3ts = 300 +3 (200) = 900 mm
𝑑𝑥 = ts – cover –db
2= 200 − 21 −
19
2= 169.5 mm
Mr = α1 β1 ∅𝑐 𝑓𝑐′ c b(d𝑥 –
β1 c
2)
33.37 × 106 = 0.798× 0.883× 1 × 35 × c × 900 (169.5 – 0.5 × 0.883 c)
9799 c2 – 3762217 c + 33.37 × 106 = 0 → c = 9.1 mm
𝜀𝑓𝑟𝑝 = 𝜀𝑐𝑢 (𝑑𝑥𝑐− 1) = 0.0035 (
169.5
9.1− 1) = 0.062
𝑓𝑓𝑟𝑝 = 𝐸𝑓𝑟𝑝 × 𝜀𝑓𝑟𝑝 = 53000 × 0.062 = 3286 MPa ≫ 𝑓𝑓𝑟𝑝𝑢 = 1210 MPa
→ Try 𝐴𝑓𝑟𝑝𝑚𝑖𝑛
The minimum area of reinforcement shall be used in each of the two orthogonal directions in
slabs according to clause 8.4.2.3 in CSA S806-12 given by
194 Appendix
𝐴𝑓𝑟𝑝𝑚𝑖𝑛 = 𝑀𝑎𝑥 [0.0025𝐴𝑔 ,400 𝐴𝑔 𝐸𝑓
] = 𝑀𝑎𝑥 [0.0025 (900 × 200),400 (200 × 900)
53000 ]
= 1358 𝑚𝑚2
From equilibrium, we can get 𝜀𝑓𝑟𝑝
C = T
𝛼1 ∅𝑐 𝛽1 𝑓𝑐′ 𝑐 𝑏 = ∅𝑓𝑟𝑝 𝐴𝑓𝑟𝑝 𝐸𝑓𝑟𝑝 𝜀𝑓𝑟𝑝
0.798 × 1 × 0.883 × 35 × c × 900 = 1 × 1358 × 53000 × 0.0035 (169.5
𝑐− 1)
22196 c2 + 251909 c − 42698576 = 0 → c = 38.6 mm
𝜀𝑓𝑟𝑝 = 𝜀𝑐𝑢 (𝑑𝑥𝑐− 1) = 0.0035 (
169.5
38.6− 1) = 0.0118
∴ 𝑓𝑓𝑟𝑝 = 𝐸𝑓𝑟𝑝 𝜀𝑓𝑟𝑝 = 53000 × 0.0118 = 625.4 MPa < 𝑓𝑓𝑟𝑝𝑢 = 1210 MPa ok…
𝑀𝑟 = 𝛼1 ∅𝑐 𝛽1 𝑓𝑐′ 𝑐 𝑏 (𝑑𝑥 –
𝛽1 𝑐
2)
𝑀𝑟 = 0.798 × 1 × 0.883 × 35 × 38.6 × 900 (169.5 – 0.883 × 38.6
2) = 130.62 kN.m
No. of bars = 1358 / 285 = 4.76 ∴ use 5 GFRP bent bars No.20 (𝐴𝑓𝑎𝑐𝑡 = 5×285 = 1425 mm2)
Spacing (s) = Width
No. of bars = 900
5= 180 mm
𝜌𝑓𝑟𝑝𝑥 =𝐴𝑓𝑟𝑝
𝑑𝑥 b=
5×285
169.5× 900= 0.0093 (Flexural reinforcement ratio ┴ free edge)
𝜌𝑓𝑟𝑝𝑏 = α1 β1 ∅𝑐∅𝑓𝑟𝑝
𝑓𝑐′
𝑓𝑓𝑟𝑝𝑢(
𝜀𝑐𝑢𝜀𝑐𝑢 + 𝜀𝑓𝑟𝑝𝑢
) = 0.798 × 0.883 ×1.00
1.00×
35
1210. (
0.0035
0.0035 + 0.023) = 0.0027
∴ 𝜌𝑓𝑟𝑝 > 𝜌𝑓𝑟𝑝𝑏 (Compression Failure)
The minimum flexure reinforcement can be used for in the rest parts of the column strip
Afrp𝑚𝑖𝑛
𝑚= max [0.0025𝐴𝑔 ,
400 𝐴𝑔
𝐸𝑓] = max [(0.0025 × (1000 × 200),
400 × (200 × 1000)
53000 ] = 1509
mm2
𝑚
195
No. of bars/ m = 1509/ 285 = 5.29/ m ∴ use 6 GFRP bent bars No.20 (𝐴𝑓𝑎𝑐𝑡 = 6 × 285 = 1710
mm2)
Smax = min of (3t𝑠 , 300 mm) = mim of (600 mm or 300 mm) → Smax = 300 mm
Spacing /𝑚 = 1000
6= 167 mm
Serviceability limit state
The modulus of elasticity of FRP bars, Ef, is lower than that of steel, Es, the higher strength
cannot be fully utilized in reinforced concrete structures. Hence, the design is mainly to control
deflection and crack width. In addition, the stress in the FRP reinforcement must be checked
against allowable service limit state stresses. The stress in the FRP reinforcement and crack
width were checked according to CSA S806-12 as follows
Service moment due to sustained service loads
The fixed end moment (MFEM) due to the sustained load
(MFEM)𝑠 = 0.084 𝑤𝑠 𝑙2 𝑙12 = 0.084 × 8.2 × 5 × 52 = 86.1 kN.m
The moment to be transferred at the edge column equals
𝑀𝑠 = 86.1 ×33.37
113.93= 25.22 kN.m
Check maximum stress under service load according
𝑓𝑓𝑟𝑝𝑠 =𝑀𝑠
𝐴𝑓𝑟𝑝 𝑗 𝑑𝑥 ≤ 0.25 𝑓𝑓𝑟𝑝𝑢
where
Ms = 25.22 kN.m
𝜌𝑓𝑟𝑝 = 0.0093 , 𝑛𝑓𝑟𝑝 = 𝐸𝑓𝐸𝑐 =
53000
26622 = 1.99
𝑘 = √(𝜌𝑓𝑟𝑝 𝑛𝑓𝑟𝑝 )2+ 2 𝜌𝑓𝑟𝑝𝑛𝑓𝑟𝑝 − 𝜌𝑓𝑟𝑝𝑛𝑓𝑟𝑝
𝑘 = √(0.0093 × 1.99 )2 + 2 × 0.0093 × 1.99 − 0.0093 × 1.99 = 0.175
196 Appendix
𝑗 = 1 −𝑘
3= 1 −
0.175
3 = 0.942
∴ 𝑓𝑓𝑟𝑝𝑠 =25.22 × 106
5 × 285 × 0.941 × 169.5= 110.96 MPa ≤ 0.25 𝑓𝑓𝑟𝑝𝑢 = 302.5 MPa
Check crack width parameter
The crack width parameter was checked based on the CSA S806-12. Clause 8.1.1.3 specifies
that, when the maximum strain in FRP tension reinforcement under full-service loads exceeds
0.0015, cross-sections of maximum positive and negative moment shall be so proportioned that
the quantity, z, given by
z = 𝑘𝑏 𝐸𝑠
𝐸𝐹 𝑓𝑓𝑟𝑝𝑠𝑒𝑟𝑣𝑖𝑐𝑒 (𝑑𝑐𝐴)
1
3 ≮ 45000 N
mm
where
dc = 21 + 0.5(19) = 30.5mm
A = 2 b dc
No. of bars =
2 × 900 × 30.5
5 = 10980 mm2
∴ z = 𝑘𝑏 𝐸𝑠𝐸𝐹 𝑓𝑓𝑟𝑝𝑠 (𝑑𝑐𝐴)
13
z = 1.2 ×200000
53000 × 110.96 × (30.5 × 10980)
13 = 34892
N
mm< 45000
N
mm ok….
∴ Place one GFRP bent bar No.20 @180 mm in the banded width and one GFRP bent bar
No.20 No.20 @ 167 mm for the rest of the connection.
Reinforcement Parallel to the Free Edge
The width of the column strip equals 1400 mm. while, clause 13.11.2.7 in CSA A23.3-14
specifies that one-third of the total factored negative moment at least transferred to the interior
columns is resisted by the reinforcement placed in the band width (bb). The reinforcement in the
band width (bb) was calculated as follows
197
Total factored -ve moment = 56.97 (Table A.4)
∴ Mr =1
3 × 56.97 = 18.99 kN.m
bb = c + 1.5 ts = 300 +1.5 (200) = 600 mm
𝑑𝑦 = t𝑠 − cover − 1.5 db = 200 − 21 − 1.5(19) = 150.5 mm
𝑀𝑟 = 𝛼1 𝛽1 ∅𝑐 𝑓𝑐′ 𝑐 𝑏(𝑑𝑦–
𝛽1 𝑐
2)
18.99 x 106 = 0.798 ×0.883 ×1× 35 x c × 600 (150.5 – 0.5 × 0.883 c)
6533 c2 – 2226996 c + 18.99 × 106 = 0 → c = 8.75 mm
𝜀𝑓𝑟𝑝 = 𝜀𝑐𝑢 (𝑑𝑦𝑐− 1) = 0.0035 (
150.5
8.75− 1) = 0.0567
𝑓𝑓 = 𝐸𝑓 × 𝜀𝑓𝑟𝑝 = 64900 × 0.0567 = 3680 MPa ≫ 𝑓𝑓𝑟𝑝𝑢 = 1334 MPa → Try 𝐴𝑓𝑟𝑝𝑚𝑖𝑛
𝐴𝑓𝑟𝑝𝑚𝑖𝑛 = max [0.0025𝐴𝑔 ,400
𝐸𝑓 𝐴𝑔 ] = max [ 0.0025 (600 × 200),
400 × (600 × 200)
64900]
= 740 𝑚𝑚2
From equilibrium, we can get 𝜀𝑓𝑟𝑝
C = T
𝛼1 𝛽1 ∅𝑐 𝑓𝑐′ 𝑐 𝑏 = ∅𝑓𝑟𝑝 𝐴𝑓𝑟𝑝 𝐸𝑓𝑟𝑝 𝜀𝑓𝑟𝑝
0.798 × 0.883 × 1 × 35 × c × 600 = 1 × 740 × 64900 × 0.0035 (150.5
𝑐− 1)
14797.31 c2 + 168091 c − 25297695.5 = 0 → c = 36.06 mm
𝜀𝑓𝑟𝑝 = 𝜀𝑐𝑢 (𝑑𝑦𝑐− 1) = 0.0035 (
150.5
36.06− 1) = 0.0111
∴ 𝑓𝑓𝑟𝑝 = 𝐸𝑓𝑟𝑝 𝜀𝑓𝑟𝑝 = 64900 × 0.0111 = 720.39 MPa < 𝑓𝑓𝑟𝑝𝑢 = 1334 MPa
𝑀𝑟 = 𝛼1 𝛽1 ∅𝑐 𝑓𝑐′ 𝑐 𝑏 (𝑑𝑦 –
𝛽1 𝑐
2)
198 Appendix
𝑀𝑟 = 0.798 × 0.883 × 1 × 35 × 36.06 × 600 (150.5 – 0.883 × 36.06
2) = 71.81 kN.m > 18.13 kN.m
No. of bars = 740 / 285 = 2.6 ∴ use 3 GFRP straight bars No.20 (𝐴𝑓𝑎𝑐𝑡 = 3 ×285 = 855 mm2)
Spacing (s) = Width
No. of bars = 600
3= 200 mm
𝜌𝑓𝑟𝑝 =𝐴𝑓𝑟𝑝
𝑑𝑦 b=
3×285
150.5× 600= 0.00947 (Flexural reinforcement ratio ∕ ∕ free edge)
𝜌𝑓𝑟𝑝𝑏 = 𝛼1 𝛽1 ∅𝑐∅𝑓𝑟𝑝
𝑓𝑐′
𝑓𝑓𝑟𝑝𝑢(
𝜀𝑐𝑢𝜀𝑐𝑢 + 𝜀𝑓𝑟𝑝𝑢
) = 0.798 × 0.883 ×1.00
1.00×
35
1334× (
0.0035
0.0035 + 0.021) = 0.00264
∴ 𝜌𝑓𝑟𝑝 > 𝜌𝑓𝑟𝑝𝑏 (Compression Failure)
The minimum flexure reinforcement can be used for in the rest parts of the column strip
Afrp𝑚𝑖𝑛
𝑚= max [0.0025𝐴𝑔 ,
400 𝐴𝑔
𝐸𝑓] = max [(0.0025 × (1000 × 200),
400 × (200 × 1000)
64900 ] = 1233
mm2
𝑚
No. of bars /m = 1233/ 285 = 4.3 /m ∴ use 5 GFRP straight bars No.20 (𝐴𝑓𝑎𝑐𝑡 = 5 × 285 =
1425 mm2)
Smax = 300 mm Spacing /𝑚 = 1000
5= 200 mm
Serviceability limit state
The stress in the FRP reinforcement must be checked against allowable service limit state
stresses. The stress in the FRP reinforcement and crack width was checked according to CSA
S806-12 as follows
Service moment due to sustained service loads
The fixed end moment (MFEM) due to the sustained load
(MFEM)𝑠 = 0.0842 𝑤𝑠 𝑙2 𝑙12 = 0.0842 × 8.2 × 2.65 × 52 = 45.74 kN.m
The service moment transferred to the interior column equals
Ms =1
3 [45.74 ×
56.97
60.52] = 14.35 kN
Check maximum stress under service load according
199
𝑓𝑓𝑟𝑝𝑠 =𝑀𝑠
𝐴𝑓𝑟𝑝 𝑗 𝑑𝑦 ≤ 0.25 𝑓𝑓𝑟𝑝𝑢
where
Ms = 14.35 kN.m
𝜌𝑓𝑟𝑝 = 0.00947 , 𝑛𝑓𝑟𝑝 = 𝐸𝑓𝐸𝑐 =
64900
26622 = 2.44
𝑘 = √(𝜌𝑓𝑟𝑝 𝑛𝑓𝑟𝑝 )2+ 2 𝜌𝑓𝑟𝑝𝑛𝑓𝑟𝑝 − 𝜌𝑓𝑟𝑝𝑛𝑓𝑟𝑝
𝑘 = √(0.00947 × 2.44 )2 + 2 × 0.00947 × 2.44 − 0.00947 × 2.44 = 0.193
𝑗 = 1 −𝑘
3= 1 −
0.193
3 = 0.936
∴ 𝑓𝑓𝑟𝑝𝑠 = 14.35 x 106
3 × 285 × 0.936 × 150.5= 119.14 MPa ≤ 0.25 𝑓𝑓𝑟𝑝𝑢 = 333.5 MPa
Check crack width parameter
z = 𝑘𝑏 𝐸𝑠
𝐸𝐹 𝑓𝑓𝑟𝑝𝑠 (𝑑𝑐𝐴)
1
3 ≮ 45000 N
mm
where
dc = 21 + 1.5(19) = 49.5 mm
A = 2 b dc
No. of bars =
2 × 600 × 49.5
3 = 19800 mm2
∴ z = 1.2 ×200000
64900 × 119.14 × (49.5 × 19800)
13 = 43764
N
mm< 45000
N
mm 𝑜𝑘 ….
Place one GFRP straight bar No.20 @200 mm in the banded width as well as in the rest of the
connection.
1.3.4 Top Reinforcement
The top flexural reinforcement bars passing through the column core were provided to satisfy
structural integrity requirement and connecting the slab to the column on all faces (CSA A23.3-
14). Similarly, two longitudinal bottom bars passing through column core. This slightly changed
the designed flexural reinforcement ratio and spacing in both orthogonal directions. The final
rienforcement details of test connections without shear reinforcement are shown in Figure 3
200 Appendix
(chapter 4). The flexural reinforcement ratios for test connections without shear reinforcement
within banded widths in both directions can be calculated as follows
Average Bottom flexural reinforcement ratios
𝜌𝑓𝑟𝑝𝑥 =𝐴𝑓𝑟𝑝𝑑𝑥 b
= 6 × 285
169.5 × 900= 0.0112 𝜌𝑓𝑟𝑝𝑦 =
𝐴𝑓𝑟𝑝𝑑𝑦 b
= 3 × 285
150.5 × 600
= 0.0095
𝜌𝑓𝑟𝑝𝑎𝑣𝑔 =0.0112 + 0.0095
2= 0.0104
Average Top flexural reinforcement ratios
𝜌𝑓𝑟𝑝𝑥 =𝐴𝑓𝑟𝑝𝑑𝑥 b
= 2 × 199
171.05 × 900= 0.0026 𝜌𝑓𝑟𝑝𝑦 =
𝐴𝑓𝑟𝑝𝑑𝑦 b
= 2 × 199
155.15 × 600= 0.0043
𝜌𝑓𝑟𝑝𝑎𝑣𝑔 =0.0026 + 0.0043
2= 0.0034
1.3.5 Test Connections with Shear Reinforcement
The test connections with shear reinforcement were designed to have high amounts of flexural
and transverse reinforcement such that punching-shear failure would be expected to occur prior
flexural failure. That would allow for measuring the shear-strength contribution of the GFRP
stirrups and for the shear-reinforcement system to achieve its maximum strength and
deformation capacity. The flexural reinforcement ratio of slabs with shear reinforcement
approximately increased by 50% than connections without shear reinforcement. The final
rienforcement details of test connections without shear reinforcement are shown in Figure 5.3
(chapter 4). In addition, the shear stirrups enclosed the top and bottom flexural reinforcement
and one longitudinal bar passed at each stirrup corner in test connections with shear
reinforcement. That was to provide enough anchorage for the vertical branch of the stirrup and
to be more effective. The flexural reinforcement ratios for test connections without shear
reinforcement within banded widths in both directions were calculated as follows
Average Bottom flexural reinforcement ratios
𝜌𝑓𝑟𝑝𝑥 =𝐴𝑓𝑟𝑝𝑑𝑥 b
= 8 × 285
169.5 × 900= 0.015 𝜌𝑓𝑟𝑝𝑦 =
𝐴𝑓𝑟𝑝𝑑𝑦 b
= 5 × 285
150.5 × 600= 0.016
201
𝜌𝑓𝑟𝑝𝑎𝑣𝑔 =0.015 + 0.016
2= 0.0155
Average Top flexural reinforcement ratios
𝜌𝑓𝑟𝑝𝑥 =𝐴𝑓𝑟𝑝𝑑𝑥 b
= 4 × 199
171.05 × 900= 0.0052 𝜌𝑓𝑟𝑝𝑦 =
𝐴𝑓𝑟𝑝𝑑𝑦 b
= 4 × 199
186.95 × 600= 0.0071
𝜌𝑓𝑟𝑝𝑎𝑣𝑔 =0.0052 + 0.0071
2= 0.0062
1.4 Punching Shear Capacity Predictions
The following part outlines the calculation procedure used to predict the punching shear capacity
predictions of specimens S-N-0.3 (steel specimen), G-N-0.3 (NSC specimen), G-H-0.3 (HSC
connection), G-CS-1.75d (connection with shear stirrups). The punching shear capacity of the
five additional connections were predicted using similar procedures in accordance with the type
of connection. The punching-shear capacities of the tested edge slab-column connections
without shear reinforcement were predicted using available equations in FRP codes and guides
namely ACI 440.1R-15, CSA S806-12, and JSCE-97. The predictions from these equations
were compared against the experimental results to evaluate their reliability in predicting
punching shear capacity of tested connections. The critical shear section for slabs without shear
reinforcement is located at d/2 from the column faces according to the previously mentioned
FRP codes and guides (refer to Figure A.6 a). on the other hand, CSA S806-12 and ACI 440.1R-
15 lack provisions for estimating the ultimate capacity of FRPRC two-way slabs with FRP shear
reinforcement. The punching-shear capacities of the tested edge slab-column connections with
shear reinforcement were predicted using the modified ACI 440.1R-15 and CSA S806-12
punching-shear equations as presented and discussed in chapter 4.
202 Appendix
Figure A.6 – Critical section properties (a) Connections without shear stirrups (b) Connection
G-CS-1.75d with shear stirrups
1.4.1. Connection S-N-0.3
1.4.1.1 Material and Critical Section Properties
• Concrete Properties
- fcˊ= 39.2 MPa 𝜆 = 1 𝜙𝑐= 1
• Reinforcement Properties
- Bent and straight Steel Bars 20M (As = 300 mm2; ƒy = 460 MPa; Es = 200 GPa; εy =
0.23)
- Straight Steel Bars 15M (As = 198 mm2; ƒy = 440 MPa; Es = 198 GPa; εy = 0.22)
- 𝐸𝑎𝑣𝑔 = 200 GPa (Average elastic modulus in both orthogonal directions)
• Average Bottom flexural reinforcement ratios
𝜌𝑓𝑟𝑝𝑥 =𝐴𝑓𝑟𝑝𝑑𝑥 b
= 6 × 300
170 × 900= 0.0118 𝜌𝑓𝑟𝑝𝑦 =
𝐴𝑓𝑟𝑝𝑑𝑦 b
= 3 × 300
150 × 600= 0.010
𝜌𝑓𝑟𝑝𝑎𝑣𝑔 =0.0118 + 0.01
2= 0.0109
• Average Top flexural reinforcement ratios
𝜌𝑓𝑟𝑝𝑥 =𝐴𝑓𝑟𝑝𝑑𝑥 b
= 2 × 200
172 × 900= 0.00258 𝜌𝑓𝑟𝑝𝑦 =
𝐴𝑓𝑟𝑝𝑑𝑦 b
= 2 × 200
156 × 600= 0.00427
(a) (b)
42
3
2.2
5d
40
4@
80
outer critical section
410
GFRP closed stirrups
l x=
10
20
ly = 660
80
80
46
0
30
0
80
300
380
Inner critical section
203
𝜌𝑓𝑟𝑝𝑎𝑣𝑔 =0.00258 + 0.00427
2= 0.0034
• Critical Section Properties
- 𝑑𝑎𝑣𝑔 =1
2 (𝑑𝑥 + 𝑑𝑦) =
1
2 (170 + 150) = 160 mm
- 𝑏𝑜 = 2 𝑏1 + 𝑏2 = 2 × (300 + 80) + (300 + 160) = 1220 𝑚𝑚
- 𝐶𝐴𝐵 =Σ 𝐴 𝑦
𝐴 =
2(380 × 160)(380 /2)
2(380 × 160)+(460 ×160)= 118.36 mm (Distance y is measured from AB)
- (Jc) is the effective polar moment of inertia for the critical shear section like the polar
moment of inertia. It is used to account for torsions and shears on the faces of the shear
perimeter.
𝐽𝑐 = 2(𝑑𝑎𝑣𝑔 𝑏1
3
3+𝑏1𝑑
3
12) − 𝑏𝑜 𝑑𝑎𝑣𝑔 𝑐𝐴𝐵
2
= 2 (160 x 3803
3+380 x 1603
12) − 1220 × 160 × 118.362
= 3377822076.5 mm4
- Fraction of moment transferred by shear (𝛾𝑣) = 1 −1
1+ (2
3)√
𝑏1𝑏2
= 1 −1
1+ (2
3)√
380
460
=
0.377
- Moment-to-shear ratio about the centroid of the shear perimeter
M0
V𝑡𝑒𝑠𝑡=
Mu
V𝑡𝑒𝑠𝑡− [
c12− (cAB −
d
2)] = 300 − (150 − (118.36 − 80) = 188.36 mm
𝛽𝑐 =long side of the column
short side of the column = 300
300= 1
1.4.1.2 Punching Shear Capacity
• Punching shear stress from testing
𝑣𝑡𝑒𝑠𝑡 = 𝑉𝑡𝑒𝑠𝑡 (1
𝑏𝑜;0.5𝑑 𝑑+𝛾𝑣 (𝑀𝑂/𝑉𝑢)
𝐽𝑐 𝐶𝐴𝐵)
= 359.40 × 103 (1
1220 × 160+0.377 × 188.36 3377822076.5
× 118.36) = 2.73 MPa
204 Appendix
• CSA A23.3-14
The punching shear strength (vc) was calculated based on the CSA A23.3-14. The punching
shear strength (vc) is the least value of the following equations
𝑣𝑐 = min of
{
(0.19 +
𝛼𝑠 𝑑
𝑏𝑜;0.5𝑑) λ ϕc (𝑓𝑐
΄)12
0.19 (1 +2
𝛽𝑐) 𝜆 𝜙𝑐 (𝑓𝑐
΄)12
0.38 𝜆 𝜙𝑐 (𝑓𝑐΄)12
where s is a factor equals 4 for interior columns, 3 for edge columns, 2 for corner columns;
bo,0.5d is the perimeter of the critical section for slabs at a distance d/2 from the column face
(mm); and βc the ratio of long side to short side of the concentrated load or reaction area.
𝑣𝑐 = (0.19 +𝛼𝑠 𝑑
𝑏𝑜;0.5𝑑) λ ϕc (𝑓𝑐
΄)1
2 = (0.19 +3 ×160
1220 ) × 1 × 1 × (39.2 )
1
2 = 3.65 MPa
𝑣𝑐 = 0.19 (1 +2
𝛽𝑐) 𝜆 𝜙𝑐 (𝑓𝑐
΄)1
2 = 0.19 (1 +2
1) × 1 × 1 × (39.2 )
1
2 = 3.57 MPa
𝑣𝑐 = 0.38 𝜆 𝜙𝑐 (𝑓𝑐΄)1
2 = 0.38 × 1 × 1 × (39.2 )1
2 = 2.38 MPa… (governs)
𝑉𝑝𝑟𝑒𝑑 =𝑣𝑐
(1
𝑏𝑜;0.5𝑑 𝑑+𝛾𝑣 (𝑀𝑂/𝑉𝑢)
𝐽𝑐 𝐶𝐴𝐵)
=2.38 × 10−3
(1
1220 × 160+0.377 × 188.36 3377822076.5
× 118.36)
= 312.69 kN
𝑉𝑡𝑒𝑠𝑡 / 𝑉𝑝𝑟𝑒𝑑 = 359.40/312.69 = 1.14
• ACI 318-14
The punching-shear strength provided by concrete (vc) for two-way slabs reinforced with steel
bars was calculated based based on the ACI 318-14. The punching shear strength (vc) is the least
value of the following equations
205
𝑣𝑐 = min of
{
0.083(2 +
𝛼𝑠 𝑑
𝑏𝑜;0.5𝑑) λ (𝑓𝑐
΄)12
0.083 (2 +4
𝛽𝑐) 𝜆 (𝑓𝑐
΄)12
0.32 𝜆 (𝑓𝑐΄)12
where s is a factor equals 40 for interior columns, 30 for edge columns, 20 for corner columns
𝑣𝑐 = 0.083 (2 +𝛼𝑠 𝑑
𝑏𝑜;0.5𝑑) λ (𝑓𝑐
΄)1
2 = 0.083 (2 +30×160
1220 ) × 1 × (39.2 )
1
2 = 3.08 MPa
𝑣𝑐 = 0.083 (2 +4
𝛽𝑐) 𝜆 (𝑓𝑐
΄)1
2 = 0.083 (2 +4
1) × 1 × (39.2 )
1
2 = 3.11 MPa
𝑣𝑐 = 0.32 𝜆 (𝑓𝑐΄)1
2 = 0.38 × 1 × (39.2 )1
2 = 2 MPa… (governs)
𝑉𝑝𝑟𝑒𝑑 =𝑣𝑐
(1
𝑏𝑜;0.5𝑑 𝑑+𝛾𝑣 (𝑀𝑂/𝑉𝑢)
𝐽𝑐 𝐶𝐴𝐵)
=2 × 10−3
(1
1220 × 160+0.377 × 188.36 3377822076.5
× 118.36)
= 262.77 kN
𝑉𝑡𝑒𝑠𝑡 / 𝑉𝑝𝑟𝑒𝑑 = 359.40/262.77 = 1.37
• JSCE-97
According to JSCE-97, The punching shear strength (vc) for steel and FRP-RC slabs was
calculated as follows
𝑣𝑐 = 𝛽𝑑 𝛽𝑝 𝛽𝑟 𝑓𝑝𝑐𝑑/𝛾𝑏
where 𝛽𝑑 = (1000/𝑑)0.25; 𝛽𝑝 = (100𝜌𝑓𝐸𝑓/𝐸𝑆)
1
3 ≤ 1.5 is a factor to consider the difference
in the elastic modulus between FRP and steel; 𝛽𝑟 = 1 + 1/(1 + 0.25 𝑢𝑜/𝑑); 𝑓𝑝𝑐𝑑 = 0.2√𝑓𝑐′ ≤
1.2 ; uo is the perimeter of reaction area of supporting column; Ef is the elastic modulus of FRP
tensile reinforcement; Es is the elastic modulus of steel reinforcement (assumed to be 200 GPa);
and ρf is average values for reinforcement ratio in both directions; γb is a partial factor of safety
equal to 1.3 or 1.5 for concrete strengths below and above 50 MPa, respectively, that was set to
1.0 to get an un factored prediction of capacity; fc' is cylinder concrete compressive strength
(MPa), and d is the effective slab depth (mm).
206 Appendix
𝛽𝑑 = (1000/160) 0.25 = 1.58 ≤ 1.5 → 𝛽𝑑 = 1.5
𝛽𝑝 = (100 × 0.0109 × (200/200))13 = 1.03 ≤ 1.5 𝑜𝑘..
𝛽𝑟 = 1 + 1/(1 + 0.25 (((2 × 300) + 300)/160) ) = 1.42
𝑓𝑝𝑐𝑑 = 0.2√39.2 = 1.25 ≤ 1.2 → 𝑓𝑝𝑐𝑑 = 1.2
𝑣𝑐 = 𝛽𝑑 𝛽𝑝 𝛽𝑟 𝑓𝑝𝑐𝑑/𝛾𝑏 = (1.5 × 1.03 × 1.42 × 1.2)/1 = 2.63 MPa
𝑉𝑝𝑟𝑒𝑑 =𝑣𝑐
(1
𝑏𝑜;0.5𝑑 𝑑+𝛾𝑣 (𝑀𝑂/𝑉𝑢)
𝐽𝑐 𝐶𝐴𝐵)
=1.73 × 10−3
(1
1220 × 160+0.377 × 188.36 3377822076.5
× 118.36)
= 345.54 kN
𝑉𝑡𝑒𝑠𝑡 / 𝑉𝑝𝑟𝑒𝑑 = 359.40/345.54 = 1.04
1.4.2. Connection G-N-0.3
1.4.2.1 Material and Critical Section Properties
• Concrete Properties
- fcˊ= 37.1 MPa 𝜆 = 1 𝜙𝑐= 1
• Critical Section Properties
All test connections had the same column dimensions and effective depth. Hence, the critical
section properties are the same. However, the M/V ratio at the centroid of the critical section
(Mo/V) is different because the test connections subjected to different M/V ratios of 0.3 and 0.6
m.
- 𝑑𝑎𝑣𝑔 =1
2 (𝑑𝑥 + 𝑑𝑦) =
1
2 (169.5 + 150.5) = 160 mm
- 𝑏𝑜 = 2 𝑏1 + 𝑏2 = 2 × 380 + 460 = 1220 𝑚𝑚
- 𝐶𝐴𝐵 =Σ 𝐴 𝑦
𝐴=
2(380 × 160)(380 /2)
2(380 × 160)+(460 ×160)= 118.36 mm
- 𝐽𝑐 = 2(𝑑𝑎𝑣𝑔 𝑏1
3
3+𝑏1𝑑
3
12) − 𝑏𝑜 𝑑𝑎𝑣𝑔 𝑐𝐴𝐵
2
207
= 2 (160 x 3803
3+380 x 1603
12) − 1220 × 160 × 118.362
= 3377822076.5 mm4
- Fraction of moment transferred by shear (𝛾𝑣) = 1 −1
1+ (2
3)√
𝑏1𝑏2
= 1 −1
1+ (2
3)√
380
460
=
0.377
- M0
𝑉𝑡𝑒𝑠𝑡=
𝑀𝑡𝑒𝑠𝑡
𝑉𝑡𝑒𝑠𝑡− [
c1
2− (cAB −
d
2)] = 300 − (150 − (118.36 − 80) = 188.36 mm
• Reinforcement Properties
- GFRP Bent Bars N0.20 (Af = 285 mm2; ƒƒrpu =1210 MPa; Efrp = 53 GPa; εƒrpu = 0.0228)
- GFRP Straight Bars No.20 (Af = 285 mm2; ƒƒrpu =1334 MPa; Efrp = 64.9 GPa; εƒrpu=
0.0206)
- 𝐸𝑎𝑣𝑔 =𝐸𝑓𝑟𝑝 ×𝑏2 +2×𝐸𝑓𝑟𝑝 × 𝑏1
𝑏𝑜=
53 ×460 +2×64.9 ×380
1220= 60.410 GPa
- 𝜌𝑓𝑟𝑝𝑎𝑣𝑔 = 0.0104
1.4.2.2 Punching Shear Capacity
• Punching shear stress from testing
𝑣𝑡𝑒𝑠𝑡 = 𝑉𝑡𝑒𝑠𝑡 (1
𝑏𝑜;0.5𝑑 𝑑+𝛾𝑣 (𝑀𝑂/𝑉𝑢)
𝐽𝑐 𝐶𝐴𝐵)
= 259.86 × 103 (1
1220 × 160+0.377 × 188.36 3377822076.5
× 118.36) = 1.98 MPa
• CSA S806-12
The punching shear strength (vc) was calculated based on the CSA S806-12. The punching shear
strength (vc) is the least value of the following equations, which are essentially the CSA A23.3-
14 equations with modifications to account for FRP bars instead of steel.
208 Appendix
𝑣𝑐 = min of
{
0.147 (0.19 +
𝛼𝑠 𝑑
𝑏𝑜;0.5𝑑)λ ϕc (𝐸𝑓 𝜌𝑓 𝑓𝑐
΄)13
0.028 (1 +2
𝛽𝑐) 𝜆 𝜙𝑐 (𝐸𝑓 𝜌𝑓𝑓𝑐
΄)13
0.056 𝜆 𝜙𝑐 (𝐸𝑓 𝜌𝑓 𝑓𝑐΄)13
where ρf is the FRP reinforcement ratio; s is a factor equals 4 for interior columns, 3 for edge
columns, 2 for corner columns; bo,0.5d is the perimeter of the critical section for slabs at a distance
d/2 from the column face (mm); and βc the ratio of long side to short side of the concentrated load
or reaction area.
𝑣𝑐 = 0.147 (0.19 +3 ×160
1220 ) × 1 × 1 × (60410 × 0.0104 × 37.1 )
1
3 = 2.45Mpa
𝑣𝑐 = 0.028 (1 +2
1) × 1 × 1 × (60410 × 0.0104 × 37.1 )
1
3 = 2.4 MPa
𝑣𝑐 = 0.056 × 1 × 1 × (60410 × 0.0104 × 37.1 )1
3 = 1.6 MPa… (governs)
𝑉𝑝𝑟𝑒𝑑 =𝑣𝑐
(1
𝑏𝑜;0.5𝑑 𝑑+𝛾𝑣 (𝑀𝑂/𝑉𝑢)
𝐽𝑐 𝐶𝐴𝐵)
=1.6 × 10−3
(1
1220 × 160+0.377 × 188.36 3377822076.5
× 118.36)
= 210.11 kN
𝑉𝑡𝑒𝑠𝑡 / 𝑉𝑝𝑟𝑒𝑑 = 259.86/210.11 = 1.24
• ACI 440.1R-15
The punching-shear stress provided by concrete (vc) for two-way slabs reinforced with FRP bars
or grids is simply the ACI 318-14. The shear strength (vc) equation for steel modified by the
factor ([5/2] k) accounts for the axial stiffness of the FRP reinforcement through the neutral-
axis-depth term (kd). The punching shear strength (vc) was calculated based on the ACI 440.1R-
15 as follows
𝑣𝑐 = 4
5 𝑘 √𝑓𝑐
′
where: 𝑘 = √2𝜌𝑓 𝑛𝑓 + (𝜌𝑓 𝑛𝑓)2 − 𝜌𝑓𝑛𝑓 ; nf is the modular ratio (𝐸𝑓/𝐸𝐶) ; 𝐸𝑓 = 4700√𝑓𝑐
′
𝑛𝑓 = 60410/4700 √37.1 = 2.11
𝑘 = √2 × 0.0104 × 2.11 + (0.0104 × 2.11)2 − 0.0104 × 2.11 = 0.189
𝑣𝑐 = 4
5 × 0.189 × √37.1 = 0.92 MPa
209
𝑉𝑝𝑟𝑒𝑑 =𝑣𝑐
(1
𝑏𝑜;0.5𝑑 𝑑+𝛾𝑣 (𝑀𝑂/𝑉𝑢)
𝐽𝑐 𝐶𝐴𝐵)
=0.92 × 10−3
(1
1220 × 160+0.377 × 188.36 3377822076.5
× 118.36)
= 120.78 kN
𝑉𝑡𝑒𝑠𝑡 / 𝑉𝑝𝑟𝑒𝑑 = 259.86/120.78 = 2.15
• JSCE -97
𝑣𝑐 = 𝛽𝑑 𝛽𝑝 𝛽𝑟 𝑓𝑝𝑐𝑑/𝛾𝑏
𝛽𝑑 = (1000/160) 0.25 = 1.58 ≤ 1.5 → 𝛽𝑑 = 1.5
𝛽𝑝 = (100 × 0.0104 × (60.410/200))13 = 0.68 ≤ 1.5 𝑜𝑘..
𝛽𝑟 = 1 +1
1 + 0.25 ((2 × 300) + 300
160 )= 1.42
𝑓𝑝𝑐𝑑 = 0.2√37.1 = 1.22 ≤ 1.2 → 𝑓𝑝𝑐𝑑 = 1.2
𝑣𝑐 = (1.5 × 0.68 × 1.42 × 1.2)/1 = 1.73 MPa
𝑉𝑝𝑟𝑒𝑑 =𝑣𝑐
(1
𝑏𝑜;0.5𝑑 𝑑+𝛾𝑣 (𝑀𝑂/𝑉𝑢)
𝐽𝑐 𝐶𝐴𝐵)
=1.73 × 10−3
(1
1220 × 160+0.377 × 188.36 3377822076.5
× 118.36)
= 227.52 kN
𝑉𝑡𝑒𝑠𝑡 / 𝑉𝑝𝑟𝑒𝑑 = 259.86/227.52 = 1.14
1.4.3. Connection G-H-0.3
1.4.3.1 Material and Critical Section Properties
• Concrete Properties
- fcˊ= 85.8 MPa 𝜆 = 1 𝜙𝑐= 1
• Critical Section Properties
𝑑𝑎𝑣𝑔 = 160 mm
- 𝑏𝑜 = 2 𝑏1 + 𝑏2 = 1220 𝑚𝑚
- 𝐶𝐴𝐵 = Σ 𝐴 𝑦
𝐴= 118.36 mm
- 𝐽𝑐 = 2(𝑑𝑎𝑣𝑔 𝑏1
3
3+
𝑏1𝑑3
12) − 𝑏𝑜 𝑑𝑎𝑣𝑔 𝑐𝐴𝐵
2 = 3377822076.5 mm4
210 Appendix
- Fraction of moment transferred by shear (𝛾𝑣) = 1 −1
1+ (2
3)√
𝑏1𝑏2
= 0.377
- M0
𝑉𝑡𝑒𝑠𝑡=
𝑀𝑡𝑒𝑠𝑡
𝑉𝑡𝑒𝑠𝑡− [
c1
2− (cAB −
d
2)] = 300 − (150 − (118.36 − 80) = 188.36 mm
• Reinforcement Properties
- GFRP Bent Bars N0.20 (Af = 285 mm2; ƒƒrpu =1210 MPa; Efrp = 53 GPa; εƒrpu = 0.0228)
- GFRP Straight Bars No.20 (Af = 285 mm2; ƒƒrpu =1334 MPa; Efrp = 64.9 GPa; εƒrpu=
0.0206)
- 𝐸𝑎𝑣𝑔 = 60.410 GPa 𝜌𝑓𝑟𝑝𝑎𝑣𝑔 = 0.0104
1.4.3.2 Punching Shear Capacity
• Punching shear stress from testing
𝑣𝑡𝑒𝑠𝑡 = 𝑉𝑡𝑒𝑠𝑡 (1
𝑏𝑜;0.5𝑑 𝑑+𝛾𝑣 (𝑀𝑂/𝑉𝑢)
𝐽𝑐 𝐶𝐴𝐵)
= 305.5 × 103 (1
1220 × 160+0.377 × 188.36 3377822076.5
× 118.36) = 2.33 MPa
• CSA S806-12
𝑣𝑐 = min of
{
0.147 (0.19 +
𝛼𝑠 𝑑
𝑏𝑜;0.5𝑑)λ ϕc (𝐸𝑓 𝜌𝑓 𝑓𝑐
΄)13
0.028 (1 +2
𝛽𝑐) 𝜆 𝜙𝑐 (𝐸𝑓 𝜌𝑓𝑓𝑐
΄)13
0.056 𝜆 𝜙𝑐 (𝐸𝑓 𝜌𝑓 𝑓𝑐΄)13
𝑣𝑐 = 0.147 (0.19 +3 ×160
1220 ) × 1 × 1 × (60410 × 0.0104 × 60 )
1
3 = 2.88 MPa
𝑣𝑐 = 0.028 (1 +2
1) × 1 × 1 × (60410 × 0.0104 × 60 )
1
3 = 2.82 MPa
𝑣𝑐 = 0.056 × 1 × 1 × (60410 × 0.0104 × 60 )1
3 = 1.88 MPa… (governs)
𝑉𝑝𝑟𝑒𝑑 =𝑣𝑐
(1
𝑏𝑜;0.5𝑑 𝑑+𝛾𝑣 (𝑀𝑂/𝑉𝑢)
𝐽𝑐 𝐶𝐴𝐵)
=1.88 × 10−3
(1
1220 × 160+0.377 × 188.36 3377822076.5
× 118.36)
= 246.63 kN
𝑉𝑡𝑒𝑠𝑡 / 𝑉𝑝𝑟𝑒𝑑 = 305.5/246.63 = 1.24
211
• ACI 440.1R-15
𝑣𝑐 = 4
5 𝑘 √𝑓𝑐
′
where: 𝑘 = √2𝜌𝑓 𝑛𝑓 + (𝜌𝑓 𝑛𝑓)2 − 𝜌𝑓𝑛𝑓 ; nf is the modular ratio (𝐸𝑓/𝐸𝐶) ; 𝐸𝑓 = 4700√𝑓𝑐
′
𝑛𝑓 = 60410/4700 √85.8 = 1.39
𝑘 = √2 × 0.0104 × 1.39 + (0.0104 × 1.39)2 − 0.0104 × 1.39 = 0.156
𝑣𝑐 = 4
5 × 0.156 × √85.8 = 1.16 MPa
𝑉𝑝𝑟𝑒𝑑 =𝑣𝑐
(1
𝑏𝑜;0.5𝑑 𝑑+𝛾𝑣 (𝑀𝑂/𝑉𝑢)
𝐽𝑐 𝐶𝐴𝐵)
=1.16 × 10−3
(1
1220 × 160+0.377 × 188.36 3377822076.5
× 118.36)
= 151.91 kN
𝑉𝑡𝑒𝑠𝑡 / 𝑉𝑝𝑟𝑒𝑑 = 305.5/151.91 = 2.01
• JSCE-97
𝑣𝑐 = 𝛽𝑑 𝛽𝑝 𝛽𝑟 𝑓𝑝𝑐𝑑/𝛾𝑏
𝛽𝑑 = (1000/𝑑)0.25 = (1000/160) 0.25 = 1.58 ≤ 1.5 → 𝛽𝑑 = 1.5
𝛽𝑝 = (100𝜌𝑓𝐸𝑓/𝐸𝑆)13 = (100 × 0.0104 × (60.410/200))
13 = 0.68 ≤ 1.5 𝑜𝑘..
𝛽𝑟 = 1 + 1/(1 + 0.25 𝑢𝑜/𝑑) = 1 +1
1 + 0.25 ((2 × 300) + 300
160 )= 1.42
𝑓𝑝𝑐𝑑 = 0.2√𝑓𝑐′ = 0.2√85.8 = 1.85 ≤ 1.2 → 𝑓𝑝𝑐𝑑 = 1.2
𝑣𝑐 = 𝛽𝑑 𝛽𝑝 𝛽𝑟 𝑓𝑝𝑐𝑑/𝛾𝑏 = (1.5 × 0.68 × 1.42 × 1.2)/1 = 1.73 MPa
𝑉𝑝𝑟𝑒𝑑 =𝑣𝑐
(1
𝑏𝑜;0.5𝑑 𝑑+𝛾𝑣 (𝑀𝑂/𝑉𝑢)
𝐽𝑐 𝐶𝐴𝐵)
=1.73 × 10−3
(1
1220 × 160+0.377 × 188.36 3377822076.5
× 118.36)
= 227.51 kN
𝑉𝑡𝑒𝑠𝑡 / 𝑉𝑝𝑟𝑒𝑑 = 305.5/227.51 = 1.34
212 Appendix
1.4.4. Connection G-CS-1.75d
1.4.4.1 Material and Critical Section Properties
• Concrete Properties
- fcˊ= 47.6 MPa 𝜆 = 1 𝜙𝑐= 1
Critical Section Properties
The critical shear section should be checked located at d/2 from the column faces and at d/2
from the outermost shear reinforcement (2.25d from the column faces) inside and outside the
shear-reinforced zone, respectively.
Critical Section Properties at d/2 from the column faces
- 𝑑𝑎𝑣𝑔 = 160 mm
- 𝑏𝑜 = 2 𝑏1 + 𝑏2 = 1220 𝑚𝑚
- 𝐶𝐴𝐵 = Σ 𝐴 𝑦
𝐴= 118.36 mm
- 𝐽𝑐 = 2(𝑑𝑎𝑣𝑔 𝑏1
3
3+𝑏1𝑑
3
12) − 𝑏𝑜 𝑑𝑎𝑣𝑔 𝑐𝐴𝐵
2 = 3377822076.5 mm4
- Fraction of moment transferred by shear (𝛾𝑣) = 1 −1
1+ (2
3)√
𝑏1𝑏2
= 0.377
- M0
𝑉𝑡𝑒𝑠𝑡=
𝑀𝑡𝑒𝑠𝑡
𝑉𝑡𝑒𝑠𝑡− [
c1
2− (cAB −
d
2)] = 310 − (150 − (118.36 − 80) = 198.36 mm
Critical Section Properties at 2.25d from the column faces
The properties of the outer critical shear perimeter cannot be calculated using the expressions
for the critical shear perimeter shown in Figure A.6. The properties of the outer critical shear
perimeter were calculated based on the expressions developed El-gabry and Ghali (1996) for
such sections as follows
- Perimeter of the outer critical section
Lengths of shear perimeter sides 𝑙1 = 410 mm , 𝑙2 = 387 mm, 𝑙3 = 423 mm
𝑏𝑜 = 2(𝑙1 + 𝑙2) + 𝑙3 = 2(410 + 387) + 423 = 2017 mm
- Centroid of the outer critical section (x)
213
𝑥 =2 [𝑙1 (𝑙𝑥 −
𝑙12) + 𝑙2
(𝑙𝑥 − 𝑙1)2
]
𝑏𝑜
=2 [410 (660 −
4102) + 387
(660 − 410)2
]
2015= 232.94mm
- Polar moment of inertia of the outer critical section
𝐽𝑐 = 𝑑 [𝑙3 𝑥2 +
𝑙13
6+ 2𝑙1(𝑙𝑥 − 0.5𝑙1 − 𝑥)
2 + 𝑙2(𝑙𝑥−𝑙1)
2
6+ 2𝑙2 (𝑥 −
𝑙𝑥−𝑙1
2)2]
𝐽𝑐 = 160 [423 × 232.942 +
4123
6+ 2 × 410 (660 − 0.5 × 410 − 232.94)2 +
387(660−410)2
6 + 2 × 387 × (232.94 −
660−410
2)2] = 14032318151mm4
- Fraction of moment transferred by shear at the centroid of the outer critical section
(𝛾𝑣) = 1 −1
1+ (2
3)√
𝑙𝑥𝑙𝑦−0.2
= 1 −1
1+ (2
3)√
660
1020−0.2
= 0.31
- M0
𝑉𝑡𝑒𝑠𝑡=
𝑀𝑡𝑒𝑠𝑡
𝑉𝑡𝑒𝑠𝑡− [ 𝑙𝑥 − 𝑥 −
c1
2] = 310 − (660 − 232.94 − 150) = 32.94 mm
• Reinforcement Properties
- GFRP Bent Bars N0.20 (Af = 285 mm2; ƒƒrpu =1210 MPa; Efrp = 53 GPa; εƒrpu = 0.0228)
- GFRP Straight Bars No.20 (Af = 285 mm2; ƒƒrpu =1334 MPa; Efrp = 64.9 GPa; εƒrpu=
0.0206)
- 𝐸𝑎𝑣𝑔 = 60.410 GPa 𝜌𝑓𝑟𝑝𝑎𝑣𝑔 = 0.0155
- GFRP Closed stirrups No.10 (Af = 71 mm2; ƒƒrpu = 967 MPa; Efrp = 45.7 GPa; εƒrpu=
0.0212)
1.4.4.2. Punching Shear Capacity
• Punching shear stress from testing
𝑣𝑡𝑒𝑠𝑡,𝑖𝑛 = 𝑉𝑡𝑒𝑠𝑡 (1
𝑏𝑜;0.5𝑑 𝑑+𝛾𝑣 (𝑀𝑜/𝑉𝑢)
𝐽𝑐 𝐶𝐴𝐵)
= 370 × 103 (1
1220 × 160+0.377 × 198.36 3377822076.5
× 118.36) = 2.87 MPa
214 Appendix
𝑣𝑡𝑒𝑠𝑡,𝑜𝑢𝑡 = 𝑉𝑡𝑒𝑠𝑡 (1
𝑏𝑜;2.25𝑑 𝑑+𝛾𝑣 (𝑀𝑜/𝑉𝑢)
𝐽𝑐 𝑥)
= 370 × 103 (1
2015 × 160+0.31 × 32.94 14032318151
× 232.94) = 1.21 MPa
• Shear capacity using Modified code provisions
Within the shear reinforced zone, the factored shear strength, computed as (vc + vs), where vc
and vs are the summations of concrete and shear-reinforcement contributions to the shear
strength inside the punching zone. To date, CSA S806-12 and ACI 440.1R-15 lack provisions
for estimating the ultimate capacity of FRPRC two-way slabs with FRP shear reinforcement.
Hence, the punching shear strength for connections with shear reinforcement was calculated
based on the proposed design provisions which is extension to CSA S806-12 and ACI 440.1R-
15 to account for FRP stirrups as shear reinforcement.
- Proposed design provisions for CSA S806-12
𝑣𝑐 𝑖𝑛𝑠𝑖𝑑𝑒 = 𝑣𝑐 𝑜𝑢𝑡𝑠𝑖𝑑𝑒 = 0.028𝜆𝜙𝑐(𝐸𝑓𝜌𝑓𝑓𝑐′)1
3
𝑣𝑓𝑣 =𝜙𝑓𝐴𝑓𝑣(0.005𝐸𝑓𝑣)
𝑏0𝑆𝑓𝑣
𝑣𝑖𝑛,𝑝𝑟𝑒𝑑. = 𝑣𝑐 𝑖𝑛𝑠𝑖𝑑𝑒 + 𝑣𝑓𝑣 = 0.99 + 2 = 2.99 MPa , 𝑣𝑜𝑢𝑡,𝑝𝑟𝑒𝑑. = 𝑣𝑐 𝑜𝑢𝑡𝑠𝑖𝑑𝑒 = 0.99 MPa
𝑉𝑖𝑛,𝑝𝑟𝑒𝑑. =𝑣𝑖𝑛,𝑝𝑟𝑒𝑑.
(1
𝑏𝑜;0.5𝑑 𝑑+𝛾𝑣 (𝑀𝑜/𝑉𝑢)
𝐽𝑐 𝐶𝐴𝐵)
=2.99 × 10−3
(1
1220 × 160+0.377 × 198.36 3377822076.5
× 118.36)= 386 kN
𝑉𝑜𝑢𝑡,𝑝𝑟𝑒𝑑. =𝑣𝑜𝑢𝑡,𝑝𝑟𝑒𝑑.
(1
𝑏𝑜;2.25𝑑 𝑑+𝛾𝑣 (𝑀𝑜/𝑉𝑢)
𝐽𝑐 𝐶𝐴𝐵)
=0.99 × 10−3
(1
2015 × 160+0.31 × 33.3 14032318151
× 233.29)
= 303 kN
𝑉𝑡𝑒𝑠𝑡 / 𝑉𝑝𝑟𝑒𝑑 = 370/303 = 1.22
The proposed provision for CSA S806-12 gave good predictions and expectations for failure
localization within or outside the shear-reinforced zone with respect to the experimental test
results for slabs with FRP stirrups as shear reinforcement.
- Proposed design provisions for ACI440.1R-15
𝑣𝑐 𝑖𝑛𝑠𝑖𝑑𝑒 = 𝑣𝑐𝑜𝑢𝑡𝑠𝑖𝑑𝑒 =2
5𝑘√𝑓𝑐
′
215
𝑣𝑓𝑣 =𝜙𝑓𝐴𝑓𝑣(0.004𝐸𝑓𝑣)
𝑏0𝑆𝑓𝑣
𝑛𝑓 = 60410/4700 √47.6 = 1.86
𝑘 = √2 × 0.0155 × 1.86 + (0.0155 × 1.86)2 − 0.0155 × 1.86 = 0.21
𝑣𝑐 𝑖𝑛𝑠𝑖𝑑𝑒 = 𝑣𝑐𝑜𝑢𝑡𝑠𝑖𝑑𝑒 = 2
5 × 0.21 × √47.6 = 0.59 MPa
𝑣𝑓𝑣 =1×(12×71)×(0.004×45700)
1220×80= 1.6 MPa
𝑣𝑖𝑛,𝑝𝑟𝑒𝑑. = 𝑣𝑐 𝑖𝑛𝑠𝑖𝑑𝑒 + 𝑣𝑓𝑣 = 0.59 + 1.6 = 2.19 MPa , 𝑣𝑜𝑢𝑡,𝑝𝑟𝑒𝑑. = 𝑣𝑐 𝑜𝑢𝑡𝑠𝑖𝑑𝑒 = 0.588 MPa
𝑉𝑖𝑛,𝑝𝑟𝑒𝑑. =𝑣𝑖𝑛,𝑝𝑟𝑒𝑑.
(1
𝑏𝑜;0.5𝑑 𝑑+𝛾𝑣 (𝑀𝑜/𝑉𝑢)
𝐽𝑐 𝐶𝐴𝐵)
=2.19 × 10−3
(1
1220 × 160+0.377 × 198.36 3377822076.5
× 118.36)= 282 kN
𝑉𝑜𝑢𝑡,𝑝𝑟𝑒𝑑. =𝑣𝑜𝑢𝑡,𝑝𝑟𝑒𝑑.
(1
𝑏𝑜;2.25𝑑 𝑑+𝛾𝑣 (𝑀𝑜/𝑉𝑢)
𝐽𝑐 𝐶𝐴𝐵)
=0.59 × 10−3
(1
2015 × 160+0.31 × 33.3 14032318151
× 233.29)
= 180 kN
𝑉𝑡𝑒𝑠𝑡 / 𝑉𝑝𝑟𝑒𝑑 = 370/180 = 2.06